# Electronic Supplementary Material (ESI) for Dalton Transactions.
# This journal is © The Royal Society of Chemistry 2021

####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_lzg
_database_code_depnum_ccdc_archive 'CCDC 2013548'
loop_
_audit_author_name
_audit_author_address
'Bassem S Bassil'
;University of Balamand
Lebanon
;
_audit_update_record             
;
2021-01-20 deposited with the CCDC.	2021-01-26 downloaded from the CCDC.
;

_audit_creation_method           SHELXL-2014/6
_chemical_name_systematic        ?
_chemical_name_common            ?
_chemical_melting_point          ?
_chemical_formula_moiety         ?
_chemical_formula_sum            'Co4 H28 Cs10 Na3 O99 Si2 W20'
_chemical_formula_weight         6979.19

loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Si Si 0.0817 0.0704 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
W W -0.8490 6.8722 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Co Co 0.3494 0.9721 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Cs Cs -0.3680 2.1192 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Na Na 0.0362 0.0249 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_space_group_crystal_system      monoclinic
_space_group_IT_number           14
_space_group_name_H-M_alt        'P 21/n'
_space_group_name_Hall           '-P 2yn'

_shelx_space_group_comment       
; 
The symmetry employed for this shelxl refinement is uniquely defined 
by the following loop, which should always be used as a source of 
symmetry information in preference to the above space-group names. 
They are only intended as comments. 
;

loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x+1/2, y+1/2, -z+1/2'
'-x, -y, -z'
'x-1/2, -y-1/2, z-1/2'

_cell_length_a                   13.1052(7)
_cell_length_b                   15.7954(8)
_cell_length_c                   23.8328(14)
_cell_angle_alpha                90
_cell_angle_beta                 100.616(3)
_cell_angle_gamma                90
_cell_volume                     4849.0(5)
_cell_formula_units_Z            2
_cell_measurement_temperature    100(2)
_cell_measurement_reflns_used    9997
_cell_measurement_theta_min      3.23
_cell_measurement_theta_max      28.21

_exptl_crystal_description       block
_exptl_crystal_colour            purple
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    ?
_exptl_crystal_density_diffrn    4.780
_exptl_crystal_F_000             6038
_exptl_transmission_factor_min   0.0362
_exptl_transmission_factor_max   0.0962
_exptl_crystal_size_max          0.100
_exptl_crystal_size_mid          0.100
_exptl_crystal_size_min          0.100
_exptl_absorpt_coefficient_mu    28.131
_shelx_estimated_absorpt_T_min   0.0362
_shelx_estimated_absorpt_T_max   0.0962
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_correction_T_min  0.0362
_exptl_absorpt_correction_T_max  0.0962
_exptl_absorpt_process_details   SADABS
_exptl_absorpt_special_details   ?
_diffrn_ambient_temperature      100(2)
_diffrn_radiation_wavelength     0.71073
_diffrn_radiation_type           MoK\a
_diffrn_source                   ?
_diffrn_measurement_device_type  'Bruker APEX-II CCD'
_diffrn_measurement_method       'φ and ω scans'
_diffrn_detector_area_resol_mean ?
_diffrn_reflns_number            100865
_diffrn_reflns_av_unetI/netI     0.0470
_diffrn_reflns_av_R_equivalents  0.0854
_diffrn_reflns_limit_h_min       -16
_diffrn_reflns_limit_h_max       16
_diffrn_reflns_limit_k_min       -20
_diffrn_reflns_limit_k_max       15
_diffrn_reflns_limit_l_min       -30
_diffrn_reflns_limit_l_max       30
_diffrn_reflns_theta_min         3.416
_diffrn_reflns_theta_max         27.103
_diffrn_reflns_theta_full        25.242
_diffrn_measured_fraction_theta_max 0.998
_diffrn_measured_fraction_theta_full 0.997
_diffrn_reflns_Laue_measured_fraction_max 0.998
_diffrn_reflns_Laue_measured_fraction_full 0.997
_diffrn_reflns_point_group_measured_fraction_max 0.998
_diffrn_reflns_point_group_measured_fraction_full 0.997
_reflns_number_total             10686
_reflns_number_gt                8491
_reflns_threshold_expression     'I > 2σ(I)'
_reflns_Friedel_coverage         0.000
_reflns_Friedel_fraction_max     .
_reflns_Friedel_fraction_full    .

_reflns_special_details          
; 
 Reflections were merged by SHELXL according to the crystal 
 class for the calculation of statistics and refinement. 
  
 _reflns_Friedel_fraction is defined as the number of unique 
 Friedel pairs measured divided by the number that would be 
 possible theoretically, ignoring centric projections and 
 systematic absences. 
;

_computing_data_collection       'Bruker APEX2'
_computing_cell_refinement       'Bruker SAINT'
_computing_data_reduction        'Bruker SAINT'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 2008)'
_computing_structure_refinement  'SHELXL-2014/6 (Sheldrick, 2014)'
_computing_molecular_graphics    'Bruker SHELXTL'
_computing_publication_material  'Bruker SHELXTL'
_refine_special_details          ?
_refine_ls_structure_factor_coef Fsqd
_refine_ls_matrix_type           full
_refine_ls_weighting_scheme      calc
_refine_ls_weighting_details     
'w=1/[σ²(Fo²)+(0.0686P)²+110.0000P] where P=(Fo²+2Fc²)/3'
_atom_sites_solution_primary     ?
_atom_sites_solution_secondary   ?
_atom_sites_solution_hydrogens   .
_refine_ls_hydrogen_treatment    undef
_refine_ls_extinction_method     none
_refine_ls_extinction_coef       .
_refine_ls_number_reflns         10686
_refine_ls_number_parameters     384
_refine_ls_number_restraints     0
_refine_ls_R_factor_all          0.0611
_refine_ls_R_factor_gt           0.0433
_refine_ls_wR_factor_ref         0.1213
_refine_ls_wR_factor_gt          0.1106
_refine_ls_goodness_of_fit_ref   1.003
_refine_ls_restrained_S_all      1.003
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_diff_density_max         3.503
_refine_diff_density_min         -3.588
_refine_diff_density_rms         0.490

loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
Si1 Si 0.4627(3) 0.6659(2) 0.14499(16) 0.0132(7) Uani 1 1 d . . . . .
W1 W 0.50896(4) 0.58605(4) 0.28471(2) 0.01567(13) Uani 1 1 d . . . . .
W2 W 0.28098(4) 0.68424(4) 0.23753(2) 0.01442(12) Uani 1 1 d . . . . .
W3 W 0.50308(4) 0.79672(4) 0.26656(2) 0.01400(12) Uani 1 1 d . . . . .
W4 W 0.23590(4) 0.53987(4) 0.11072(2) 0.01451(12) Uani 1 1 d . . . . .
W5 W 0.46142(4) 0.44334(4) 0.15742(3) 0.01581(13) Uani 1 1 d . . . . .
W6 W 0.70720(4) 0.57283(4) 0.19118(2) 0.01541(13) Uani 1 1 d . . . . .
W7 W 0.70088(4) 0.78305(4) 0.17202(2) 0.01461(12) Uani 1 1 d . . . . .
W8 W 0.22812(4) 0.77372(4) 0.09079(2) 0.01549(13) Uani 1 1 d . . . . .
W9 W 0.44542(4) 0.88835(4) 0.12065(2) 0.01478(12) Uani 1 1 d . . . . .
W10 W 0.41073(4) 0.75159(4) 0.00481(3) 0.01779(13) Uani 1 1 d . . . . .
Co1 Co 0.41576(14) 0.52943(12) 0.03219(8) 0.0155(4) Uani 1 1 d . . . . .
Co2 Co 0.65174(13) 0.65502(11) 0.06324(8) 0.0122(4) Uani 1 1 d . . . . .
O12 O 0.3645(7) 0.6137(6) 0.2918(4) 0.016(2) Uiso 1 1 d . . . . .
O13 O 0.5374(7) 0.7005(6) 0.3162(4) 0.0143(19) Uiso 1 1 d . . . . .
O15 O 0.4606(7) 0.5020(6) 0.2335(4) 0.019(2) Uiso 1 1 d . . . . .
O16 O 0.6318(7) 0.5917(6) 0.2566(4) 0.017(2) Uiso 1 1 d . . . . .
O23 O 0.3578(7) 0.7798(6) 0.2742(4) 0.017(2) Uiso 1 1 d . . . . .
O24 O 0.2492(7) 0.5936(6) 0.1876(4) 0.015(2) Uiso 1 1 d . . . . .
O28 O 0.2439(7) 0.7549(6) 0.1716(4) 0.016(2) Uiso 1 1 d . . . . .
O37 O 0.6240(7) 0.7850(6) 0.2383(4) 0.016(2) Uiso 1 1 d . . . . .
O39 O 0.4481(7) 0.8603(6) 0.1998(4) 0.0143(19) Uiso 1 1 d . . . . .
O48 O 0.2094(7) 0.6545(6) 0.0843(4) 0.018(2) Uiso 1 1 d . . . . .
O67 O 0.7671(7) 0.6834(6) 0.2113(4) 0.018(2) Uiso 1 1 d . . . . .
O79 O 0.5873(7) 0.8521(6) 0.1366(4) 0.0147(19) Uiso 1 1 d . . . . .
O89 O 0.2975(7) 0.8815(6) 0.1104(4) 0.017(2) Uiso 1 1 d . . . . .
O810 O 0.2626(7) 0.7818(6) 0.0186(4) 0.019(2) Uiso 1 1 d . . . . .
O910 O 0.4377(7) 0.8715(6) 0.0434(4) 0.0155(19) Uiso 1 1 d . . . . .
O1C1 O 0.2631(7) 0.5057(6) 0.0419(4) 0.016(2) Uiso 1 1 d . . . . .
O1C2 O 0.5479(7) 0.7365(6) 0.0214(4) 0.017(2) Uiso 1 1 d . . . . .
O2C1 O 0.4554(7) 0.4223(6) 0.0842(4) 0.017(2) Uiso 1 1 d . . . . .
O2C2 O 0.7391(7) 0.7544(6) 0.1061(4) 0.020(2) Uiso 1 1 d . . . . .
O3C1 O 0.3719(7) 0.6435(6) -0.0056(4) 0.018(2) Uiso 1 1 d . . . . .
O3C2 O 0.7463(7) 0.5744(6) 0.1223(4) 0.018(2) Uiso 1 1 d . . . . .
O4C1 O 0.5991(7) 0.4913(6) 0.1678(4) 0.017(2) Uiso 1 1 d . . . . .
O4C2 O 0.5760(7) 0.5446(6) 0.0384(4) 0.017(2) Uiso 1 1 d . . . . .
O5C2 O 0.7411(8) 0.6556(7) -0.0021(5) 0.025(2) Uiso 1 1 d . . . . .
O6C1 O 0.3113(7) 0.4455(6) 0.1503(4) 0.017(2) Uiso 1 1 d . . . . .
O1SI O 0.5867(7) 0.6677(6) 0.1446(4) 0.0138(19) Uiso 1 1 d . . . . .
O2SI O 0.4050(7) 0.7422(6) 0.1045(4) 0.016(2) Uiso 1 1 d . . . . .
O3SI O 0.4106(7) 0.5770(6) 0.1215(4) 0.015(2) Uiso 1 1 d . . . . .
O4SI O 0.4447(7) 0.6805(6) 0.2105(4) 0.015(2) Uiso 1 1 d . . . . .
O1T O 0.5469(8) 0.5303(7) 0.3471(5) 0.023(2) Uiso 1 1 d . . . . .
O2T O 0.1722(7) 0.6931(6) 0.2683(4) 0.017(2) Uiso 1 1 d . . . . .
O3T O 0.5337(7) 0.8755(6) 0.3181(4) 0.018(2) Uiso 1 1 d . . . . .
O4T O 0.1098(7) 0.5022(6) 0.1068(4) 0.020(2) Uiso 1 1 d . . . . .
O5T O 0.4867(8) 0.3424(7) 0.1866(5) 0.023(2) Uiso 1 1 d . . . . .
O6T O 0.8033(7) 0.5116(6) 0.2307(4) 0.019(2) Uiso 1 1 d . . . . .
O7T O 0.7910(7) 0.8573(6) 0.1986(4) 0.018(2) Uiso 1 1 d . . . . .
O8T O 0.1005(8) 0.8075(7) 0.0751(5) 0.022(2) Uiso 1 1 d . . . . .
O9T O 0.4619(7) 0.9971(6) 0.1258(4) 0.018(2) Uiso 1 1 d . . . . .
O10T O 0.3911(7) 0.7916(6) -0.0648(4) 0.019(2) Uiso 1 1 d . . . . .
Cs1 Cs 0.80043(7) 0.53922(6) 0.36242(4) 0.0243(2) Uani 1 1 d . . . . .
Cs2 Cs 0.47437(8) 0.33932(7) 0.31140(5) 0.0308(2) Uani 1 1 d . . . . .
Cs3 Cs 0.46073(7) 0.04104(6) 0.26253(5) 0.0250(2) Uani 1 1 d . . . . .
Cs4 Cs 0.77436(7) 0.83526(6) 0.35335(5) 0.0265(2) Uani 1 1 d . . . . .
Cs5 Cs 0.38196(8) 0.19754(7) 0.09323(5) 0.0313(2) Uani 1 1 d . . . . .
Na1 Na 0.0004(4) 0.3857(4) 0.0839(3) 0.0226(13) Uani 1 1 d . . . . .
Na2 Na 0.6264(9) 0.4453(8) 0.5210(5) 0.026(3) Uiso 0.5 1 d . . P . .
O1W O 0.1646(8) 0.3072(7) 0.1166(5) 0.027(2) Uiso 1 1 d . . . . .
O2W O 0.0134(10) 0.3785(8) -0.0173(6) 0.038(3) Uiso 1 1 d . . . . .
O3W O -0.1024(12) 0.2642(10) 0.0708(7) 0.057(4) Uiso 1 1 d . . . . .
O4W O -0.1313(10) 0.4855(8) 0.0605(6) 0.037(3) Uiso 1 1 d . . . . .
O5W O 0.5476(9) 0.1669(8) 0.3623(6) 0.037(3) Uiso 1 1 d . . . . .
O6W O 0.9235(8) 0.6830(7) 0.3008(5) 0.028(2) Uiso 1 1 d . . . . .
O7W O 0.2416(7) -0.0630(6) 0.2285(4) 0.020(2) Uiso 1 1 d . . . . .
O8W O 0.7192(10) 0.4480(8) 0.6153(6) 0.037(3) Uiso 1 1 d . . . . .
O9W O 0.606(2) 0.2906(18) 0.5185(12) 0.044(7) Uiso 0.5 1 d . . P B .
O10W O 0.4961(17) 0.4630(14) 0.4432(10) 0.027(5) Uiso 0.5 1 d . . P B .
O11W O 0.7139(19) 0.5500(16) 0.4798(12) 0.039(6) Uiso 0.5 1 d . . P B .
O12W O 0.586(2) 0.972(2) 0.0129(13) 0.053(8) Uiso 0.5 1 d . . P A 1
O13W O 0.830(3) 0.394(2) 0.4754(17) 0.077(10) Uiso 0.5 1 d . . P B 2


_geom_special_details            
; 
 All esds (except the esd in the dihedral angle between two l.s. planes) 
 are estimated using the full covariance matrix.  The cell esds are taken 
 into account individually in the estimation of esds in distances, angles 
 and torsion angles; correlations between esds in cell parameters are only 
 used when they are defined by crystal symmetry.  An approximate (isotropic) 
 treatment of cell esds is used for estimating esds involving l.s. planes. 
;

loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Si1 O3SI 1.615(10) . ?
Si1 O1SI 1.627(10) . ?
Si1 O4SI 1.638(10) . ?
Si1 O2SI 1.640(10) . ?
W1 O1T 1.720(11) . ?
W1 O15 1.836(10) . ?
W1 O16 1.855(10) . ?
W1 O13 1.967(9) . ?
W1 O12 1.980(9) . ?
W1 O4SI 2.348(10) . ?
W2 O2T 1.725(10) . ?
W2 O24 1.859(9) . ?
W2 O12 1.895(10) . ?
W2 O28 1.915(10) . ?
W2 O23 1.933(10) . ?
W2 O4SI 2.352(9) . ?
W3 O3T 1.743(10) . ?
W3 O37 1.842(9) . ?
W3 O39 1.908(9) . ?
W3 O13 1.928(9) . ?
W3 O23 1.964(9) . ?
W3 O4SI 2.316(10) . ?
W4 O4T 1.743(10) . ?
W4 O1C1 1.823(10) . ?
W4 O48 1.927(10) . ?
W4 O6C1 1.935(10) . ?
W4 O24 1.998(10) . ?
W4 O3SI 2.332(9) . ?
W5 O5T 1.746(10) . ?
W5 O2C1 1.764(10) . ?
W5 O4C1 1.930(9) . ?
W5 O6C1 1.944(9) . ?
W5 O15 2.038(10) . ?
W5 O3SI 2.329(9) . ?
W6 O6T 1.724(10) . ?
W6 O3C2 1.809(10) . ?
W6 O4C1 1.920(9) . ?
W6 O67 1.939(10) . ?
W6 O16 2.017(10) . ?
W6 O1SI 2.308(9) . ?
W7 O7T 1.701(10) . ?
W7 O2C2 1.793(10) . ?
W7 O79 1.912(9) . ?
W7 O67 1.951(10) . ?
W7 O37 2.024(10) . ?
W7 O1SI 2.372(9) . ?
W8 O8T 1.730(10) . ?
W8 O810 1.862(10) . ?
W8 O48 1.902(10) . ?
W8 O28 1.922(10) . ?
W8 O89 1.946(10) . ?
W8 O2SI 2.334(9) . ?
W9 O9T 1.733(10) . ?
W9 O910 1.845(10) . ?
W9 O89 1.912(9) . ?
W9 O79 1.915(9) . ?
W9 O39 1.931(10) . ?
W9 O2SI 2.383(10) . ?
W10 O10T 1.749(10) . ?
W10 O1C2 1.784(9) . ?
W10 O3C1 1.786(10) . ?
W10 O810 2.083(10) . ?
W10 O910 2.107(9) . ?
W10 O2SI 2.395(10) . ?
Co1 O3C1 2.049(10) . ?
Co1 O4C2 2.068(10) 3_665 ?
Co1 O1C1 2.090(9) . ?
Co1 O4C2 2.092(10) . ?
Co1 O2C1 2.106(10) . ?
Co1 O3SI 2.269(10) . ?
Co2 O1C2 2.001(10) . ?
Co2 O4C2 2.040(10) . ?
Co2 O2C2 2.095(10) . ?
Co2 O5C2 2.113(11) . ?
Co2 O3C2 2.120(10) . ?
Co2 O1SI 2.265(10) . ?
Co2 Cs5 4.350(2) 3_665 ?
O13 Cs4 3.734(9) . ?
O15 Cs2 3.156(10) . ?
O16 Cs1 3.143(10) . ?
O24 Cs3 3.298(9) 2 ?
O28 Cs2 3.249(9) 2 ?
O37 Cs4 3.169(10) . ?
O39 Cs3 3.213(9) 1_565 ?
O79 Cs1 3.300(9) 2_655 ?
O1C2 Cs5 3.212(10) 3_665 ?
O2C1 Cs5 3.694(10) . ?
O3C1 Cs4 3.385(10) 4_575 ?
O4C1 Cs4 3.064(10) 2_645 ?
O4C2 Co1 2.068(10) 3_665 ?
O5C2 Cs5 3.377(11) 3_665 ?
O1T Cs2 3.229(10) . ?
O1T Cs1 3.278(10) . ?
O2T Cs3 2.979(9) 2 ?
O2T Cs2 3.360(10) 2 ?
O2T Cs5 3.502(10) 2 ?
O3T Na1 2.462(12) 2 ?
O3T Cs3 3.007(10) 1_565 ?
O3T Cs4 3.175(9) . ?
O4T Na1 2.336(11) . ?
O4T Cs3 3.463(10) 2 ?
O5T Cs2 3.010(11) . ?
O5T Cs5 3.308(11) . ?
O5T Cs4 3.438(10) 2_645 ?
O6T Cs3 3.101(10) 2_655 ?
O6T Cs1 3.176(10) . ?
O6T Cs4 3.473(10) 2_645 ?
O7T Cs2 3.141(10) 2_655 ?
O7T Cs1 3.341(10) 2_655 ?
O7T Cs4 3.751(10) . ?
O8T Cs2 3.083(11) 2 ?
O9T Cs1 3.146(9) 2_655 ?
O9T Cs3 3.335(10) 1_565 ?
O9T Cs5 3.380(10) 1_565 ?
O10T Cs4 3.010(10) 4_575 ?
O10T Cs5 3.174(10) 3_665 ?
O10T Cs1 3.287(10) 4_575 ?
Cs1 O9T 3.146(10) 2_645 ?
Cs1 O11W 3.21(3) . ?
Cs1 O12W 3.24(3) 2_645 ?
Cs1 O6W 3.285(11) . ?
Cs1 O10T 3.287(10) 4_676 ?
Cs1 O79 3.300(9) 2_645 ?
Cs1 O7T 3.341(10) 2_645 ?
Cs1 O13W 3.50(4) . ?
Cs2 O5W 3.062(12) . ?
Cs2 O8T 3.083(11) 2_545 ?
Cs2 O7T 3.141(10) 2_645 ?
Cs2 O7W 3.210(10) 2 ?
Cs2 O28 3.249(9) 2_545 ?
Cs2 O2T 3.360(10) 2_545 ?
Cs2 O10W 3.66(2) . ?
Cs3 O2T 2.979(9) 2_545 ?
Cs3 O3T 3.007(10) 1_545 ?
Cs3 O6T 3.101(10) 2_645 ?
Cs3 O5W 3.147(13) . ?
Cs3 O39 3.213(9) 1_545 ?
Cs3 O6W 3.234(11) 2_645 ?
Cs3 O7W 3.279(10) . ?
Cs3 O24 3.298(9) 2_545 ?
Cs3 O9T 3.335(10) 1_545 ?
Cs3 O4T 3.463(10) 2_545 ?
Cs4 O10T 3.010(10) 4_676 ?
Cs4 O4C1 3.064(10) 2_655 ?
Cs4 O3W 3.332(16) 2 ?
Cs4 O3C1 3.385(10) 4_676 ?
Cs4 O5T 3.438(10) 2_655 ?
Cs4 O6T 3.473(10) 2_655 ?
Cs4 O6W 3.474(11) . ?
Cs5 O13W 3.12(4) 4_565 ?
Cs5 O10T 3.175(10) 3_665 ?
Cs5 O1C2 3.212(10) 3_665 ?
Cs5 O8W 3.245(13) 4_565 ?
Cs5 O6W 3.249(11) 2_645 ?
Cs5 O5C2 3.377(11) 3_665 ?
Cs5 O9T 3.380(10) 1_545 ?
Cs5 O1W 3.465(11) . ?
Cs5 O2T 3.502(10) 2_545 ?
Cs5 O9W 3.73(3) 4_565 ?
Na1 O4W 2.328(14) . ?
Na1 O3W 2.331(17) . ?
Na1 O2W 2.451(14) . ?
Na1 O3T 2.462(12) 2_545 ?
Na1 O1W 2.482(12) . ?
Na1 Cs4 4.221(6) 2_545 ?
Na1 Cs3 4.358(6) 2 ?
Na2 O10W 2.30(3) . ?
Na2 O11W 2.33(3) . ?
Na2 O8W 2.350(18) . ?
Na2 O10W 2.43(3) 3_666 ?
Na2 O9W 2.46(3) . ?
Na2 Na2 3.71(2) 3_666 ?
Na2 Cs5 4.140(12) 4_666 ?
O3W Cs4 3.332(16) 2_545 ?
O6W Cs3 3.234(11) 2_655 ?
O6W Cs5 3.250(11) 2_655 ?
O7W Cs2 3.210(10) 2_545 ?
O8W Cs5 3.245(13) 4_666 ?
O9W Cs5 3.73(3) 4_666 ?
O10W Na2 2.43(3) 3_666 ?
O12W Cs1 3.24(3) 2_655 ?
O12W Cs5 3.76(3) 3_665 ?
O13W Cs5 3.12(4) 4_666 ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O3SI Si1 O1SI 111.8(5) . . ?
O3SI Si1 O4SI 109.1(5) . . ?
O1SI Si1 O4SI 108.8(5) . . ?
O3SI Si1 O2SI 108.4(5) . . ?
O1SI Si1 O2SI 109.6(5) . . ?
O4SI Si1 O2SI 109.0(5) . . ?
O1T W1 O15 102.3(5) . . ?
O1T W1 O16 101.8(5) . . ?
O15 W1 O16 90.6(4) . . ?
O1T W1 O13 97.8(4) . . ?
O15 W1 O13 159.5(4) . . ?
O16 W1 O13 88.7(4) . . ?
O1T W1 O12 99.7(4) . . ?
O15 W1 O12 89.9(4) . . ?
O16 W1 O12 157.9(4) . . ?
O13 W1 O12 83.2(4) . . ?
O1T W1 O4SI 169.3(4) . . ?
O15 W1 O4SI 85.8(4) . . ?
O16 W1 O4SI 85.0(4) . . ?
O13 W1 O4SI 73.7(4) . . ?
O12 W1 O4SI 73.1(4) . . ?
O1T W1 Cs2 52.1(3) . . ?
O15 W1 Cs2 50.5(3) . . ?
O16 W1 Cs2 103.7(3) . . ?
O13 W1 Cs2 148.9(3) . . ?
O12 W1 Cs2 93.6(3) . . ?
O4SI W1 Cs2 134.9(2) . . ?
O1T W1 Cs1 53.5(3) . . ?
O15 W1 Cs1 111.0(3) . . ?
O16 W1 Cs1 50.0(3) . . ?
O13 W1 Cs1 84.0(3) . . ?
O12 W1 Cs1 148.0(3) . . ?
O4SI W1 Cs1 130.3(2) . . ?
Cs2 W1 Cs1 82.66(2) . . ?
O2T W2 O24 103.3(4) . . ?
O2T W2 O12 100.1(4) . . ?
O24 W2 O12 91.0(4) . . ?
O2T W2 O28 101.4(4) . . ?
O24 W2 O28 86.0(4) . . ?
O12 W2 O28 158.4(4) . . ?
O2T W2 O23 98.4(4) . . ?
O24 W2 O23 158.1(4) . . ?
O12 W2 O23 87.8(4) . . ?
O28 W2 O23 87.0(4) . . ?
O2T W2 O4SI 170.3(4) . . ?
O24 W2 O4SI 85.0(4) . . ?
O12 W2 O4SI 74.4(4) . . ?
O28 W2 O4SI 84.0(4) . . ?
O23 W2 O4SI 73.6(4) . . ?
O2T W2 Cs3 46.5(3) . 2 ?
O24 W2 Cs3 57.7(3) . 2 ?
O12 W2 Cs3 91.5(3) . 2 ?
O28 W2 Cs3 104.8(3) . 2 ?
O23 W2 Cs3 144.1(3) . 2 ?
O4SI W2 Cs3 140.2(2) . 2 ?
O2T W2 Cs2 51.9(3) . 2 ?
O24 W2 Cs2 101.6(3) . 2 ?
O12 W2 Cs2 151.1(3) . 2 ?
O28 W2 Cs2 49.8(3) . 2 ?
O23 W2 Cs2 89.6(3) . 2 ?
O4SI W2 Cs2 132.0(2) . 2 ?
Cs3 W2 Cs2 74.22(2) 2 2 ?
O3T W3 O37 103.2(4) . . ?
O3T W3 O39 102.4(4) . . ?
O37 W3 O39 88.1(4) . . ?
O3T W3 O13 97.6(4) . . ?
O37 W3 O13 91.5(4) . . ?
O39 W3 O13 159.5(4) . . ?
O3T W3 O23 97.6(4) . . ?
O37 W3 O23 159.1(4) . . ?
O39 W3 O23 85.7(4) . . ?
O13 W3 O23 87.5(4) . . ?
O3T W3 O4SI 168.9(4) . . ?
O37 W3 O4SI 85.6(4) . . ?
O39 W3 O4SI 84.4(4) . . ?
O13 W3 O4SI 75.2(4) . . ?
O23 W3 O4SI 73.9(4) . . ?
O3T W3 Cs4 55.5(3) . . ?
O37 W3 Cs4 55.7(3) . . ?
O39 W3 Cs4 122.6(3) . . ?
O13 W3 Cs4 72.8(3) . . ?
O23 W3 Cs4 142.5(3) . . ?
O4SI W3 Cs4 127.9(2) . . ?
O3T W3 Cs3 47.4(3) . 1_565 ?
O37 W3 Cs3 102.7(3) . 1_565 ?
O39 W3 Cs3 55.1(3) . 1_565 ?
O13 W3 Cs3 144.3(3) . 1_565 ?
O23 W3 Cs3 90.0(3) . 1_565 ?
O4SI W3 Cs3 137.8(2) . 1_565 ?
Cs4 W3 Cs3 88.26(2) . 1_565 ?
O4T W4 O1C1 101.0(5) . . ?
O4T W4 O48 101.0(4) . . ?
O1C1 W4 O48 92.1(4) . . ?
O4T W4 O6C1 99.0(4) . . ?
O1C1 W4 O6C1 92.5(4) . . ?
O48 W4 O6C1 158.1(4) . . ?
O4T W4 O24 96.7(4) . . ?
O1C1 W4 O24 162.3(4) . . ?
O48 W4 O24 83.1(4) . . ?
O6C1 W4 O24 86.0(4) . . ?
O4T W4 O3SI 173.8(4) . . ?
O1C1 W4 O3SI 79.8(4) . . ?
O48 W4 O3SI 85.0(4) . . ?
O6C1 W4 O3SI 74.8(4) . . ?
O24 W4 O3SI 82.8(4) . . ?
O4T W4 Cs3 50.0(3) . 2 ?
O1C1 W4 Cs3 150.6(3) . 2 ?
O48 W4 Cs3 97.5(3) . 2 ?
O6C1 W4 Cs3 88.8(3) . 2 ?
O24 W4 Cs3 47.1(3) . 2 ?
O3SI W4 Cs3 128.5(2) . 2 ?
O5T W5 O2C1 101.1(5) . . ?
O5T W5 O4C1 101.7(4) . . ?
O2C1 W5 O4C1 94.1(4) . . ?
O5T W5 O6C1 99.5(4) . . ?
O2C1 W5 O6C1 93.3(4) . . ?
O4C1 W5 O6C1 155.7(4) . . ?
O5T W5 O15 95.3(5) . . ?
O2C1 W5 O15 163.6(4) . . ?
O4C1 W5 O15 82.3(4) . . ?
O6C1 W5 O15 84.2(4) . . ?
O5T W5 O3SI 173.9(4) . . ?
O2C1 W5 O3SI 81.3(4) . . ?
O4C1 W5 O3SI 83.6(4) . . ?
O6C1 W5 O3SI 74.7(4) . . ?
O15 W5 O3SI 82.4(4) . . ?
O5T W5 Cs4 61.5(3) . 2_645 ?
O2C1 W5 Cs4 74.4(3) . 2_645 ?
O4C1 W5 Cs4 50.4(3) . 2_645 ?
O6C1 W5 Cs4 153.6(3) . 2_645 ?
O15 W5 Cs4 114.0(3) . 2_645 ?
O3SI W5 Cs4 124.6(2) . 2_645 ?
O5T W5 Cs2 44.5(4) . . ?
O2C1 W5 Cs2 144.8(3) . . ?
O4C1 W5 Cs2 99.4(3) . . ?
O6C1 W5 Cs2 87.6(3) . . ?
O15 W5 Cs2 51.4(3) . . ?
O3SI W5 Cs2 132.2(2) . . ?
Cs4 W5 Cs2 89.57(2) 2_645 . ?
O5T W5 Cs5 47.3(3) . . ?
O2C1 W5 Cs5 60.4(3) . . ?
O4C1 W5 Cs5 124.6(3) . . ?
O6C1 W5 Cs5 78.9(3) . . ?
O15 W5 Cs5 134.2(3) . . ?
O3SI W5 Cs5 131.6(2) . . ?
Cs4 W5 Cs5 74.79(2) 2_645 . ?
Cs2 W5 Cs5 85.45(3) . . ?
O6T W6 O3C2 101.7(5) . . ?
O6T W6 O4C1 102.0(4) . . ?
O3C2 W6 O4C1 93.6(4) . . ?
O6T W6 O67 98.5(4) . . ?
O3C2 W6 O67 92.5(4) . . ?
O4C1 W6 O67 156.9(4) . . ?
O6T W6 O16 94.2(4) . . ?
O3C2 W6 O16 164.1(4) . . ?
O4C1 W6 O16 83.3(4) . . ?
O67 W6 O16 84.8(4) . . ?
O6T W6 O1SI 173.4(4) . . ?
O3C2 W6 O1SI 80.6(4) . . ?
O4C1 W6 O1SI 83.8(4) . . ?
O67 W6 O1SI 75.2(4) . . ?
O16 W6 O1SI 83.5(4) . . ?
O6T W6 Cs4 62.3(3) . 2_645 ?
O3C2 W6 Cs4 74.0(3) . 2_645 ?
O4C1 W6 Cs4 50.1(3) . 2_645 ?
O67 W6 Cs4 152.5(3) . 2_645 ?
O16 W6 Cs4 114.5(3) . 2_645 ?
O1SI W6 Cs4 124.2(2) . 2_645 ?
O6T W6 Cs1 47.6(3) . . ?
O3C2 W6 Cs1 146.0(3) . . ?
O4C1 W6 Cs1 105.8(3) . . ?
O67 W6 Cs1 80.6(3) . . ?
O16 W6 Cs1 49.0(3) . . ?
O1SI W6 Cs1 128.3(2) . . ?
Cs4 W6 Cs1 97.15(2) 2_645 . ?
O6T W6 Cs3 36.3(3) . 2_655 ?
O3C2 W6 Cs3 78.1(3) . 2_655 ?
O4C1 W6 Cs3 130.7(3) . 2_655 ?
O67 W6 Cs3 72.5(3) . 2_655 ?
O16 W6 Cs3 115.7(3) . 2_655 ?
O1SI W6 Cs3 140.1(2) . 2_655 ?
Cs4 W6 Cs3 81.28(2) 2_645 2_655 ?
Cs1 W6 Cs3 68.08(2) . 2_655 ?
O7T W7 O2C2 102.3(5) . . ?
O7T W7 O79 101.6(4) . . ?
O2C2 W7 O79 94.4(4) . . ?
O7T W7 O67 99.2(4) . . ?
O2C2 W7 O67 92.6(4) . . ?
O79 W7 O67 156.0(4) . . ?
O7T W7 O37 96.3(4) . . ?
O2C2 W7 O37 161.3(4) . . ?
O79 W7 O37 82.9(4) . . ?
O67 W7 O37 83.0(4) . . ?
O7T W7 O1SI 172.5(4) . . ?
O2C2 W7 O1SI 80.1(4) . . ?
O79 W7 O1SI 85.2(4) . . ?
O67 W7 O1SI 73.4(4) . . ?
O37 W7 O1SI 81.2(4) . . ?
O7T W7 Cs1 51.4(3) . 2_655 ?
O2C2 W7 Cs1 93.7(3) . 2_655 ?
O79 W7 Cs1 51.6(3) . 2_655 ?
O67 W7 Cs1 150.6(3) . 2_655 ?
O37 W7 Cs1 99.0(3) . 2_655 ?
O1SI W7 Cs1 136.0(2) . 2_655 ?
O7T W7 Cs2 38.3(3) . 2_655 ?
O2C2 W7 Cs2 72.6(3) . 2_655 ?
O79 W7 Cs2 126.9(3) . 2_655 ?
O67 W7 Cs2 77.1(3) . 2_655 ?
O37 W7 Cs2 123.5(3) . 2_655 ?
O1SI W7 Cs2 138.5(2) . 2_655 ?
Cs1 W7 Cs2 77.48(2) 2_655 2_655 ?
O7T W7 Cs4 59.1(3) . . ?
O2C2 W7 Cs4 151.2(3) . . ?
O79 W7 Cs4 110.1(3) . . ?
O67 W7 Cs4 71.2(3) . . ?
O37 W7 Cs4 43.1(3) . . ?
O1SI W7 Cs4 115.8(2) . . ?
Cs1 W7 Cs4 90.22(2) 2_655 . ?
Cs2 W7 Cs4 80.46(2) 2_655 . ?
O8T W8 O810 99.7(5) . . ?
O8T W8 O48 100.5(4) . . ?
O810 W8 O48 92.4(4) . . ?
O8T W8 O28 100.7(5) . . ?
O810 W8 O28 159.5(4) . . ?
O48 W8 O28 85.3(4) . . ?
O8T W8 O89 100.0(4) . . ?
O810 W8 O89 88.9(4) . . ?
O48 W8 O89 159.0(4) . . ?
O28 W8 O89 86.3(4) . . ?
O8T W8 O2SI 172.7(4) . . ?
O810 W8 O2SI 75.0(4) . . ?
O48 W8 O2SI 84.8(4) . . ?
O28 W8 O2SI 84.6(4) . . ?
O89 W8 O2SI 75.2(4) . . ?
O8T W8 Cs2 47.4(4) . 2 ?
O810 W8 Cs2 145.6(3) . 2 ?
O48 W8 Cs2 102.5(3) . 2 ?
O28 W8 Cs2 54.1(3) . 2 ?
O89 W8 Cs2 87.9(3) . 2 ?
O2SI W8 Cs2 136.5(2) . 2 ?
O9T W9 O910 101.3(4) . . ?
O9T W9 O89 100.1(4) . . ?
O910 W9 O89 89.8(4) . . ?
O9T W9 O79 100.3(4) . . ?
O910 W9 O79 91.6(4) . . ?
O89 W9 O79 158.9(4) . . ?
O9T W9 O39 100.3(4) . . ?
O910 W9 O39 158.4(4) . . ?
O89 W9 O39 87.0(4) . . ?
O79 W9 O39 84.0(4) . . ?
O9T W9 O2SI 173.0(4) . . ?
O910 W9 O2SI 74.3(4) . . ?
O89 W9 O2SI 74.6(4) . . ?
O79 W9 O2SI 85.5(4) . . ?
O39 W9 O2SI 84.2(4) . . ?
O9T W9 Cs1 47.2(3) . 2_655 ?
O910 W9 Cs1 94.4(3) . 2_655 ?
O89 W9 Cs1 147.2(3) . 2_655 ?
O79 W9 Cs1 53.6(3) . 2_655 ?
O39 W9 Cs1 99.8(3) . 2_655 ?
O2SI W9 Cs1 137.7(2) . 2_655 ?
O9T W9 Cs3 51.4(3) . 1_565 ?
O910 W9 Cs3 152.5(3) . 1_565 ?
O89 W9 Cs3 91.9(3) . 1_565 ?
O79 W9 Cs3 96.5(3) . 1_565 ?
O39 W9 Cs3 49.1(3) . 1_565 ?
O2SI W9 Cs3 132.4(2) . 1_565 ?
Cs1 W9 Cs3 70.12(2) 2_655 1_565 ?
O10T W10 O1C2 103.0(5) . . ?
O10T W10 O3C1 103.0(5) . . ?
O1C2 W10 O3C1 98.8(4) . . ?
O10T W10 O810 95.1(4) . . ?
O1C2 W10 O810 157.8(4) . . ?
O3C1 W10 O810 89.5(4) . . ?
O10T W10 O910 94.2(4) . . ?
O1C2 W10 O910 86.7(4) . . ?
O3C1 W10 O910 160.2(4) . . ?
O810 W10 O910 79.1(4) . . ?
O10T W10 O2SI 159.5(4) . . ?
O1C2 W10 O2SI 89.2(4) . . ?
O3C1 W10 O2SI 91.1(4) . . ?
O810 W10 O2SI 70.0(4) . . ?
O910 W10 O2SI 69.9(3) . . ?
O10T W10 Cs4 45.5(3) . 4_575 ?
O1C2 W10 Cs4 115.0(3) . 4_575 ?
O3C1 W10 Cs4 58.2(3) . 4_575 ?
O810 W10 Cs4 86.9(3) . 4_575 ?
O910 W10 Cs4 136.0(3) . 4_575 ?
O2SI W10 Cs4 142.2(2) . 4_575 ?
O10T W10 Cs5 50.7(3) . 3_665 ?
O1C2 W10 Cs5 52.2(3) . 3_665 ?
O3C1 W10 Cs5 108.6(3) . 3_665 ?
O810 W10 Cs5 143.5(3) . 3_665 ?
O910 W10 Cs5 89.8(3) . 3_665 ?
O2SI W10 Cs5 138.1(2) . 3_665 ?
Cs4 W10 Cs5 77.13(2) 4_575 3_665 ?
O3C1 Co1 O4C2 101.1(4) . 3_665 ?
O3C1 Co1 O1C1 90.5(4) . . ?
O4C2 Co1 O1C1 100.5(4) 3_665 . ?
O3C1 Co1 O4C2 97.3(4) . . ?
O4C2 Co1 O4C2 85.4(4) 3_665 . ?
O1C1 Co1 O4C2 169.1(4) . . ?
O3C1 Co1 O2C1 169.9(4) . . ?
O4C2 Co1 O2C1 88.9(4) 3_665 . ?
O1C1 Co1 O2C1 85.9(4) . . ?
O4C2 Co1 O2C1 85.1(4) . . ?
O3C1 Co1 O3SI 93.8(4) . . ?
O4C2 Co1 O3SI 164.8(4) 3_665 . ?
O1C1 Co1 O3SI 76.2(4) . . ?
O4C2 Co1 O3SI 95.7(4) . . ?
O2C1 Co1 O3SI 76.2(4) . . ?
O1C2 Co2 O4C2 98.9(4) . . ?
O1C2 Co2 O2C2 91.2(4) . . ?
O4C2 Co2 O2C2 167.3(4) . . ?
O1C2 Co2 O5C2 92.8(4) . . ?
O4C2 Co2 O5C2 95.5(4) . . ?
O2C2 Co2 O5C2 91.6(4) . . ?
O1C2 Co2 O3C2 168.0(4) . . ?
O4C2 Co2 O3C2 82.7(4) . . ?
O2C2 Co2 O3C2 85.8(4) . . ?
O5C2 Co2 O3C2 99.0(4) . . ?
O1C2 Co2 O1SI 92.4(4) . . ?
O4C2 Co2 O1SI 94.8(4) . . ?
O2C2 Co2 O1SI 77.0(4) . . ?
O5C2 Co2 O1SI 167.6(4) . . ?
O3C2 Co2 O1SI 75.6(4) . . ?
O1C2 Co2 Cs5 43.6(3) . 3_665 ?
O4C2 Co2 Cs5 104.0(3) . 3_665 ?
O2C2 Co2 Cs5 88.7(3) . 3_665 ?
O5C2 Co2 Cs5 49.3(3) . 3_665 ?
O3C2 Co2 Cs5 147.7(3) . 3_665 ?
O1SI Co2 Cs5 133.7(2) . 3_665 ?
W2 O12 W1 120.8(5) . . ?
W3 O13 W1 118.9(5) . . ?
W3 O13 Cs4 77.6(3) . . ?
W1 O13 Cs4 134.9(4) . . ?
W1 O15 W5 149.6(6) . . ?
W1 O15 Cs2 102.8(4) . . ?
W5 O15 Cs2 98.3(4) . . ?
W1 O16 W6 148.6(5) . . ?
W1 O16 Cs1 103.1(4) . . ?
W6 O16 Cs1 102.1(3) . . ?
W2 O23 W3 119.8(5) . . ?
W2 O24 W4 152.3(5) . . ?
W2 O24 Cs3 93.8(3) . 2 ?
W4 O24 Cs3 106.6(3) . 2 ?
W2 O28 W8 151.2(6) . . ?
W2 O28 Cs2 103.5(4) . 2 ?
W8 O28 Cs2 97.3(3) . 2 ?
W3 O37 W7 150.7(5) . . ?
W3 O37 Cs4 95.6(4) . . ?
W7 O37 Cs4 111.1(4) . . ?
W3 O39 W9 150.6(5) . . ?
W3 O39 Cs3 95.7(3) . 1_565 ?
W9 O39 Cs3 103.9(4) . 1_565 ?
W8 O48 W4 153.0(6) . . ?
W6 O67 W7 118.9(5) . . ?
W7 O79 W9 155.1(6) . . ?
W7 O79 Cs1 101.4(3) . 2_655 ?
W9 O79 Cs1 98.6(3) . 2_655 ?
W9 O89 W8 119.9(5) . . ?
W8 O810 W10 121.4(5) . . ?
W9 O910 W10 122.6(5) . . ?
W4 O1C1 Co1 113.3(5) . . ?
W10 O1C2 Co2 139.6(6) . . ?
W10 O1C2 Cs5 101.7(4) . 3_665 ?
Co2 O1C2 Cs5 111.0(4) . 3_665 ?
W5 O2C1 Co1 113.1(5) . . ?
W5 O2C1 Cs5 95.1(4) . . ?
Co1 O2C1 Cs5 140.2(4) . . ?
W7 O2C2 Co2 113.6(5) . . ?
W10 O3C1 Co1 136.8(5) . . ?
W10 O3C1 Cs4 95.1(4) . 4_575 ?
Co1 O3C1 Cs4 123.2(4) . 4_575 ?
W6 O3C2 Co2 112.5(5) . . ?
W6 O4C1 W5 157.4(6) . . ?
W6 O4C1 Cs4 101.2(4) . 2_645 ?
W5 O4C1 Cs4 100.6(4) . 2_645 ?
Co2 O4C2 Co1 128.6(5) . 3_665 ?
Co2 O4C2 Co1 123.1(5) . . ?
Co1 O4C2 Co1 94.6(4) 3_665 . ?
Co2 O5C2 Cs5 102.3(4) . 3_665 ?
W4 O6C1 W5 118.3(5) . . ?
Si1 O1SI Co2 122.5(5) . . ?
Si1 O1SI W6 125.5(5) . . ?
Co2 O1SI W6 91.3(3) . . ?
Si1 O1SI W7 126.3(5) . . ?
Co2 O1SI W7 89.2(3) . . ?
W6 O1SI W7 91.4(3) . . ?
Si1 O2SI W8 125.3(5) . . ?
Si1 O2SI W9 123.5(5) . . ?
W8 O2SI W9 90.1(3) . . ?
Si1 O2SI W10 122.3(5) . . ?
W8 O2SI W10 93.4(3) . . ?
W9 O2SI W10 93.1(3) . . ?
Si1 O3SI Co1 122.0(5) . . ?
Si1 O3SI W5 125.9(5) . . ?
Co1 O3SI W5 89.4(3) . . ?
Si1 O3SI W4 126.9(5) . . ?
Co1 O3SI W4 90.7(3) . . ?
W5 O3SI W4 91.2(3) . . ?
Si1 O4SI W3 124.8(5) . . ?
Si1 O4SI W1 122.3(5) . . ?
W3 O4SI W1 92.0(3) . . ?
Si1 O4SI W2 124.3(5) . . ?
W3 O4SI W2 92.5(3) . . ?
W1 O4SI W2 91.6(3) . . ?
W1 O1T Cs2 103.1(4) . . ?
W1 O1T Cs1 101.6(4) . . ?
Cs2 O1T Cs1 108.2(3) . . ?
W2 O2T Cs3 108.7(4) . 2 ?
W2 O2T Cs2 104.3(4) . 2 ?
Cs3 O2T Cs2 99.6(3) 2 2 ?
W2 O2T Cs5 136.8(4) . 2 ?
Cs3 O2T Cs5 92.2(3) 2 2 ?
Cs2 O2T Cs5 109.0(3) 2 2 ?
W3 O3T Na1 131.1(5) . 2 ?
W3 O3T Cs3 107.3(4) . 1_565 ?
Na1 O3T Cs3 105.2(4) 2 1_565 ?
W3 O3T Cs4 97.6(4) . . ?
Na1 O3T Cs4 96.1(3) 2 . ?
Cs3 O3T Cs4 120.7(3) 1_565 . ?
W4 O4T Na1 144.8(6) . . ?
W4 O4T Cs3 107.4(4) . 2 ?
Na1 O4T Cs3 95.5(3) . 2 ?
W5 O5T Cs2 111.5(5) . . ?
W5 O5T Cs5 109.8(4) . . ?
Cs2 O5T Cs5 124.2(3) . . ?
W5 O5T Cs4 92.0(4) . 2_645 ?
Cs2 O5T Cs4 119.4(3) . 2_645 ?
Cs5 O5T Cs4 94.4(3) . 2_645 ?
W6 O6T Cs3 124.5(5) . 2_655 ?
W6 O6T Cs1 108.8(4) . . ?
Cs3 O6T Cs1 97.0(3) 2_655 . ?
W6 O6T Cs4 91.6(4) . 2_645 ?
Cs3 O6T Cs4 109.5(3) 2_655 2_645 ?
Cs1 O6T Cs4 128.6(3) . 2_645 ?
W7 O7T Cs2 122.1(5) . 2_655 ?
W7 O7T Cs1 105.2(4) . 2_655 ?
Cs2 O7T Cs1 108.8(3) 2_655 2_655 ?
W7 O7T Cs4 98.1(4) . . ?
Cs2 O7T Cs4 107.5(3) 2_655 . ?
Cs1 O7T Cs4 115.2(3) 2_655 . ?
W8 O8T Cs2 108.2(5) . 2 ?
W9 O9T Cs1 108.9(4) . 2_655 ?
W9 O9T Cs3 104.6(4) . 1_565 ?
Cs1 O9T Cs3 93.0(3) 2_655 1_565 ?
W9 O9T Cs5 152.0(5) . 1_565 ?
Cs1 O9T Cs5 94.7(3) 2_655 1_565 ?
Cs3 O9T Cs5 88.4(2) 1_565 1_565 ?
W10 O10T Cs4 110.0(4) . 4_575 ?
W10 O10T Cs5 104.0(4) . 3_665 ?
Cs4 O10T Cs5 106.4(3) 4_575 3_665 ?
W10 O10T Cs1 140.3(5) . 4_575 ?
Cs4 O10T Cs1 96.2(3) 4_575 4_575 ?
Cs5 O10T Cs1 96.0(3) 3_665 4_575 ?
O16 Cs1 O9T 131.7(3) . 2_645 ?
O16 Cs1 O6T 51.5(3) . . ?
O9T Cs1 O6T 82.4(3) 2_645 . ?
O16 Cs1 O11W 112.1(5) . . ?
O9T Cs1 O11W 115.9(5) 2_645 . ?
O6T Cs1 O11W 159.9(5) . . ?
O16 Cs1 O12W 163.0(6) . 2_645 ?
O9T Cs1 O12W 64.6(6) 2_645 2_645 ?
O6T Cs1 O12W 140.7(6) . 2_645 ?
O11W Cs1 O12W 52.8(7) . 2_645 ?
O16 Cs1 O1T 51.2(3) . . ?
O9T Cs1 O1T 165.3(3) 2_645 . ?
O6T Cs1 O1T 94.6(3) . . ?
O11W Cs1 O1T 65.6(5) . . ?
O12W Cs1 O1T 111.8(6) 2_645 . ?
O16 Cs1 O6W 77.9(3) . . ?
O9T Cs1 O6W 68.1(3) 2_645 . ?
O6T Cs1 O6W 63.7(3) . . ?
O11W Cs1 O6W 129.3(5) . . ?
O12W Cs1 O6W 117.1(6) 2_645 . ?
O1T Cs1 O6W 123.4(3) . . ?
O16 Cs1 O10T 110.0(2) . 4_676 ?
O9T Cs1 O10T 82.5(2) 2_645 4_676 ?
O6T Cs1 O10T 124.3(3) . 4_676 ?
O11W Cs1 O10T 69.4(5) . 4_676 ?
O12W Cs1 O10T 73.9(6) 2_645 4_676 ?
O1T Cs1 O10T 110.8(3) . 4_676 ?
O6W Cs1 O10T 60.9(3) . 4_676 ?
O16 Cs1 O79 119.3(2) . 2_645 ?
O9T Cs1 O79 51.5(2) 2_645 2_645 ?
O6T Cs1 O79 78.3(2) . 2_645 ?
O11W Cs1 O79 105.7(5) . 2_645 ?
O12W Cs1 O79 64.7(6) 2_645 2_645 ?
O1T Cs1 O79 113.8(2) . 2_645 ?
O6W Cs1 O79 111.6(3) . 2_645 ?
O10T Cs1 O79 127.4(2) 4_676 2_645 ?
O16 Cs1 O7T 74.6(2) . 2_645 ?
O9T Cs1 O7T 97.3(2) 2_645 2_645 ?
O6T Cs1 O7T 61.4(3) . 2_645 ?
O11W Cs1 O7T 105.6(5) . 2_645 ?
O12W Cs1 O7T 100.7(6) 2_645 2_645 ?
O1T Cs1 O7T 68.9(2) . 2_645 ?
O6W Cs1 O7T 124.5(3) . 2_645 ?
O10T Cs1 O7T 174.1(3) 4_676 2_645 ?
O79 Cs1 O7T 49.9(2) 2_645 2_645 ?
O16 Cs1 O13W 138.6(6) . . ?
O9T Cs1 O13W 80.0(6) 2_645 . ?
O6T Cs1 O13W 130.5(7) . . ?
O11W Cs1 O13W 51.1(8) . . ?
O1T Cs1 O13W 91.3(6) . . ?
O6W Cs1 O13W 143.4(6) . . ?
O10T Cs1 O13W 98.6(7) 4_676 . ?
O79 Cs1 O13W 54.8(7) 2_645 . ?
O7T Cs1 O13W 75.6(7) 2_645 . ?
O16 Cs1 W1 26.89(18) . . ?
O9T Cs1 W1 157.93(19) 2_645 . ?
O6T Cs1 W1 75.63(18) . . ?
O11W Cs1 W1 86.2(5) . . ?
O12W Cs1 W1 136.2(5) 2_645 . ?
O1T Cs1 W1 24.95(19) . . ?
O6W Cs1 W1 99.8(2) . . ?
O10T Cs1 W1 108.42(17) 4_676 . ?
O79 Cs1 W1 123.79(16) 2_645 . ?
O7T Cs1 W1 73.86(16) 2_645 . ?
O13W Cs1 W1 115.9(6) . . ?
O5T Cs2 O5W 109.6(3) . . ?
O5T Cs2 O8T 162.4(3) . 2_545 ?
O5W Cs2 O8T 68.6(3) . 2_545 ?
O5T Cs2 O7T 72.1(3) . 2_645 ?
O5W Cs2 O7T 82.6(3) . 2_645 ?
O8T Cs2 O7T 123.7(3) 2_545 2_645 ?
O5T Cs2 O15 54.0(3) . . ?
O5W Cs2 O15 159.5(3) . . ?
O8T Cs2 O15 131.0(3) 2_545 . ?
O7T Cs2 O15 80.4(3) 2_645 . ?
O5T Cs2 O7W 84.5(3) . 2 ?
O5W Cs2 O7W 137.7(3) . 2 ?
O8T Cs2 O7W 86.1(3) 2_545 2 ?
O7T Cs2 O7W 139.1(3) 2_645 2 ?
O15 Cs2 O7W 58.8(3) . 2 ?
O5T Cs2 O1T 100.3(3) . . ?
O5W Cs2 O1T 132.1(3) . . ?
O8T Cs2 O1T 92.7(3) 2_545 . ?
O7T Cs2 O1T 72.0(3) 2_645 . ?
O15 Cs2 O1T 51.4(3) . . ?
O7W Cs2 O1T 80.2(3) 2 . ?
O5T Cs2 O28 109.8(3) . 2_545 ?
O5W Cs2 O28 78.7(3) . 2_545 ?
O8T Cs2 O28 52.7(3) 2_545 2_545 ?
O7T Cs2 O28 160.7(2) 2_645 2_545 ?
O15 Cs2 O28 116.8(2) . 2_545 ?
O7W Cs2 O28 59.0(2) 2 2_545 ?
O1T Cs2 O28 125.0(3) . 2_545 ?
O5T Cs2 O2T 65.2(3) . 2_545 ?
O5W Cs2 O2T 73.6(3) . 2_545 ?
O8T Cs2 O2T 98.2(3) 2_545 2_545 ?
O7T Cs2 O2T 119.0(2) 2_645 2_545 ?
O15 Cs2 O2T 105.2(2) . 2_545 ?
O7W Cs2 O2T 77.4(2) 2 2_545 ?
O1T Cs2 O2T 154.3(2) . 2_545 ?
O28 Cs2 O2T 50.5(2) 2_545 2_545 ?
O5T Cs2 O10W 146.0(4) . . ?
O5W Cs2 O10W 99.5(4) . . ?
O8T Cs2 O10W 47.3(4) 2_545 . ?
O7T Cs2 O10W 95.4(4) 2_645 . ?
O15 Cs2 O10W 93.3(4) . . ?
O7W Cs2 O10W 85.6(4) 2 . ?
O1T Cs2 O10W 45.9(4) . . ?
O28 Cs2 O10W 92.5(4) 2_545 . ?
O2T Cs2 O10W 142.8(4) 2_545 . ?
O5T Cs2 W8 138.3(2) . 2_545 ?
O5W Cs2 W8 74.4(2) . 2_545 ?
O8T Cs2 W8 24.39(19) 2_545 2_545 ?
O7T Cs2 W8 146.72(19) 2_645 2_545 ?
O15 Cs2 W8 125.78(18) . 2_545 ?
O7W Cs2 W8 69.63(18) 2 2_545 ?
O1T Cs2 W8 106.55(19) . 2_545 ?
O28 Cs2 W8 28.64(18) 2_545 2_545 ?
O2T Cs2 W8 77.21(17) 2_545 2_545 ?
O10W Cs2 W8 65.9(3) . 2_545 ?
O5T Cs2 W1 78.4(2) . . ?
O5W Cs2 W1 153.6(2) . . ?
O8T Cs2 W1 111.30(19) 2_545 . ?
O7T Cs2 W1 76.00(18) 2_645 . ?
O15 Cs2 W1 26.66(18) . . ?
O7W Cs2 W1 66.60(18) 2 . ?
O1T Cs2 W1 24.84(19) . . ?
O28 Cs2 W1 123.33(17) 2_545 . ?
O2T Cs2 W1 130.65(17) 2_545 . ?
O10W Cs2 W1 67.8(4) . . ?
W8 Cs2 W1 117.11(3) 2_545 . ?
O2T Cs3 O3T 159.1(3) 2_545 1_545 ?
O2T Cs3 O6T 131.7(3) 2_545 2_645 ?
O3T Cs3 O6T 67.3(3) 1_545 2_645 ?
O2T Cs3 O5W 77.9(3) 2_545 . ?
O3T Cs3 O5W 100.1(3) 1_545 . ?
O6T Cs3 O5W 80.6(3) 2_645 . ?
O2T Cs3 O39 128.6(3) 2_545 1_545 ?
O3T Cs3 O39 54.4(3) 1_545 1_545 ?
O6T Cs3 O39 81.8(2) 2_645 1_545 ?
O5W Cs3 O39 153.3(3) . 1_545 ?
O2T Cs3 O6W 68.2(3) 2_545 2_645 ?
O3T Cs3 O6W 132.1(3) 1_545 2_645 ?
O6T Cs3 O6W 65.1(3) 2_645 2_645 ?
O5W Cs3 O6W 77.2(3) . 2_645 ?
O39 Cs3 O6W 112.8(3) 1_545 2_645 ?
O2T Cs3 O7W 84.1(3) 2_545 . ?
O3T Cs3 O7W 82.3(3) 1_545 . ?
O6T Cs3 O7W 139.2(3) 2_645 . ?
O5W Cs3 O7W 133.0(3) . . ?
O39 Cs3 O7W 58.1(2) 1_545 . ?
O6W Cs3 O7W 134.2(3) 2_645 . ?
O2T Cs3 O24 52.9(2) 2_545 2_545 ?
O3T Cs3 O24 106.2(3) 1_545 2_545 ?
O6T Cs3 O24 155.3(3) 2_645 2_545 ?
O5W Cs3 O24 77.2(3) . 2_545 ?
O39 Cs3 O24 114.6(2) 1_545 2_545 ?
O6W Cs3 O24 119.2(3) 2_645 2_545 ?
O7W Cs3 O24 57.6(2) . 2_545 ?
O2T Cs3 O9T 92.0(3) 2_545 1_545 ?
O3T Cs3 O9T 101.0(3) 1_545 1_545 ?
O6T Cs3 O9T 80.5(3) 2_645 1_545 ?
O5W Cs3 O9T 143.5(3) . 1_545 ?
O39 Cs3 O9T 50.9(2) 1_545 1_545 ?
O6W Cs3 O9T 66.5(3) 2_645 1_545 ?
O7W Cs3 O9T 79.4(2) . 1_545 ?
O24 Cs3 O9T 124.0(2) 2_545 1_545 ?
O2T Cs3 O4T 97.1(3) 2_545 2_545 ?
O3T Cs3 O4T 64.2(3) 1_545 2_545 ?
O6T Cs3 O4T 110.8(2) 2_645 2_545 ?
O5W Cs3 O4T 63.4(3) . 2_545 ?
O39 Cs3 O4T 105.2(2) 1_545 2_545 ?
O6W Cs3 O4T 140.2(3) 2_645 2_545 ?
O7W Cs3 O4T 76.5(2) . 2_545 ?
O24 Cs3 O4T 48.8(2) 2_545 2_545 ?
O9T Cs3 O4T 153.1(2) 1_545 2_545 ?
O2T Cs3 W2 24.81(19) 2_545 2_545 ?
O3T Cs3 W2 134.30(19) 1_545 2_545 ?
O6T Cs3 W2 152.95(19) 2_645 2_545 ?
O5W Cs3 W2 79.3(2) . 2_545 ?
O39 Cs3 W2 122.96(16) 1_545 2_545 ?
O6W Cs3 W2 92.8(2) 2_645 2_545 ?
O7W Cs3 W2 67.38(17) . 2_545 ?
O24 Cs3 W2 28.46(16) 2_545 2_545 ?
O9T Cs3 W2 105.72(17) 1_545 2_545 ?
O4T Cs3 W2 75.60(16) 2_545 2_545 ?
O2T Cs3 W3 151.48(18) 2_545 1_545 ?
O3T Cs3 W3 25.28(19) 1_545 1_545 ?
O6T Cs3 W3 73.40(18) 2_645 1_545 ?
O5W Cs3 W3 125.2(2) . 1_545 ?
O39 Cs3 W3 29.14(17) 1_545 1_545 ?
O6W Cs3 W3 128.4(2) 2_645 1_545 ?
O7W Cs3 W3 67.92(17) . 1_545 ?
O24 Cs3 W3 111.41(16) 2_545 1_545 ?
O9T Cs3 W3 77.98(17) 1_545 1_545 ?
O4T Cs3 W3 82.11(16) 2_545 1_545 ?
W2 Cs3 W3 133.45(3) 2_545 1_545 ?
O10T Cs4 O4C1 114.6(3) 4_676 2_655 ?
O10T Cs4 O37 123.7(3) 4_676 . ?
O4C1 Cs4 O37 109.2(3) 2_655 . ?
O10T Cs4 O3T 131.8(3) 4_676 . ?
O4C1 Cs4 O3T 109.7(3) 2_655 . ?
O37 Cs4 O3T 52.6(3) . . ?
O10T Cs4 O3W 74.8(3) 4_676 2 ?
O4C1 Cs4 O3W 143.2(3) 2_655 2 ?
O37 Cs4 O3W 90.6(3) . 2 ?
O3T Cs4 O3W 58.2(3) . 2 ?
O10T Cs4 O3C1 50.8(3) 4_676 4_676 ?
O4C1 Cs4 O3C1 88.1(2) 2_655 4_676 ?
O37 Cs4 O3C1 160.9(2) . 4_676 ?
O3T Cs4 O3C1 114.7(2) . 4_676 ?
O3W Cs4 O3C1 70.4(3) 2 4_676 ?
O10T Cs4 O5T 79.7(3) 4_676 2_655 ?
O4C1 Cs4 O5T 51.7(3) 2_655 2_655 ?
O37 Cs4 O5T 102.8(2) . 2_655 ?
O3T Cs4 O5T 146.2(3) . 2_655 ?
O3W Cs4 O5T 154.5(3) 2 2_655 ?
O3C1 Cs4 O5T 94.3(2) 4_676 2_655 ?
O10T Cs4 O6T 165.4(2) 4_676 2_655 ?
O4C1 Cs4 O6T 50.9(2) 2_655 2_655 ?
O37 Cs4 O6T 68.4(2) . 2_655 ?
O3T Cs4 O6T 61.0(2) . 2_655 ?
O3W Cs4 O6T 115.3(3) 2 2_655 ?
O3C1 Cs4 O6T 120.7(2) 4_676 2_655 ?
O5T Cs4 O6T 90.0(2) 2_655 2_655 ?
O10T Cs4 O6W 61.3(3) 4_676 . ?
O4C1 Cs4 O6W 98.1(3) 2_655 . ?
O37 Cs4 O6W 79.4(3) . . ?
O3T Cs4 O6W 129.8(3) . . ?
O3W Cs4 O6W 116.4(3) 2 . ?
O3C1 Cs4 O6W 107.0(3) 4_676 . ?
O5T Cs4 O6W 47.3(3) 2_655 . ?
O6T Cs4 O6W 118.2(3) 2_655 . ?
O10T Cs4 O13 94.3(2) 4_676 . ?
O4C1 Cs4 O13 150.6(2) 2_655 . ?
O37 Cs4 O13 45.1(2) . . ?
O3T Cs4 O13 46.3(2) . . ?
O3W Cs4 O13 47.2(3) 2 . ?
O3C1 Cs4 O13 115.9(2) 4_676 . ?
O5T Cs4 O13 135.5(2) 2_655 . ?
O6T Cs4 O13 100.2(2) 2_655 . ?
O6W Cs4 O13 91.1(2) . . ?
O10T Cs4 O7T 125.8(2) 4_676 . ?
O4C1 Cs4 O7T 68.4(2) 2_655 . ?
O37 Cs4 O7T 46.5(2) . . ?
O3T Cs4 O7T 87.5(2) . . ?
O3W Cs4 O7T 137.1(3) 2 . ?
O3C1 Cs4 O7T 152.6(2) 4_676 . ?
O5T Cs4 O7T 60.3(2) 2_655 . ?
O6T Cs4 O7T 54.7(2) 2_655 . ?
O6W Cs4 O7T 64.6(2) . . ?
O13 Cs4 O7T 90.9(2) . . ?
O10T Cs4 W3 123.80(19) 4_676 . ?
O4C1 Cs4 W3 121.15(18) 2_655 . ?
O37 Cs4 W3 28.69(17) . . ?
O3T Cs4 W3 26.90(18) . . ?
O3W Cs4 W3 65.5(3) 2 . ?
O3C1 Cs4 W3 134.20(17) 4_676 . ?
O5T Cs4 W3 131.30(18) 2_655 . ?
O6T Cs4 W3 70.76(16) 2_655 . ?
O6W Cs4 W3 102.93(19) . . ?
O13 Cs4 W3 29.55(14) . . ?
O7T Cs4 W3 72.48(15) . . ?
O13W Cs5 O10T 83.8(7) 4_565 3_665 ?
O13W Cs5 O1C2 55.6(7) 4_565 3_665 ?
O10T Cs5 O1C2 51.3(3) 3_665 3_665 ?
O13W Cs5 O8W 77.0(7) 4_565 4_565 ?
O10T Cs5 O8W 138.0(3) 3_665 4_565 ?
O1C2 Cs5 O8W 131.9(3) 3_665 4_565 ?
O13W Cs5 O6W 132.7(7) 4_565 2_645 ?
O10T Cs5 O6W 62.5(3) 3_665 2_645 ?
O1C2 Cs5 O6W 112.2(3) 3_665 2_645 ?
O8W Cs5 O6W 105.6(3) 4_565 2_645 ?
O13W Cs5 O5T 157.0(7) 4_565 . ?
O10T Cs5 O5T 79.5(3) 3_665 . ?
O1C2 Cs5 O5T 101.5(3) 3_665 . ?
O8W Cs5 O5T 125.8(3) 4_565 . ?
O6W Cs5 O5T 50.0(3) 2_645 . ?
O13W Cs5 O5C2 74.9(7) 4_565 3_665 ?
O10T Cs5 O5C2 100.4(3) 3_665 3_665 ?
O1C2 Cs5 O5C2 53.7(3) 3_665 3_665 ?
O8W Cs5 O5C2 109.9(3) 4_565 3_665 ?
O6W Cs5 O5C2 139.6(3) 2_645 3_665 ?
O5T Cs5 O5C2 92.7(3) . 3_665 ?
O13W Cs5 O9T 77.3(7) 4_565 1_545 ?
O10T Cs5 O9T 80.6(2) 3_665 1_545 ?
O1C2 Cs5 O9T 112.0(2) 3_665 1_545 ?
O8W Cs5 O9T 59.0(3) 4_565 1_545 ?
O6W Cs5 O9T 65.8(3) 2_645 1_545 ?
O5T Cs5 O9T 114.9(2) . 1_545 ?
O5C2 Cs5 O9T 151.9(3) 3_665 1_545 ?
O13W Cs5 O1W 109.0(7) 4_565 . ?
O10T Cs5 O1W 146.9(3) 3_665 . ?
O1C2 Cs5 O1W 110.3(3) 3_665 . ?
O8W Cs5 O1W 75.2(3) 4_565 . ?
O6W Cs5 O1W 117.4(3) 2_645 . ?
O5T Cs5 O1W 78.3(3) . . ?
O5C2 Cs5 O1W 56.7(3) 3_665 . ?
O9T Cs5 O1W 131.4(2) 1_545 . ?
O13W Cs5 O2T 142.2(7) 4_565 2_545 ?
O10T Cs5 O2T 124.3(2) 3_665 2_545 ?
O1C2 Cs5 O2T 161.3(2) 3_665 2_545 ?
O8W Cs5 O2T 65.1(3) 4_565 2_545 ?
O6W Cs5 O2T 62.1(3) 2_645 2_545 ?
O5T Cs5 O2T 60.7(2) . 2_545 ?
O5C2 Cs5 O2T 117.7(2) 3_665 2_545 ?
O9T Cs5 O2T 82.7(2) 1_545 2_545 ?
O1W Cs5 O2T 62.8(2) . 2_545 ?
O13W Cs5 O2C1 114.2(7) 4_565 . ?
O10T Cs5 O2C1 70.8(2) 3_665 . ?
O1C2 Cs5 O2C1 61.3(2) 3_665 . ?
O8W Cs5 O2C1 151.2(3) 4_565 . ?
O6W Cs5 O2C1 86.4(2) 2_645 . ?
O5T Cs5 O2C1 45.1(2) . . ?
O5C2 Cs5 O2C1 53.2(2) 3_665 . ?
O9T Cs5 O2C1 147.2(2) 1_545 . ?
O1W Cs5 O2C1 76.1(2) . . ?
O2T Cs5 O2C1 100.0(2) 2_545 . ?
O13W Cs5 O9W 64.0(8) 4_565 4_565 ?
O10T Cs5 O9W 139.4(5) 3_665 4_565 ?
O1C2 Cs5 O9W 89.0(5) 3_665 4_565 ?
O8W Cs5 O9W 60.3(5) 4_565 4_565 ?
O6W Cs5 O9W 158.0(5) 2_645 4_565 ?
O5T Cs5 O9W 122.1(5) . 4_565 ?
O5C2 Cs5 O9W 49.7(5) 3_665 4_565 ?
O9T Cs5 O9W 112.9(5) 1_545 4_565 ?
O1W Cs5 O9W 45.4(5) . 4_565 ?
O2T Cs5 O9W 95.9(5) 2_545 4_565 ?
O2C1 Cs5 O9W 99.5(5) . 4_565 ?
O4W Na1 O3W 98.1(5) . . ?
O4W Na1 O4T 85.3(4) . . ?
O3W Na1 O4T 173.9(6) . . ?
O4W Na1 O2W 88.8(5) . . ?
O3W Na1 O2W 88.5(5) . . ?
O4T Na1 O2W 96.6(4) . . ?
O4W Na1 O3T 90.9(4) . 2_545 ?
O3W Na1 O3T 82.6(5) . 2_545 ?
O4T Na1 O3T 92.3(4) . 2_545 ?
O2W Na1 O3T 171.0(5) . 2_545 ?
O4W Na1 O1W 167.2(5) . . ?
O3W Na1 O1W 94.5(5) . . ?
O4T Na1 O1W 82.0(4) . . ?
O2W Na1 O1W 94.2(5) . . ?
O3T Na1 O1W 88.2(4) 2_545 . ?
O4W Na1 Cs4 64.5(3) . 2_545 ?
O3W Na1 Cs4 51.9(4) . 2_545 ?
O4T Na1 Cs4 126.4(3) . 2_545 ?
O2W Na1 Cs4 123.9(3) . 2_545 ?
O3T Na1 Cs4 48.4(2) 2_545 2_545 ?
O1W Na1 Cs4 122.8(3) . 2_545 ?
O4W Na1 Cs3 77.7(4) . 2 ?
O3W Na1 Cs3 123.4(5) . 2 ?
O4T Na1 Cs3 52.3(3) . 2 ?
O2W Na1 Cs3 146.5(4) . 2 ?
O3T Na1 Cs3 41.7(2) 2_545 2 ?
O1W Na1 Cs3 93.2(3) . 2 ?
Cs4 Na1 Cs3 77.53(10) 2_545 2 ?
O10W Na2 O11W 85.6(9) . . ?
O10W Na2 O8W 161.3(9) . . ?
O11W Na2 O8W 100.5(9) . . ?
O10W Na2 O10W 76.7(10) . 3_666 ?
O11W Na2 O10W 97.6(9) . 3_666 ?
O8W Na2 O10W 85.0(7) . 3_666 ?
O10W Na2 O9W 92.2(10) . . ?
O11W Na2 O9W 139.1(11) . . ?
O8W Na2 O9W 94.4(9) . . ?
O10W Na2 O9W 121.6(10) 3_666 . ?
O10W Na2 Na2 39.6(6) . 3_666 ?
O11W Na2 Na2 92.3(8) . 3_666 ?
O8W Na2 Na2 121.9(7) . 3_666 ?
O10W Na2 Na2 37.1(6) 3_666 3_666 ?
O9W Na2 Na2 111.6(8) . 3_666 ?
O10W Na2 Cs5 145.7(7) . 4_666 ?
O11W Na2 Cs5 98.0(7) . 4_666 ?
O8W Na2 Cs5 51.4(4) . 4_666 ?
O10W Na2 Cs5 135.6(7) 3_666 4_666 ?
O9W Na2 Cs5 63.0(7) . 4_666 ?
Na2 Na2 Cs5 168.7(6) 3_666 4_666 ?
O10W Na2 Cs1 74.2(6) . . ?
O11W Na2 Cs1 30.7(7) . . ?
O8W Na2 Cs1 119.4(5) . . ?
O10W Na2 Cs1 120.8(7) 3_666 . ?
O9W Na2 Cs1 109.9(8) . . ?
Na2 Na2 Cs1 99.6(4) 3_666 . ?
Cs5 Na2 Cs1 91.7(2) 4_666 . ?
Na1 O1W Cs5 152.9(5) . . ?
Na1 O3W Cs4 94.7(5) . 2_545 ?
Cs2 O5W Cs3 102.7(4) . . ?
Cs3 O6W Cs5 92.5(3) 2_655 2_655 ?
Cs3 O6W Cs1 92.3(3) 2_655 . ?
Cs5 O6W Cs1 94.6(3) 2_655 . ?
Cs3 O6W Cs4 172.7(4) 2_655 . ?
Cs5 O6W Cs4 94.8(3) 2_655 . ?
Cs1 O6W Cs4 87.9(3) . . ?
Cs2 O7W Cs3 177.0(4) 2_545 . ?
Na2 O8W Cs5 94.1(5) . 4_666 ?
Na2 O9W Cs5 81.1(8) . 4_666 ?
Na2 O10W Na2 103.3(10) . 3_666 ?
Na2 O10W Cs2 123.8(9) . . ?
Na2 O10W Cs2 131.8(8) 3_666 . ?
Na2 O11W Cs1 127.6(10) . . ?
Cs1 O12W Cs5 139.4(9) 2_655 3_665 ?
Cs5 O13W Cs1 165.8(13) 4_666 . ?


_shelxl_version_number           2014/6

####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_try
_database_code_depnum_ccdc_archive 'CCDC 2013549'
loop_
_audit_author_name
_audit_author_address
'Bassem S Bassil'
;University of Balamand
Lebanon
;
_audit_update_record             
;
2021-01-20 deposited with the CCDC.	2021-01-26 downloaded from the CCDC.
;

_audit_creation_method           SHELXL-2014/6
_chemical_name_systematic        ?
_chemical_name_common            ?
_chemical_melting_point          ?
_chemical_formula_moiety         ?
_chemical_formula_sum            'Cs10 H29 Na2 Ni4 O98 Si2 W20'
_chemical_formula_weight         6940.33

loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Na Na 0.0362 0.0249 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Si Si 0.0817 0.0704 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ni Ni 0.3393 1.1124 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Cs Cs -0.3680 2.1192 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
W W -0.8490 6.8722 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_space_group_crystal_system      monoclinic
_space_group_IT_number           14
_space_group_name_H-M_alt        'P 21/n'
_space_group_name_Hall           '-P 2yn'

_shelx_space_group_comment       
; 
The symmetry employed for this shelxl refinement is uniquely defined 
by the following loop, which should always be used as a source of 
symmetry information in preference to the above space-group names. 
They are only intended as comments. 
;

loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x+1/2, y+1/2, -z+1/2'
'-x, -y, -z'
'x-1/2, -y-1/2, z-1/2'

_cell_length_a                   13.0666(5)
_cell_length_b                   15.6924(6)
_cell_length_c                   23.7612(9)
_cell_angle_alpha                90
_cell_angle_beta                 100.454(3)
_cell_angle_gamma                90
_cell_volume                     4791.3(3)
_cell_formula_units_Z            2
_cell_measurement_temperature    100(2)
_cell_measurement_reflns_used    5297
_cell_measurement_theta_min      3.30
_cell_measurement_theta_max      25.05

_exptl_crystal_description       plate
_exptl_crystal_colour            green
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    ?
_exptl_crystal_density_diffrn    4.811
_exptl_crystal_F_000             6010
_exptl_transmission_factor_min   0.208
_exptl_transmission_factor_max   0.279
_exptl_crystal_size_max          0.080
_exptl_crystal_size_mid          0.060
_exptl_crystal_size_min          0.060
_exptl_absorpt_coefficient_mu    28.558
_shelx_estimated_absorpt_T_min   0.208
_shelx_estimated_absorpt_T_max   0.279
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_correction_T_min  0.208
_exptl_absorpt_correction_T_max  0.279
_exptl_absorpt_process_details   SADABS
_exptl_absorpt_special_details   ?
_diffrn_ambient_temperature      100(2)
_diffrn_radiation_wavelength     0.71073
_diffrn_radiation_type           MoK\a
_diffrn_source                   ?
_diffrn_measurement_device_type  'Bruker APEX-II CCD'
_diffrn_measurement_method       'φ and ω scans'
_diffrn_detector_area_resol_mean ?
_diffrn_reflns_number            38995
_diffrn_reflns_av_unetI/netI     0.0863
_diffrn_reflns_av_R_equivalents  0.0934
_diffrn_reflns_limit_h_min       -15
_diffrn_reflns_limit_h_max       15
_diffrn_reflns_limit_k_min       -18
_diffrn_reflns_limit_k_max       18
_diffrn_reflns_limit_l_min       -28
_diffrn_reflns_limit_l_max       28
_diffrn_reflns_theta_min         3.426
_diffrn_reflns_theta_max         25.027
_diffrn_reflns_theta_full        25.242
_diffrn_measured_fraction_theta_max 0.995
_diffrn_measured_fraction_theta_full 0.969
_diffrn_reflns_Laue_measured_fraction_max 0.995
_diffrn_reflns_Laue_measured_fraction_full 0.969
_diffrn_reflns_point_group_measured_fraction_max 0.995
_diffrn_reflns_point_group_measured_fraction_full 0.969
_reflns_number_total             8421
_reflns_number_gt                5871
_reflns_threshold_expression     'I > 2σ(I)'
_reflns_Friedel_coverage         0.000
_reflns_Friedel_fraction_max     .
_reflns_Friedel_fraction_full    .

_reflns_special_details          
; 
 Reflections were merged by SHELXL according to the crystal 
 class for the calculation of statistics and refinement. 
  
 _reflns_Friedel_fraction is defined as the number of unique 
 Friedel pairs measured divided by the number that would be 
 possible theoretically, ignoring centric projections and 
 systematic absences. 
;

_computing_data_collection       'Bruker APEX2'
_computing_cell_refinement       'Bruker SAINT'
_computing_data_reduction        'Bruker SAINT'
_computing_structure_solution    'SHELXS-97 (Sheldrick 2008)'
_computing_structure_refinement  'SHELXL-2014/6 (Sheldrick, 2014)'
_computing_molecular_graphics    'Bruker SHELXTL'
_computing_publication_material  'Bruker SHELXTL'
_refine_special_details          ?
_refine_ls_structure_factor_coef Fsqd
_refine_ls_matrix_type           full
_refine_ls_weighting_scheme      calc
_refine_ls_weighting_details     
'w=1/[σ²(Fo²)+(0.0630P)²+230.0000P] where P=(Fo²+2Fc²)/3'
_atom_sites_solution_primary     ?
_atom_sites_solution_secondary   ?
_atom_sites_solution_hydrogens   .
_refine_ls_hydrogen_treatment    undef
_refine_ls_extinction_method     none
_refine_ls_extinction_coef       .
_refine_ls_number_reflns         8421
_refine_ls_number_parameters     376
_refine_ls_number_restraints     0
_refine_ls_R_factor_all          0.0903
_refine_ls_R_factor_gt           0.0531
_refine_ls_wR_factor_ref         0.1438
_refine_ls_wR_factor_gt          0.1266
_refine_ls_goodness_of_fit_ref   1.007
_refine_ls_restrained_S_all      1.007
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_diff_density_max         2.988
_refine_diff_density_min         -4.156
_refine_diff_density_rms         0.520

loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
W1 W -0.22094(7) 0.81625(6) 0.23601(4) 0.0161(2) Uani 1 1 d . . . A 1
W2 W 0.00784(7) 0.91459(6) 0.28421(4) 0.0184(2) Uani 1 1 d . . . A 1
W3 W 0.00091(7) 0.70248(6) 0.26547(4) 0.0167(2) Uani 1 1 d . . . A 1
W4 W -0.26425(7) 0.96146(6) 0.10913(4) 0.0162(2) Uani 1 1 d . . . A 1
W5 W -0.03848(7) 1.05879(6) 0.15713(4) 0.0180(2) Uani 1 1 d . . . A 1
W6 W 0.20772(7) 0.92865(6) 0.19099(4) 0.0175(2) Uani 1 1 d . . . A 1
W7 W 0.20085(7) 0.71695(6) 0.17140(4) 0.0162(2) Uani 1 1 d . . . A 1
W8 W -0.05437(7) 0.61068(6) 0.11917(4) 0.0175(2) Uani 1 1 d . . . A 1
W9 W -0.27243(7) 0.72586(6) 0.08892(4) 0.0173(2) Uani 1 1 d . . . A 1
W10 W -0.08724(7) 0.74971(7) 0.00456(4) 0.0222(2) Uani 1 1 d . . . A 1
Si1 Si -0.0373(4) 0.8344(4) 0.1441(3) 0.0135(13) Uani 1 1 d . . . A 1
Ni1 Ni -0.0812(2) 0.97275(19) 0.03334(14) 0.0188(7) Uani 1 1 d . . . A 1
Ni2 Ni 0.15263(19) 0.84606(18) 0.06417(13) 0.0149(7) Uani 1 1 d . . . A 1
O1NI O -0.0745(11) 1.0448(9) -0.0374(7) 0.018(3) Uiso 1 1 d . . . A 1
O1SI O -0.0562(11) 0.8197(9) 0.2100(7) 0.014(3) Uiso 1 1 d . . . A 1
O1T O -0.3287(12) 0.8090(10) 0.2668(7) 0.024(4) Uiso 1 1 d . . . A 1
O2SI O -0.0881(10) 0.9238(9) 0.1209(6) 0.014(3) Uiso 1 1 d . . . A 1
O2T O 0.0455(13) 0.9712(11) 0.3473(8) 0.028(4) Uiso 1 1 d . . . A 1
O3T O 0.0327(11) 0.6232(10) 0.3165(7) 0.019(4) Uiso 1 1 d . . . A 1
O3SI O 0.0870(11) 0.8332(9) 0.1432(7) 0.017(3) Uiso 1 1 d . . . A 1
O4A O -0.2346(12) 0.9952(10) 0.0416(7) 0.023(4) Uiso 1 1 d . . . A 1
O4T O -0.3894(12) 1.0004(10) 0.1045(7) 0.023(4) Uiso 1 1 d . . . A 1
O4SI O -0.0958(11) 0.7568(10) 0.1031(7) 0.019(4) Uiso 1 1 d . . . A 1
O5 O -0.0426(11) 1.0800(10) 0.0838(7) 0.018(3) Uiso 1 1 d . . . A 1
O5T O -0.0146(13) 1.1614(11) 0.1851(8) 0.028(4) Uiso 1 1 d . . . A 1
O6T O 0.3064(11) 0.9900(10) 0.2295(7) 0.019(4) Uiso 1 1 d . . . A 1
O6A O 0.2466(12) 0.9248(10) 0.1217(7) 0.022(4) Uiso 1 1 d . . . A 1
O7T O 0.2923(12) 0.6433(10) 0.1969(7) 0.025(4) Uiso 1 1 d . . . A 1
O7A O 0.2394(12) 0.7466(10) 0.1045(7) 0.023(4) Uiso 1 1 d . . . A 1
O8T O -0.0387(12) 0.5020(10) 0.1246(7) 0.023(4) Uiso 1 1 d . . . A 1
O9T O -0.4000(12) 0.6914(10) 0.0734(7) 0.023(4) Uiso 1 1 d . . . A 1
O10A O -0.1270(11) 0.8575(10) -0.0046(7) 0.020(4) Uiso 1 1 d . . . A 1
O10T O -0.1067(12) 0.7110(10) -0.0655(7) 0.025(4) Uiso 1 1 d . . . A 1
O10B O 0.0487(11) 0.7673(10) 0.0220(7) 0.020(4) Uiso 1 1 d . . . A 1
O12 O -0.1358(11) 0.8853(10) 0.2908(7) 0.020(4) Uiso 1 1 d . . . A 1
O13 O -0.1439(12) 0.7194(10) 0.2731(7) 0.021(4) Uiso 1 1 d . . . A 1
O14 O -0.2514(11) 0.9079(9) 0.1859(7) 0.016(3) Uiso 1 1 d . . . A 1
O19 O -0.2565(11) 0.7438(10) 0.1706(7) 0.018(3) Uiso 1 1 d . . . A 1
O23 O 0.0361(12) 0.7986(10) 0.3156(7) 0.020(4) Uiso 1 1 d . . . A 1
O25 O -0.0418(11) 0.9981(10) 0.2325(7) 0.020(4) Uiso 1 1 d . . . A 1
O26 O 0.1315(11) 0.9077(10) 0.2549(7) 0.020(4) Uiso 1 1 d . . . A 1
O37 O 0.1244(12) 0.7152(10) 0.2357(7) 0.022(4) Uiso 1 1 d . . . A 1
O38 O -0.0550(11) 0.6375(10) 0.1986(7) 0.021(4) Uiso 1 1 d . . . A 1
O45 O -0.1889(12) 1.0563(10) 0.1495(7) 0.021(4) Uiso 1 1 d . . . A 1
O49 O -0.2924(12) 0.8456(10) 0.0828(7) 0.022(4) Uiso 1 1 d . . . A 1
O56 O 0.1001(11) 1.0112(10) 0.1677(7) 0.019(4) Uiso 1 1 d . . . A 1
O67 O 0.2658(11) 0.8168(10) 0.2096(7) 0.019(4) Uiso 1 1 d . . . A 1
O78 O 0.0887(11) 0.6481(10) 0.1361(7) 0.018(4) Uiso 1 1 d . . . A 1
O89 O -0.2015(11) 0.6181(10) 0.1087(7) 0.021(4) Uiso 1 1 d . . . A 1
O810 O -0.0617(11) 0.6276(10) 0.0409(7) 0.018(4) Uiso 1 1 d . . . A 1
O910 O -0.2374(11) 0.7199(10) 0.0160(7) 0.021(4) Uiso 1 1 d . . . A 1
Cs1 Cs 0.29968(12) 0.96075(11) 0.36233(7) 0.0289(4) Uani 1 1 d . . . A 1
Cs2 Cs 0.12217(13) 0.69844(12) -0.09223(8) 0.0365(4) Uani 1 1 d . . . A 1
Cs3 Cs 0.27296(12) 0.66729(11) 0.35151(8) 0.0317(4) Uani 1 1 d . . . A 1
Cs4 Cs -0.47610(13) 0.66286(13) 0.18653(9) 0.0403(5) Uani 1 1 d . . . A 1
Cs5 Cs -0.04033(15) 0.46008(13) 0.26181(11) 0.0502(6) Uani 1 1 d . . . A 1
Na1 Na -0.4980(8) 1.1191(7) 0.0836(4) 0.032(2) Uani 1 1 d . . . A 1
O1W O 0.2377(12) 0.8446(10) 0.0011(7) 0.024(4) Uiso 1 1 d . . . A 1
O2W O -0.2548(12) 0.5614(11) 0.2288(7) 0.027(4) Uiso 1 1 d . . . A 1
O3W O -0.1649(13) 0.6957(11) 0.3846(8) 0.033(4) Uiso 1 1 d . . . B 1
O4W O 0.4251(14) 0.8203(12) 0.2991(8) 0.036(5) Uiso 1 1 d . . . A 1
O5W O -0.545(2) 0.8423(17) 0.1392(12) 0.077(8) Uiso 1 1 d . . . A 1
O6W O -0.5168(16) 0.8764(14) 0.0183(10) 0.051(6) Uiso 1 1 d . . . C 1
O7W O -0.2872(18) 0.4510(15) 0.1172(11) 0.063(7) Uiso 1 1 d . . . D 1
O8W O -0.3642(17) 0.9727(14) -0.0629(10) 0.055(6) Uiso 1 1 d . . . E 1
O9W O 0.0936(18) 0.7479(16) 0.4282(11) 0.066(7) Uiso 1 1 d . . . A 1
O10W O -0.294(2) 0.551(2) -0.0229(14) 0.023(8) Uiso 0.5 1 d . . P F 1
O11W O -0.482(3) 0.431(3) 0.0340(19) 0.051(11) Uiso 0.5 1 d . . P G 1
O12W O 0.094(4) 0.528(3) 0.013(2) 0.067(14) Uiso 0.5 1 d . . P A 1
O13W O 0.165(4) 0.602(3) 0.021(2) 0.072(15) Uiso 0.5 1 d . . P H 2


_geom_special_details            
; 
 All esds (except the esd in the dihedral angle between two l.s. planes) 
 are estimated using the full covariance matrix.  The cell esds are taken 
 into account individually in the estimation of esds in distances, angles 
 and torsion angles; correlations between esds in cell parameters are only 
 used when they are defined by crystal symmetry.  An approximate (isotropic) 
 treatment of cell esds is used for estimating esds involving l.s. planes. 
;

loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
W1 O1T 1.705(16) . ?
W1 O14 1.864(15) . ?
W1 O12 1.893(15) . ?
W1 O19 1.913(16) . ?
W1 O13 1.944(16) . ?
W1 O1SI 2.345(14) . ?
W2 O2T 1.735(18) . ?
W2 O25 1.832(16) . ?
W2 O26 1.875(15) . ?
W2 O12 1.965(15) . ?
W2 O23 1.977(16) . ?
W2 O1SI 2.343(15) . ?
W2 Cs1 3.9929(17) . ?
W2 Cs4 3.992(2) 2_455 ?
W3 O3T 1.734(16) . ?
W3 O37 1.886(16) . ?
W3 O38 1.918(16) . ?
W3 O23 1.924(16) . ?
W3 O13 1.951(15) . ?
W3 O1SI 2.306(15) . ?
W4 O4T 1.731(15) . ?
W4 O4A 1.799(17) . ?
W4 O45 1.940(16) . ?
W4 O49 1.937(16) . ?
W4 O14 1.987(15) . ?
W4 O2SI 2.344(14) . ?
W5 O5T 1.748(17) . ?
W5 O5 1.765(16) . ?
W5 O45 1.941(15) . ?
W5 O56 1.932(15) . ?
W5 O25 2.036(16) . ?
W5 O2SI 2.334(14) . ?
W6 O6T 1.731(15) . ?
W6 O6A 1.810(17) . ?
W6 O56 1.919(15) . ?
W6 O67 1.932(15) . ?
W6 O26 1.989(16) . ?
W6 O3SI 2.317(15) . ?
W7 O7T 1.694(16) . ?
W7 O7A 1.814(17) . ?
W7 O78 1.890(15) . ?
W7 O67 1.929(15) . ?
W7 O37 1.971(16) . ?
W7 O3SI 2.372(15) . ?
W8 O8T 1.720(16) . ?
W8 O810 1.864(16) . ?
W8 O89 1.897(15) . ?
W8 O78 1.931(14) . ?
W8 O38 1.935(16) . ?
W8 O4SI 2.371(15) . ?
W9 O9T 1.728(15) . ?
W9 O910 1.873(17) . ?
W9 O49 1.899(16) . ?
W9 O19 1.936(16) . ?
W9 O89 1.944(16) . ?
W9 O4SI 2.323(14) . ?
W10 O10T 1.746(17) . ?
W10 O10A 1.772(16) . ?
W10 O10B 1.770(15) . ?
W10 O910 2.083(15) . ?
W10 O810 2.103(15) . ?
W10 O4SI 2.367(16) . ?
Si1 O2SI 1.605(15) . ?
Si1 O3SI 1.629(15) . ?
Si1 O1SI 1.646(16) . ?
Si1 O4SI 1.657(16) . ?
Ni1 O1NI 2.037(15) 3_575 ?
Ni1 O1NI 2.041(16) . ?
Ni1 O5 2.074(15) . ?
Ni1 O10A 2.060(16) . ?
Ni1 O4A 2.079(16) . ?
Ni1 O2SI 2.235(15) . ?
Ni1 Ni1 2.994(6) 3_575 ?
Ni2 O10B 1.971(15) . ?
Ni2 O1W 2.021(17) . ?
Ni2 O1NI 2.036(15) 3_575 ?
Ni2 O7A 2.060(16) . ?
Ni2 O6A 2.072(16) . ?
Ni2 O3SI 2.211(16) . ?
Ni2 Cs2 4.336(4) . ?
O1NI Ni1 2.037(15) 3_575 ?
O1NI Ni2 2.036(15) 3_575 ?
O1T Cs5 2.931(16) 2_455 ?
O1T Cs4 3.358(16) . ?
O1T Cs2 3.524(17) 4_576 ?
O2T Cs4 3.201(17) 2_455 ?
O2T Cs1 3.279(16) . ?
O3T Na1 2.50(2) 2_445 ?
O3T Cs5 2.949(16) . ?
O3T Cs3 3.175(15) . ?
O4T Na1 2.340(19) . ?
O4T Cs5 3.519(17) 2_455 ?
O5 Cs2 3.645(15) 3_575 ?
O5T Cs4 3.074(18) 2_455 ?
O5T Cs2 3.249(17) 3_575 ?
O5T Cs3 3.426(17) 2 ?
O6T Cs5 3.062(15) 2 ?
O6T Cs1 3.206(16) . ?
O6T Cs3 3.435(15) 2 ?
O7T Cs4 3.096(16) 1_655 ?
O7T Cs1 3.318(16) 2_545 ?
O7T Cs3 3.747(18) . ?
O8T Cs1 3.150(15) 2_545 ?
O8T Cs5 3.329(17) . ?
O8T Cs2 3.371(16) 3_565 ?
O9T Cs4 3.062(17) . ?
O10A Cs3 3.453(16) 4_575 ?
O10T Cs3 2.981(16) 4_575 ?
O10T Cs2 3.175(16) . ?
O10T Cs1 3.308(16) 4_575 ?
O10B Cs2 3.226(16) . ?
O14 Cs5 3.294(15) 2_455 ?
O19 Cs4 3.222(15) . ?
O23 Cs3 3.687(15) . ?
O25 Cs4 3.206(16) 2_455 ?
O26 Cs1 3.163(15) . ?
O37 Cs3 3.158(16) . ?
O38 Cs5 3.152(16) . ?
O56 Cs3 3.039(15) 2 ?
O78 Cs1 3.279(15) 2_545 ?
Cs1 O8T 3.150(15) 2 ?
Cs1 O10W 3.19(3) 4_676 ?
Cs1 O12W 3.22(5) 2 ?
Cs1 O4W 3.270(19) . ?
Cs1 O78 3.279(15) 2 ?
Cs1 O10T 3.308(16) 4_676 ?
Cs1 O7T 3.318(16) 2 ?
Cs2 O5T 3.249(17) 3_575 ?
Cs2 O7W 3.31(2) 3_565 ?
Cs2 O4W 3.313(19) 4_575 ?
Cs2 O1W 3.354(16) . ?
Cs2 O8T 3.371(16) 3_565 ?
Cs2 O3W 3.370(18) 4_675 ?
Cs2 O1T 3.524(17) 4_675 ?
Cs2 O5 3.645(15) 3_575 ?
Cs2 O12W 3.72(5) . ?
Cs3 O10T 2.981(17) 4_676 ?
Cs3 O56 3.039(15) 2_545 ?
Cs3 O5T 3.426(17) 2_545 ?
Cs3 O6T 3.435(16) 2_545 ?
Cs3 O10A 3.453(16) 4_676 ?
Cs3 O4W 3.488(19) . ?
Cs3 O9W 3.46(2) . ?
Cs3 O8W 3.67(2) 4_676 ?
Cs4 O5T 3.074(18) 2_445 ?
Cs4 O7T 3.096(16) 1_455 ?
Cs4 O5W 3.11(3) . ?
Cs4 O25 3.206(16) 2_445 ?
Cs4 O2T 3.201(17) 2_445 ?
Cs4 O2W 3.294(16) . ?
Cs5 O1T 2.931(16) 2_445 ?
Cs5 O6T 3.063(15) 2_545 ?
Cs5 O5W 3.04(3) 2_445 ?
Cs5 O4W 3.157(19) 2_545 ?
Cs5 O2W 3.193(16) . ?
Cs5 O14 3.294(15) 2_445 ?
Cs5 O4T 3.519(17) 2_445 ?
Na1 O8W 2.29(2) 3_475 ?
Na1 O9W 2.37(3) 2_455 ?
Na1 O3W 2.44(2) 2_455 ?
Na1 O6W 2.47(2) 3_475 ?
Na1 O3T 2.50(2) 2_455 ?
Na1 Cs3 4.227(11) 2_455 ?
Na1 Cs5 4.394(11) 2_455 ?
O3W Na1 2.44(2) 2_445 ?
O3W Cs2 3.370(18) 4_576 ?
O4W Cs5 3.157(19) 2 ?
O4W Cs2 3.313(19) 4_676 ?
O5W Cs5 3.04(3) 2_455 ?
O6W Na1 2.47(2) 3_475 ?
O7W Cs2 3.31(2) 3_565 ?
O8W Na1 2.29(2) 3_475 ?
O8W Cs3 3.67(2) 4_575 ?
O9W Na1 2.37(3) 2_445 ?
O10W Cs1 3.19(3) 4_575 ?
O12W Cs1 3.22(5) 2_545 ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O1T W1 O14 103.2(7) . . ?
O1T W1 O12 99.9(7) . . ?
O14 W1 O12 91.6(7) . . ?
O1T W1 O19 102.2(7) . . ?
O14 W1 O19 87.0(7) . . ?
O12 W1 O19 157.6(6) . . ?
O1T W1 O13 98.8(7) . . ?
O14 W1 O13 157.8(7) . . ?
O12 W1 O13 86.8(7) . . ?
O19 W1 O13 86.2(6) . . ?
O1T W1 O1SI 169.7(7) . . ?
O14 W1 O1SI 85.1(6) . . ?
O12 W1 O1SI 73.4(6) . . ?
O19 W1 O1SI 84.2(6) . . ?
O13 W1 O1SI 73.3(6) . . ?
O1T W1 Cs5 45.6(5) . 2_455 ?
O14 W1 Cs5 58.5(5) . 2_455 ?
O12 W1 Cs5 91.8(5) . 2_455 ?
O19 W1 Cs5 106.3(4) . 2_455 ?
O13 W1 Cs5 143.6(5) . 2_455 ?
O1SI W1 Cs5 140.6(4) . 2_455 ?
O1T W1 Cs4 52.6(6) . . ?
O14 W1 Cs4 101.6(4) . . ?
O12 W1 Cs4 151.4(5) . . ?
O19 W1 Cs4 49.8(5) . . ?
O13 W1 Cs4 89.9(4) . . ?
O1SI W1 Cs4 132.4(4) . . ?
Cs5 W1 Cs4 74.36(4) 2_455 . ?
O2T W2 O25 102.9(8) . . ?
O2T W2 O26 102.8(7) . . ?
O25 W2 O26 90.9(7) . . ?
O2T W2 O12 100.2(7) . . ?
O25 W2 O12 89.7(7) . . ?
O26 W2 O12 156.3(7) . . ?
O2T W2 O23 98.2(7) . . ?
O25 W2 O23 158.5(7) . . ?
O26 W2 O23 88.4(7) . . ?
O12 W2 O23 82.6(6) . . ?
O2T W2 O1SI 169.1(7) . . ?
O25 W2 O1SI 85.2(6) . . ?
O26 W2 O1SI 84.2(6) . . ?
O12 W2 O1SI 72.3(6) . . ?
O23 W2 O1SI 73.4(6) . . ?
O2T W2 Cs1 53.7(5) . . ?
O25 W2 Cs1 111.9(5) . . ?
O26 W2 Cs1 50.8(5) . . ?
O12 W2 Cs1 148.3(5) . . ?
O23 W2 Cs1 83.9(4) . . ?
O1SI W2 Cs1 130.2(3) . . ?
O2T W2 Cs4 51.1(6) . 2_455 ?
O25 W2 Cs4 52.0(5) . 2_455 ?
O26 W2 Cs4 104.1(5) . 2_455 ?
O12 W2 Cs4 94.8(5) . 2_455 ?
O23 W2 Cs4 148.4(5) . 2_455 ?
O1SI W2 Cs4 135.8(4) . 2_455 ?
Cs1 W2 Cs4 82.10(4) . 2_455 ?
O3T W3 O37 103.1(7) . . ?
O3T W3 O38 101.8(7) . . ?
O37 W3 O38 88.2(7) . . ?
O3T W3 O23 97.5(7) . . ?
O37 W3 O23 91.4(7) . . ?
O38 W3 O23 160.3(7) . . ?
O3T W3 O13 98.4(7) . . ?
O37 W3 O13 158.5(7) . . ?
O38 W3 O13 85.4(7) . . ?
O23 W3 O13 87.8(7) . . ?
O3T W3 O1SI 169.5(6) . . ?
O37 W3 O1SI 84.9(6) . . ?
O38 W3 O1SI 85.2(6) . . ?
O23 W3 O1SI 75.2(6) . . ?
O13 W3 O1SI 74.1(6) . . ?
O3T W3 Cs3 55.9(5) . . ?
O37 W3 Cs3 55.8(5) . . ?
O38 W3 Cs3 123.1(5) . . ?
O23 W3 Cs3 71.7(4) . . ?
O13 W3 Cs3 142.8(5) . . ?
O1SI W3 Cs3 126.6(3) . . ?
O3T W3 Cs5 47.2(5) . . ?
O37 W3 Cs5 102.9(5) . . ?
O38 W3 Cs5 54.8(5) . . ?
O23 W3 Cs5 143.8(5) . . ?
O13 W3 Cs5 90.2(5) . . ?
O1SI W3 Cs5 138.4(4) . . ?
Cs3 W3 Cs5 88.97(4) . . ?
O4T W4 O4A 101.2(7) . . ?
O4T W4 O45 98.6(7) . . ?
O4A W4 O45 92.5(7) . . ?
O4T W4 O49 100.9(7) . . ?
O4A W4 O49 92.7(7) . . ?
O45 W4 O49 158.4(6) . . ?
O4T W4 O14 97.4(7) . . ?
O4A W4 O14 161.4(6) . . ?
O45 W4 O14 85.3(6) . . ?
O49 W4 O14 83.1(7) . . ?
O4T W4 O2SI 173.2(6) . . ?
O4A W4 O2SI 79.3(6) . . ?
O45 W4 O2SI 74.7(6) . . ?
O49 W4 O2SI 85.8(6) . . ?
O14 W4 O2SI 82.3(6) . . ?
O4T W4 Cs5 51.3(6) . 2_455 ?
O4A W4 Cs5 152.1(5) . 2_455 ?
O45 W4 Cs5 88.0(5) . 2_455 ?
O49 W4 Cs5 97.0(5) . 2_455 ?
O14 W4 Cs5 46.4(4) . 2_455 ?
O2SI W4 Cs5 127.3(4) . 2_455 ?
O5T W5 O5 100.0(8) . . ?
O5T W5 O45 99.3(7) . . ?
O5 W5 O45 93.6(7) . . ?
O5T W5 O56 102.0(7) . . ?
O5 W5 O56 93.5(7) . . ?
O45 W5 O56 156.0(6) . . ?
O5T W5 O25 97.3(7) . . ?
O5 W5 O25 162.7(7) . . ?
O45 W5 O25 83.7(6) . . ?
O56 W5 O25 82.7(6) . . ?
O5T W5 O2SI 174.1(6) . . ?
O5 W5 O2SI 81.4(6) . . ?
O45 W5 O2SI 74.8(6) . . ?
O56 W5 O2SI 83.6(6) . . ?
O25 W5 O2SI 81.4(6) . . ?
O5T W5 Cs3 61.3(6) . 2 ?
O5 W5 Cs3 74.6(5) . 2 ?
O45 W5 Cs3 154.0(5) . 2 ?
O56 W5 Cs3 49.8(5) . 2 ?
O25 W5 Cs3 114.3(4) . 2 ?
O2SI W5 Cs3 124.5(3) . 2 ?
O5T W5 Cs4 45.6(6) . 2_455 ?
O5 W5 Cs4 145.2(5) . 2_455 ?
O45 W5 Cs4 88.4(5) . 2_455 ?
O56 W5 Cs4 98.6(5) . 2_455 ?
O25 W5 Cs4 52.0(4) . 2_455 ?
O2SI W5 Cs4 132.2(4) . 2_455 ?
Cs3 W5 Cs4 88.73(4) 2 2_455 ?
O5T W5 Cs2 47.0(6) . 3_575 ?
O5 W5 Cs2 60.3(5) . 3_575 ?
O45 W5 Cs2 78.0(5) . 3_575 ?
O56 W5 Cs2 125.2(5) . 3_575 ?
O25 W5 Cs2 134.8(4) . 3_575 ?
O2SI W5 Cs2 130.9(4) . 3_575 ?
Cs3 W5 Cs2 76.03(4) 2 3_575 ?
Cs4 W5 Cs2 86.34(4) 2_455 3_575 ?
O6T W6 O6A 101.2(7) . . ?
O6T W6 O56 102.3(7) . . ?
O6A W6 O56 94.2(7) . . ?
O6T W6 O67 99.2(7) . . ?
O6A W6 O67 90.8(7) . . ?
O56 W6 O67 156.5(6) . . ?
O6T W6 O26 96.7(7) . . ?
O6A W6 O26 162.0(7) . . ?
O56 W6 O26 83.6(7) . . ?
O67 W6 O26 84.6(7) . . ?
O6T W6 O3SI 173.5(6) . . ?
O6A W6 O3SI 79.1(6) . . ?
O56 W6 O3SI 84.1(6) . . ?
O67 W6 O3SI 74.3(6) . . ?
O26 W6 O3SI 82.9(6) . . ?
O6T W6 Cs3 61.7(5) . 2 ?
O6A W6 Cs3 75.8(5) . 2 ?
O56 W6 Cs3 49.8(5) . 2 ?
O67 W6 Cs3 153.0(4) . 2 ?
O26 W6 Cs3 114.9(4) . 2 ?
O3SI W6 Cs3 124.4(4) . 2 ?
O6T W6 Cs1 49.1(5) . . ?
O6A W6 Cs1 146.6(5) . . ?
O56 W6 Cs1 105.8(5) . . ?
O67 W6 Cs1 81.4(5) . . ?
O26 W6 Cs1 49.7(4) . . ?
O3SI W6 Cs1 128.5(4) . . ?
Cs3 W6 Cs1 96.85(4) 2 . ?
O6T W6 Cs5 35.0(5) . 2 ?
O6A W6 Cs5 78.7(5) . 2 ?
O56 W6 Cs5 130.5(4) . 2 ?
O67 W6 Cs5 73.1(4) . 2 ?
O26 W6 Cs5 116.2(4) . 2 ?
O3SI W6 Cs5 139.9(4) . 2 ?
Cs3 W6 Cs5 81.26(4) 2 2 ?
Cs1 W6 Cs5 67.94(4) . 2 ?
O7T W7 O7A 101.4(8) . . ?
O7T W7 O78 102.0(7) . . ?
O7A W7 O78 94.2(7) . . ?
O7T W7 O67 99.5(7) . . ?
O7A W7 O67 92.1(7) . . ?
O78 W7 O67 155.9(6) . . ?
O7T W7 O37 97.9(7) . . ?
O7A W7 O37 160.6(7) . . ?
O78 W7 O37 82.8(7) . . ?
O67 W7 O37 83.6(7) . . ?
O7T W7 O3SI 172.5(7) . . ?
O7A W7 O3SI 79.3(6) . . ?
O78 W7 O3SI 85.3(6) . . ?
O67 W7 O3SI 73.0(6) . . ?
O37 W7 O3SI 81.3(6) . . ?
O7T W7 Cs1 51.4(5) . 2_545 ?
O7A W7 Cs1 94.1(5) . 2_545 ?
O78 W7 Cs1 51.6(4) . 2_545 ?
O67 W7 Cs1 150.9(4) . 2_545 ?
O37 W7 Cs1 98.9(5) . 2_545 ?
O3SI W7 Cs1 136.1(4) . 2_545 ?
O7T W7 Cs4 37.7(6) . 1_655 ?
O7A W7 Cs4 72.3(5) . 1_655 ?
O78 W7 Cs4 126.9(5) . 1_655 ?
O67 W7 Cs4 77.1(4) . 1_655 ?
O37 W7 Cs4 124.5(4) . 1_655 ?
O3SI W7 Cs4 137.6(4) . 1_655 ?
Cs1 W7 Cs4 77.73(4) 2_545 1_655 ?
O7T W7 Cs3 60.4(6) . . ?
O7A W7 Cs3 151.3(5) . . ?
O78 W7 Cs3 110.6(5) . . ?
O67 W7 Cs3 71.3(5) . . ?
O37 W7 Cs3 43.4(4) . . ?
O3SI W7 Cs3 115.8(4) . . ?
Cs1 W7 Cs3 90.52(4) 2_545 . ?
Cs4 W7 Cs3 81.05(4) 1_655 . ?
O8T W8 O810 101.6(7) . . ?
O8T W8 O89 100.1(7) . . ?
O810 W8 O89 89.6(7) . . ?
O8T W8 O78 100.9(7) . . ?
O810 W8 O78 92.1(7) . . ?
O89 W8 O78 158.2(7) . . ?
O8T W8 O38 99.4(7) . . ?
O810 W8 O38 159.0(7) . . ?
O89 W8 O38 86.0(7) . . ?
O78 W8 O38 84.6(7) . . ?
O8T W8 O4SI 172.6(6) . . ?
O810 W8 O4SI 74.5(6) . . ?
O89 W8 O4SI 73.9(6) . . ?
O78 W8 O4SI 85.6(6) . . ?
O38 W8 O4SI 84.6(6) . . ?
O8T W8 Cs1 47.9(5) . 2_545 ?
O810 W8 Cs1 94.8(5) . 2_545 ?
O89 W8 Cs1 147.9(5) . 2_545 ?
O78 W8 Cs1 53.6(4) . 2_545 ?
O38 W8 Cs1 99.8(4) . 2_545 ?
O4SI W8 Cs1 137.8(4) . 2_545 ?
O8T W8 Cs5 51.7(6) . . ?
O810 W8 Cs5 153.1(5) . . ?
O89 W8 Cs5 92.1(5) . . ?
O78 W8 Cs5 96.1(5) . . ?
O38 W8 Cs5 47.8(5) . . ?
O4SI W8 Cs5 131.6(4) . . ?
Cs1 W8 Cs5 70.26(4) 2_545 . ?
O9T W9 O910 100.1(7) . . ?
O9T W9 O49 100.3(7) . . ?
O910 W9 O49 91.8(7) . . ?
O9T W9 O19 100.5(7) . . ?
O910 W9 O19 159.3(6) . . ?
O49 W9 O19 85.5(7) . . ?
O9T W9 O89 100.3(7) . . ?
O910 W9 O89 89.7(7) . . ?
O49 W9 O89 158.7(6) . . ?
O19 W9 O89 85.6(7) . . ?
O9T W9 O4SI 172.6(7) . . ?
O910 W9 O4SI 75.0(6) . . ?
O49 W9 O4SI 85.6(6) . . ?
O19 W9 O4SI 84.3(6) . . ?
O89 W9 O4SI 74.3(6) . . ?
O9T W9 Cs4 47.3(6) . . ?
O910 W9 Cs4 146.3(5) . . ?
O49 W9 Cs4 101.2(5) . . ?
O19 W9 Cs4 53.8(4) . . ?
O89 W9 Cs4 89.0(5) . . ?
O4SI W9 Cs4 136.3(4) . . ?
O10T W10 O10A 103.1(8) . . ?
O10T W10 O10B 104.1(7) . . ?
O10A W10 O10B 98.0(7) . . ?
O10T W10 O910 93.9(7) . . ?
O10A W10 O910 88.2(7) . . ?
O10B W10 O910 159.0(7) . . ?
O10T W10 O810 93.4(7) . . ?
O10A W10 O810 160.3(7) . . ?
O10B W10 O810 88.2(6) . . ?
O910 W10 O810 79.9(6) . . ?
O10T W10 O4SI 159.1(6) . . ?
O10A W10 O4SI 90.7(7) . . ?
O10B W10 O4SI 89.2(6) . . ?
O910 W10 O4SI 70.5(6) . . ?
O810 W10 O4SI 70.7(6) . . ?
O10T W10 Cs2 51.2(5) . . ?
O10A W10 Cs2 109.9(5) . . ?
O10B W10 Cs2 53.0(5) . . ?
O910 W10 Cs2 142.8(4) . . ?
O810 W10 Cs2 88.8(4) . . ?
O4SI W10 Cs2 138.2(4) . . ?
O10T W10 Cs3 43.9(5) . 4_575 ?
O10A W10 Cs3 60.0(5) . 4_575 ?
O10B W10 Cs3 115.9(5) . 4_575 ?
O910 W10 Cs3 84.6(4) . 4_575 ?
O810 W10 Cs3 133.3(4) . 4_575 ?
O4SI W10 Cs3 142.4(4) . 4_575 ?
Cs2 W10 Cs3 77.70(4) . 4_575 ?
O2SI Si1 O3SI 110.9(8) . . ?
O2SI Si1 O1SI 109.0(8) . . ?
O3SI Si1 O1SI 109.4(8) . . ?
O2SI Si1 O4SI 108.8(8) . . ?
O3SI Si1 O4SI 109.8(8) . . ?
O1SI Si1 O4SI 108.9(8) . . ?
O1NI Ni1 O1NI 85.6(6) 3_575 . ?
O1NI Ni1 O5 86.9(6) 3_575 . ?
O1NI Ni1 O5 89.1(6) . . ?
O1NI Ni1 O10A 96.3(6) 3_575 . ?
O1NI Ni1 O10A 100.2(6) . . ?
O5 Ni1 O10A 170.3(6) . . ?
O1NI Ni1 O4A 171.8(7) 3_575 . ?
O1NI Ni1 O4A 99.8(6) . . ?
O5 Ni1 O4A 86.9(6) . . ?
O10A Ni1 O4A 88.9(6) . . ?
O1NI Ni1 O2SI 96.8(6) 3_575 . ?
O1NI Ni1 O2SI 166.5(6) . . ?
O5 Ni1 O2SI 77.8(6) . . ?
O10A Ni1 O2SI 92.8(6) . . ?
O4A Ni1 O2SI 76.6(6) . . ?
O1NI Ni1 Ni1 42.8(4) 3_575 3_575 ?
O1NI Ni1 Ni1 42.7(4) . 3_575 ?
O5 Ni1 Ni1 87.3(4) . 3_575 ?
O10A Ni1 Ni1 101.3(5) . 3_575 ?
O4A Ni1 Ni1 142.1(5) . 3_575 ?
O2SI Ni1 Ni1 138.0(4) . 3_575 ?
O10B Ni2 O1W 92.2(7) . . ?
O10B Ni2 O1NI 96.2(6) . 3_575 ?
O1W Ni2 O1NI 95.2(6) . 3_575 ?
O10B Ni2 O7A 91.8(6) . . ?
O1W Ni2 O7A 90.3(7) . . ?
O1NI Ni2 O7A 170.1(7) 3_575 . ?
O10B Ni2 O6A 168.7(7) . . ?
O1W Ni2 O6A 98.9(6) . . ?
O1NI Ni2 O6A 84.7(6) 3_575 . ?
O7A Ni2 O6A 86.2(6) . . ?
O10B Ni2 O3SI 92.1(6) . . ?
O1W Ni2 O3SI 168.2(6) . . ?
O1NI Ni2 O3SI 95.3(6) 3_575 . ?
O7A Ni2 O3SI 78.6(6) . . ?
O6A Ni2 O3SI 76.6(6) . . ?
O10B Ni2 Cs2 44.1(5) . . ?
O1W Ni2 Cs2 48.4(5) . . ?
O1NI Ni2 Cs2 102.7(5) 3_575 . ?
O7A Ni2 Cs2 87.2(5) . . ?
O6A Ni2 Cs2 146.6(5) . . ?
O3SI Ni2 Cs2 133.6(4) . . ?
Ni1 O1NI Ni2 124.7(8) 3_575 3_575 ?
Ni1 O1NI Ni1 94.4(6) 3_575 . ?
Ni2 O1NI Ni1 129.0(8) 3_575 . ?
Si1 O1SI W3 124.6(8) . . ?
Si1 O1SI W2 122.1(8) . . ?
W3 O1SI W2 92.5(5) . . ?
Si1 O1SI W1 123.8(8) . . ?
W3 O1SI W1 92.8(5) . . ?
W2 O1SI W1 92.1(5) . . ?
W1 O1T Cs5 109.8(7) . 2_455 ?
W1 O1T Cs4 103.6(7) . . ?
Cs5 O1T Cs4 99.8(4) 2_455 . ?
W1 O1T Cs2 135.8(7) . 4_576 ?
Cs5 O1T Cs2 92.8(4) 2_455 4_576 ?
Cs4 O1T Cs2 109.4(4) . 4_576 ?
Si1 O2SI Ni1 122.4(8) . . ?
Si1 O2SI W5 126.6(8) . . ?
Ni1 O2SI W5 88.6(5) . . ?
Si1 O2SI W4 126.7(8) . . ?
Ni1 O2SI W4 90.4(5) . . ?
W5 O2SI W4 90.9(5) . . ?
W2 O2T Cs4 104.0(7) . 2_455 ?
W2 O2T Cs1 101.1(7) . . ?
Cs4 O2T Cs1 108.0(5) 2_455 . ?
W3 O3T Na1 128.4(8) . 2_445 ?
W3 O3T Cs5 107.3(7) . . ?
Na1 O3T Cs5 107.3(6) 2_445 . ?
W3 O3T Cs3 97.3(6) . . ?
Na1 O3T Cs3 95.6(5) 2_445 . ?
Cs5 O3T Cs3 122.0(5) . . ?
Si1 O3SI Ni2 123.4(8) . . ?
Si1 O3SI W6 125.3(9) . . ?
Ni2 O3SI W6 91.3(5) . . ?
Si1 O3SI W7 125.6(8) . . ?
Ni2 O3SI W7 89.4(5) . . ?
W6 O3SI W7 91.3(5) . . ?
W4 O4A Ni1 113.7(8) . . ?
W4 O4T Na1 145.5(9) . . ?
W4 O4T Cs5 106.1(7) . 2_455 ?
Na1 O4T Cs5 95.0(6) . 2_455 ?
Si1 O4SI W9 125.4(8) . . ?
Si1 O4SI W10 121.1(8) . . ?
W9 O4SI W10 94.0(5) . . ?
Si1 O4SI W8 123.3(8) . . ?
W9 O4SI W8 90.7(5) . . ?
W10 O4SI W8 93.6(6) . . ?
W5 O5 Ni1 112.2(8) . . ?
W5 O5 Cs2 94.8(6) . 3_575 ?
Ni1 O5 Cs2 139.8(6) . 3_575 ?
W5 O5T Cs4 110.4(8) . 2_455 ?
W5 O5T Cs2 109.9(7) . 3_575 ?
Cs4 O5T Cs2 125.4(6) 2_455 3_575 ?
W5 O5T Cs3 92.1(6) . 2 ?
Cs4 O5T Cs3 117.1(5) 2_455 2 ?
Cs2 O5T Cs3 96.5(5) 3_575 2 ?
W6 O6T Cs5 126.1(7) . 2 ?
W6 O6T Cs1 106.9(7) . . ?
Cs5 O6T Cs1 96.7(4) 2 . ?
W6 O6T Cs3 92.0(6) . 2 ?
Cs5 O6T Cs3 111.0(5) 2 2 ?
Cs1 O6T Cs3 127.4(5) . 2 ?
W6 O6A Ni2 112.9(8) . . ?
W7 O7T Cs4 122.7(8) . 1_655 ?
W7 O7T Cs1 105.1(7) . 2_545 ?
Cs4 O7T Cs1 109.6(5) 1_655 2_545 ?
W7 O7T Cs3 96.5(7) . . ?
Cs4 O7T Cs3 108.0(4) 1_655 . ?
Cs1 O7T Cs3 114.8(5) 2_545 . ?
W7 O7A Ni2 112.6(8) . . ?
W8 O8T Cs1 108.2(7) . 2_545 ?
W8 O8T Cs5 104.4(7) . . ?
Cs1 O8T Cs5 92.6(4) 2_545 . ?
W8 O8T Cs2 151.5(7) . 3_565 ?
Cs1 O8T Cs2 96.0(4) 2_545 3_565 ?
Cs5 O8T Cs2 88.9(4) . 3_565 ?
W9 O9T Cs4 108.3(7) . . ?
W10 O10A Ni1 136.8(9) . . ?
W10 O10A Cs3 93.7(6) . 4_575 ?
Ni1 O10A Cs3 124.1(6) . 4_575 ?
W10 O10T Cs3 112.1(7) . 4_575 ?
W10 O10T Cs2 103.5(6) . . ?
Cs3 O10T Cs2 108.1(5) 4_575 . ?
W10 O10T Cs1 138.9(8) . 4_575 ?
Cs3 O10T Cs1 94.5(4) 4_575 4_575 ?
Cs2 O10T Cs1 96.8(4) . 4_575 ?
W10 O10B Ni2 141.9(9) . . ?
W10 O10B Cs2 100.9(6) . . ?
Ni2 O10B Cs2 110.8(6) . . ?
W1 O12 W2 122.0(8) . . ?
W1 O13 W3 119.7(8) . . ?
W1 O14 W4 152.3(9) . . ?
W1 O14 Cs5 92.6(5) . 2_455 ?
W4 O14 Cs5 107.6(5) . 2_455 ?
W1 O19 W9 150.1(9) . . ?
W1 O19 Cs4 103.3(6) . . ?
W9 O19 Cs4 97.1(5) . . ?
W3 O23 W2 118.8(8) . . ?
W3 O23 Cs3 78.6(5) . . ?
W2 O23 Cs3 133.9(6) . . ?
W2 O25 W5 149.7(9) . . ?
W2 O25 Cs4 101.3(6) . 2_455 ?
W5 O25 Cs4 98.0(5) . 2_455 ?
W2 O26 W6 149.2(9) . . ?
W2 O26 Cs1 101.8(6) . . ?
W6 O26 Cs1 101.6(5) . . ?
W3 O37 W7 151.7(9) . . ?
W3 O37 Cs3 94.6(6) . . ?
W7 O37 Cs3 111.1(6) . . ?
W3 O38 W8 148.8(9) . . ?
W3 O38 Cs5 95.4(6) . . ?
W8 O38 Cs5 105.2(6) . . ?
W5 O45 W4 118.4(8) . . ?
W9 O49 W4 152.8(9) . . ?
W6 O56 W5 156.8(9) . . ?
W6 O56 Cs3 101.3(6) . 2 ?
W5 O56 Cs3 101.2(6) . 2 ?
W6 O67 W7 120.6(8) . . ?
W7 O78 W8 155.4(9) . . ?
W7 O78 Cs1 101.6(5) . 2_545 ?
W8 O78 Cs1 98.1(5) . 2_545 ?
W8 O89 W9 120.9(8) . . ?
W8 O810 W10 121.0(8) . . ?
W9 O910 W10 120.2(8) . . ?
O8T Cs1 O26 131.7(4) 2 . ?
O8T Cs1 O10W 117.1(6) 2 4_676 ?
O26 Cs1 O10W 110.9(6) . 4_676 ?
O8T Cs1 O6T 82.2(4) 2 . ?
O26 Cs1 O6T 51.8(4) . . ?
O10W Cs1 O6T 158.8(6) 4_676 . ?
O8T Cs1 O12W 65.6(9) 2 2 ?
O26 Cs1 O12W 162.0(9) . 2 ?
O10W Cs1 O12W 53.1(10) 4_676 2 ?
O6T Cs1 O12W 141.0(9) . 2 ?
O8T Cs1 O2T 165.3(4) 2 . ?
O26 Cs1 O2T 51.9(4) . . ?
O10W Cs1 O2T 63.7(6) 4_676 . ?
O6T Cs1 O2T 95.4(4) . . ?
O12W Cs1 O2T 110.1(9) 2 . ?
O8T Cs1 O4W 67.2(4) 2 . ?
O26 Cs1 O4W 77.6(4) . . ?
O10W Cs1 O4W 131.0(7) 4_676 . ?
O6T Cs1 O4W 62.5(4) . . ?
O12W Cs1 O4W 118.4(9) 2 . ?
O2T Cs1 O4W 124.4(4) . . ?
O8T Cs1 O78 52.0(4) 2 2 ?
O26 Cs1 O78 119.2(4) . 2 ?
O10W Cs1 O78 106.3(6) 4_676 2 ?
O6T Cs1 O78 78.0(4) . 2 ?
O12W Cs1 O78 65.1(9) 2 2 ?
O2T Cs1 O78 113.3(4) . 2 ?
O4W Cs1 O78 110.6(4) . 2 ?
O8T Cs1 O10T 81.3(4) 2 4_676 ?
O26 Cs1 O10T 110.0(4) . 4_676 ?
O10W Cs1 O10T 70.9(6) 4_676 4_676 ?
O6T Cs1 O10T 123.6(4) . 4_676 ?
O12W Cs1 O10T 74.3(9) 2 4_676 ?
O2T Cs1 O10T 111.7(4) . 4_676 ?
O4W Cs1 O10T 61.3(5) . 4_676 ?
O78 Cs1 O10T 127.1(4) 2 4_676 ?
O8T Cs1 O7T 98.1(4) 2 2 ?
O26 Cs1 O7T 74.9(4) . 2 ?
O10W Cs1 O7T 104.2(6) 4_676 2 ?
O6T Cs1 O7T 62.1(4) . 2 ?
O12W Cs1 O7T 99.9(9) 2 2 ?
O2T Cs1 O7T 68.2(4) . 2 ?
O4W Cs1 O7T 124.1(5) . 2 ?
O78 Cs1 O7T 50.0(4) 2 2 ?
O10T Cs1 O7T 174.0(4) 4_676 2 ?
O8T Cs1 W2 158.3(3) 2 . ?
O26 Cs1 W2 27.4(3) . . ?
O10W Cs1 W2 84.5(6) 4_676 . ?
O6T Cs1 W2 76.3(3) . . ?
O12W Cs1 W2 134.8(9) 2 . ?
O2T Cs1 W2 25.2(3) . . ?
O4W Cs1 W2 100.4(3) . . ?
O78 Cs1 W2 123.6(3) 2 . ?
O10T Cs1 W2 109.0(3) 4_676 . ?
O7T Cs1 W2 73.6(3) 2 . ?
O8T Cs1 W8 23.9(3) 2 2 ?
O26 Cs1 W8 132.9(3) . 2 ?
O10W Cs1 W8 112.2(6) 4_676 2 ?
O6T Cs1 W8 81.6(3) . 2 ?
O12W Cs1 W8 59.9(9) 2 2 ?
O2T Cs1 W8 141.4(3) . 2 ?
O4W Cs1 W8 88.3(3) . 2 ?
O78 Cs1 W8 28.3(3) 2 2 ?
O10T Cs1 W8 101.5(3) 4_676 2 ?
O7T Cs1 W8 76.8(3) 2 2 ?
W2 Cs1 W8 148.86(5) . 2 ?
O10T Cs2 O10B 51.3(4) . . ?
O10T Cs2 O5T 77.7(4) . 3_575 ?
O10B Cs2 O5T 100.8(4) . 3_575 ?
O10T Cs2 O7W 138.4(5) . 3_565 ?
O10B Cs2 O7W 133.7(5) . 3_565 ?
O5T Cs2 O7W 125.0(5) 3_575 3_565 ?
O10T Cs2 O4W 62.2(5) . 4_575 ?
O10B Cs2 O4W 112.2(4) . 4_575 ?
O5T Cs2 O4W 49.6(4) 3_575 4_575 ?
O7W Cs2 O4W 103.7(5) 3_565 4_575 ?
O10T Cs2 O1W 98.8(4) . . ?
O10B Cs2 O1W 51.8(4) . . ?
O5T Cs2 O1W 94.2(4) 3_575 . ?
O7W Cs2 O1W 111.9(5) 3_565 . ?
O4W Cs2 O1W 140.3(4) 4_575 . ?
O10T Cs2 O8T 80.0(4) . 3_565 ?
O10B Cs2 O8T 111.8(4) . 3_565 ?
O5T Cs2 O8T 113.2(4) 3_575 3_565 ?
O7W Cs2 O8T 59.5(5) 3_565 3_565 ?
O4W Cs2 O8T 64.3(4) 4_575 3_565 ?
O1W Cs2 O8T 151.3(4) . 3_565 ?
O10T Cs2 O3W 146.9(4) . 4_675 ?
O10B Cs2 O3W 110.7(4) . 4_675 ?
O5T Cs2 O3W 79.8(4) 3_575 4_675 ?
O7W Cs2 O3W 74.7(5) 3_565 4_675 ?
O4W Cs2 O3W 117.7(5) 4_575 4_675 ?
O1W Cs2 O3W 59.0(4) . 4_675 ?
O8T Cs2 O3W 131.7(4) 3_565 4_675 ?
O10T Cs2 O1T 122.2(4) . 4_675 ?
O10B Cs2 O1T 160.8(4) . 4_675 ?
O5T Cs2 O1T 60.5(4) 3_575 4_675 ?
O7W Cs2 O1T 64.5(5) 3_565 4_675 ?
O4W Cs2 O1T 60.4(4) 4_575 4_675 ?
O1W Cs2 O1T 120.9(4) . 4_675 ?
O8T Cs2 O1T 81.9(4) 3_565 4_675 ?
O3W Cs2 O1T 64.1(4) 4_675 4_675 ?
O10T Cs2 O5 69.0(4) . 3_575 ?
O10B Cs2 O5 60.2(4) . 3_575 ?
O5T Cs2 O5 45.5(4) 3_575 3_575 ?
O7W Cs2 O5 152.5(5) 3_565 3_575 ?
O4W Cs2 O5 86.5(4) 4_575 3_575 ?
O1W Cs2 O5 53.8(4) . 3_575 ?
O8T Cs2 O5 145.0(3) 3_565 3_575 ?
O3W Cs2 O5 77.9(4) 4_675 3_575 ?
O1T Cs2 O5 100.8(4) 4_675 3_575 ?
O10T Cs2 O12W 72.4(8) . . ?
O10B Cs2 O12W 66.2(8) . . ?
O5T Cs2 O12W 149.1(8) 3_575 . ?
O7W Cs2 O12W 76.0(9) 3_565 . ?
O4W Cs2 O12W 107.4(8) 4_575 . ?
O1W Cs2 O12W 97.9(8) . . ?
O8T Cs2 O12W 54.1(8) 3_565 . ?
O3W Cs2 O12W 130.5(8) 4_675 . ?
O1T Cs2 O12W 132.0(8) 4_675 . ?
O5 Cs2 O12W 125.8(8) 3_575 . ?
O10T Cs2 W10 25.4(3) . . ?
O10B Cs2 W10 26.0(3) . . ?
O5T Cs2 W10 89.9(3) 3_575 . ?
O7W Cs2 W10 142.0(4) 3_565 . ?
O4W Cs2 W10 87.1(3) 4_575 . ?
O1W Cs2 W10 75.7(3) . . ?
O8T Cs2 W10 95.3(3) 3_565 . ?
O3W Cs2 W10 132.2(3) 4_675 . ?
O1T Cs2 W10 145.3(3) 4_675 . ?
O5 Cs2 W10 62.7(2) 3_575 . ?
O12W Cs2 W10 66.1(8) . . ?
O10T Cs3 O56 112.3(4) 4_676 2_545 ?
O10T Cs3 O37 126.2(4) 4_676 . ?
O56 Cs3 O37 109.1(4) 2_545 . ?
O10T Cs3 O3T 133.7(4) 4_676 . ?
O56 Cs3 O3T 109.0(4) 2_545 . ?
O37 Cs3 O3T 53.2(4) . . ?
O10T Cs3 O5T 77.6(4) 4_676 2_545 ?
O56 Cs3 O5T 52.1(4) 2_545 2_545 ?
O37 Cs3 O5T 103.6(4) . 2_545 ?
O3T Cs3 O5T 147.2(4) . 2_545 ?
O10T Cs3 O6T 163.6(4) 4_676 2_545 ?
O56 Cs3 O6T 51.7(4) 2_545 2_545 ?
O37 Cs3 O6T 68.2(4) . 2_545 ?
O3T Cs3 O6T 59.5(4) . 2_545 ?
O5T Cs3 O6T 92.0(4) 2_545 2_545 ?
O10T Cs3 O10A 50.0(4) 4_676 4_676 ?
O56 Cs3 O10A 86.5(4) 2_545 4_676 ?
O37 Cs3 O10A 162.2(4) . 4_676 ?
O3T Cs3 O10A 114.4(4) . 4_676 ?
O5T Cs3 O10A 92.7(4) 2_545 4_676 ?
O6T Cs3 O10A 119.0(4) 2_545 4_676 ?
O10T Cs3 O4W 61.9(5) 4_676 . ?
O56 Cs3 O4W 98.0(4) 2_545 . ?
O37 Cs3 O4W 79.9(4) . . ?
O3T Cs3 O4W 131.1(4) . . ?
O5T Cs3 O4W 46.9(4) 2_545 . ?
O6T Cs3 O4W 119.4(4) 2_545 . ?
O10A Cs3 O4W 107.1(4) 4_676 . ?
O10T Cs3 O9W 75.1(5) 4_676 . ?
O56 Cs3 O9W 144.5(5) 2_545 . ?
O37 Cs3 O9W 90.2(5) . . ?
O3T Cs3 O9W 59.0(5) . . ?
O5T Cs3 O9W 152.6(5) 2_545 . ?
O6T Cs3 O9W 115.3(5) 2_545 . ?
O10A Cs3 O9W 72.0(5) 4_676 . ?
O4W Cs3 O9W 114.9(5) . . ?
O10T Cs3 O23 96.6(4) 4_676 . ?
O56 Cs3 O23 150.9(4) 2_545 . ?
O37 Cs3 O23 46.2(4) . . ?
O3T Cs3 O23 46.6(4) . . ?
O5T Cs3 O23 136.9(4) 2_545 . ?
O6T Cs3 O23 99.6(3) 2_545 . ?
O10A Cs3 O23 116.3(4) 4_676 . ?
O4W Cs3 O23 92.4(4) . . ?
O9W Cs3 O23 45.3(5) . . ?
O10T Cs3 O8W 105.6(5) 4_676 4_676 ?
O56 Cs3 O8W 86.3(5) 2_545 4_676 ?
O37 Cs3 O8W 109.9(5) . 4_676 ?
O3T Cs3 O8W 57.0(5) . 4_676 ?
O5T Cs3 O8W 133.6(4) 2_545 4_676 ?
O6T Cs3 O8W 72.4(4) 2_545 4_676 ?
O10A Cs3 O8W 61.3(4) 4_676 4_676 ?
O4W Cs3 O8W 167.5(5) . 4_676 ?
O9W Cs3 O8W 58.8(5) . 4_676 ?
O23 Cs3 O8W 89.4(4) . 4_676 ?
O10T Cs3 O7T 126.3(4) 4_676 . ?
O56 Cs3 O7T 68.6(4) 2_545 . ?
O37 Cs3 O7T 46.3(4) . . ?
O3T Cs3 O7T 87.7(4) . . ?
O5T Cs3 O7T 61.2(4) 2_545 . ?
O6T Cs3 O7T 55.7(4) 2_545 . ?
O10A Cs3 O7T 151.5(4) 4_676 . ?
O4W Cs3 O7T 64.8(4) . . ?
O9W Cs3 O7T 136.6(5) . . ?
O23 Cs3 O7T 91.8(4) . . ?
O8W Cs3 O7T 127.5(4) 4_676 . ?
O9T Cs4 O5T 161.6(4) . 2_445 ?
O9T Cs4 O7T 124.2(4) . 1_455 ?
O5T Cs4 O7T 72.9(4) 2_445 1_455 ?
O9T Cs4 O5W 70.7(6) . . ?
O5T Cs4 O5W 107.8(6) 2_445 . ?
O7T Cs4 O5W 83.9(6) 1_455 . ?
O9T Cs4 O25 130.1(4) . 2_445 ?
O5T Cs4 O25 53.9(4) 2_445 2_445 ?
O7T Cs4 O25 80.7(4) 1_455 2_445 ?
O5W Cs4 O25 159.0(6) . 2_445 ?
O9T Cs4 O2T 92.3(4) . 2_445 ?
O5T Cs4 O2T 100.5(5) 2_445 2_445 ?
O7T Cs4 O2T 71.9(4) 1_455 2_445 ?
O5W Cs4 O2T 135.2(6) . 2_445 ?
O25 Cs4 O2T 51.6(4) 2_445 2_445 ?
O9T Cs4 O19 53.3(4) . . ?
O5T Cs4 O19 108.4(4) 2_445 . ?
O7T Cs4 O19 162.3(4) 1_455 . ?
O5W Cs4 O19 78.9(6) . . ?
O25 Cs4 O19 114.8(4) 2_445 . ?
O2T Cs4 O19 124.0(4) 2_445 . ?
O9T Cs4 O2W 86.1(4) . . ?
O5T Cs4 O2W 83.4(4) 2_445 . ?
O7T Cs4 O2W 138.1(4) 1_455 . ?
O5W Cs4 O2W 136.9(6) . . ?
O25 Cs4 O2W 57.5(4) 2_445 . ?
O2T Cs4 O2W 79.4(4) 2_445 . ?
O19 Cs4 O2W 58.3(4) . . ?
O9T Cs4 O1T 98.9(4) . . ?
O5T Cs4 O1T 64.1(4) 2_445 . ?
O7T Cs4 O1T 119.4(4) 1_455 . ?
O5W Cs4 O1T 71.7(6) . . ?
O25 Cs4 O1T 103.8(4) 2_445 . ?
O2T Cs4 O1T 153.1(4) 2_445 . ?
O19 Cs4 O1T 50.7(4) . . ?
O2W Cs4 O1T 77.0(4) . . ?
O9T Cs4 W9 24.5(3) . . ?
O5T Cs4 W9 137.3(3) 2_445 . ?
O7T Cs4 W9 147.4(3) 1_455 . ?
O5W Cs4 W9 75.1(5) . . ?
O25 Cs4 W9 124.7(3) 2_445 . ?
O2T Cs4 W9 106.1(3) 2_445 . ?
O19 Cs4 W9 29.0(3) . . ?
O2W Cs4 W9 69.7(3) . . ?
O1T Cs4 W9 77.6(3) . . ?
O9T Cs4 W2 110.9(3) . 2_445 ?
O5T Cs4 W2 78.2(3) 2_445 2_445 ?
O7T Cs4 W2 75.8(3) 1_455 2_445 ?
O5W Cs4 W2 156.3(5) . 2_445 ?
O25 Cs4 W2 26.7(3) 2_445 2_445 ?
O2T Cs4 W2 24.9(3) 2_445 2_445 ?
O19 Cs4 W2 121.9(3) . 2_445 ?
O2W Cs4 W2 65.7(3) . 2_445 ?
O1T Cs4 W2 129.4(3) . 2_445 ?
W9 Cs4 W2 116.60(5) . 2_445 ?
O9T Cs4 W5 154.1(3) . 2_445 ?
O5T Cs4 W5 24.0(3) 2_445 2_445 ?
O7T Cs4 W5 76.7(3) 1_455 2_445 ?
O5W Cs4 W5 131.6(5) . 2_445 ?
O25 Cs4 W5 30.0(3) 2_445 2_445 ?
O2T Cs4 W5 79.3(3) 2_445 2_445 ?
O19 Cs4 W5 111.9(3) . 2_445 ?
O2W Cs4 W5 68.4(3) . 2_445 ?
O1T Cs4 W5 80.0(3) . 2_445 ?
W9 Cs4 W5 135.77(5) . 2_445 ?
W2 Cs4 W5 55.47(3) 2_445 2_445 ?
O1T Cs5 O3T 158.9(5) 2_445 . ?
O1T Cs5 O6T 132.3(4) 2_445 2_545 ?
O3T Cs5 O6T 66.3(4) . 2_545 ?
O1T Cs5 O5W 78.8(6) 2_445 2_445 ?
O3T Cs5 O5W 98.2(6) . 2_445 ?
O6T Cs5 O5W 79.5(6) 2_545 2_445 ?
O1T Cs5 O38 128.4(4) 2_445 . ?
O3T Cs5 O38 55.3(4) . . ?
O6T Cs5 O38 82.6(4) 2_545 . ?
O5W Cs5 O38 152.5(6) 2_445 . ?
O1T Cs5 O4W 68.8(5) 2_445 2_545 ?
O3T Cs5 O4W 131.4(4) . 2_545 ?
O6T Cs5 O4W 65.4(4) 2_545 2_545 ?
O5W Cs5 O4W 78.1(6) 2_445 2_545 ?
O38 Cs5 O4W 112.8(5) . 2_545 ?
O1T Cs5 O2W 84.1(4) 2_445 . ?
O3T Cs5 O2W 82.8(4) . . ?
O6T Cs5 O2W 139.5(4) 2_545 . ?
O5W Cs5 O2W 132.5(6) 2_445 . ?
O38 Cs5 O2W 57.9(4) . . ?
O4W Cs5 O2W 134.7(5) 2_545 . ?
O1T Cs5 O14 53.1(4) 2_445 2_445 ?
O3T Cs5 O14 105.8(4) . 2_445 ?
O6T Cs5 O14 153.6(4) 2_545 2_445 ?
O5W Cs5 O14 76.7(6) 2_445 2_445 ?
O38 Cs5 O14 114.6(4) . 2_445 ?
O4W Cs5 O14 119.7(4) 2_545 2_445 ?
O2W Cs5 O14 57.9(4) . 2_445 ?
O1T Cs5 O8T 92.3(4) 2_445 . ?
O3T Cs5 O8T 101.6(4) . . ?
O6T Cs5 O8T 81.5(4) 2_545 . ?
O5W Cs5 O8T 144.2(6) 2_445 . ?
O38 Cs5 O8T 50.9(4) . . ?
O4W Cs5 O8T 66.4(4) 2_545 . ?
O2W Cs5 O8T 79.8(4) . . ?
O14 Cs5 O8T 124.8(4) 2_445 . ?
O1T Cs5 O4T 96.8(4) 2_445 2_445 ?
O3T Cs5 O4T 64.1(4) . 2_445 ?
O6T Cs5 O4T 109.4(4) 2_545 2_445 ?
O5W Cs5 O4T 62.0(6) 2_445 2_445 ?
O38 Cs5 O4T 105.5(4) . 2_445 ?
O4W Cs5 O4T 139.7(4) 2_545 2_445 ?
O2W Cs5 O4T 76.8(4) . 2_445 ?
O14 Cs5 O4T 48.4(4) 2_445 2_445 ?
O8T Cs5 O4T 153.8(4) . 2_445 ?
O1T Cs5 W3 151.6(3) 2_445 . ?
O3T Cs5 W3 25.5(3) . . ?
O6T Cs5 W3 73.3(3) 2_545 . ?
O5W Cs5 W3 123.6(5) 2_445 . ?
O38 Cs5 W3 29.8(3) . . ?
O4W Cs5 W3 128.5(3) 2_545 . ?
O2W Cs5 W3 68.0(3) . . ?
O14 Cs5 W3 111.1(3) 2_445 . ?
O8T Cs5 W3 78.5(3) . . ?
O4T Cs5 W3 82.0(3) 2_445 . ?
O1T Cs5 W1 24.6(3) 2_445 2_445 ?
O3T Cs5 W1 134.4(3) . 2_445 ?
O6T Cs5 W1 152.7(3) 2_545 2_445 ?
O5W Cs5 W1 79.6(5) 2_445 2_445 ?
O38 Cs5 W1 122.9(3) . 2_445 ?
O4W Cs5 W1 93.1(3) 2_545 2_445 ?
O2W Cs5 W1 67.6(3) . 2_445 ?
O14 Cs5 W1 28.9(3) 2_445 2_445 ?
O8T Cs5 W1 106.1(3) . 2_445 ?
O4T Cs5 W1 75.5(3) 2_445 2_445 ?
W3 Cs5 W1 133.60(6) . 2_445 ?
O8W Na1 O4T 88.1(8) 3_475 . ?
O8W Na1 O9W 97.8(9) 3_475 2_455 ?
O4T Na1 O9W 172.8(9) . 2_455 ?
O8W Na1 O3W 169.7(9) 3_475 2_455 ?
O4T Na1 O3W 82.2(6) . 2_455 ?
O9W Na1 O3W 91.6(8) 2_455 2_455 ?
O8W Na1 O6W 90.4(8) 3_475 3_475 ?
O4T Na1 O6W 94.5(7) . 3_475 ?
O9W Na1 O6W 89.6(9) 2_455 3_475 ?
O3W Na1 O6W 94.0(8) 2_455 3_475 ?
O8W Na1 O3T 87.1(8) 3_475 2_455 ?
O4T Na1 O3T 91.5(6) . 2_455 ?
O9W Na1 O3T 84.7(8) 2_455 2_455 ?
O3W Na1 O3T 89.5(7) 2_455 2_455 ?
O6W Na1 O3T 173.4(7) 3_475 2_455 ?
O8W Na1 Cs3 60.2(6) 3_475 2_455 ?
O4T Na1 Cs3 126.0(5) . 2_455 ?
O9W Na1 Cs3 54.9(6) 2_455 2_455 ?
O3W Na1 Cs3 123.4(6) 2_455 2_455 ?
O6W Na1 Cs3 125.2(6) 3_475 2_455 ?
O3T Na1 Cs3 48.4(4) 2_455 2_455 ?
O8W Na1 Cs5 77.7(6) 3_475 2_455 ?
O4T Na1 Cs5 52.9(5) . 2_455 ?
O9W Na1 Cs5 124.2(7) 2_455 2_455 ?
O3W Na1 Cs5 93.4(5) 2_455 2_455 ?
O6W Na1 Cs5 145.1(6) 3_475 2_455 ?
O3T Na1 Cs5 39.9(4) 2_455 2_455 ?
Cs3 Na1 Cs5 76.82(18) 2_455 2_455 ?
Ni2 O1W Cs2 104.8(6) . . ?
Cs5 O2W Cs4 176.5(6) . . ?
Na1 O3W Cs2 153.0(8) 2_445 4_576 ?
Cs5 O4W Cs1 93.6(5) 2 . ?
Cs5 O4W Cs2 92.9(5) 2 4_676 ?
Cs1 O4W Cs2 94.9(5) . 4_676 ?
Cs5 O4W Cs3 172.9(6) 2 . ?
Cs1 O4W Cs3 86.2(4) . . ?
Cs2 O4W Cs3 94.2(5) 4_676 . ?
Cs5 O5W Cs4 103.2(8) 2_455 . ?
Na1 O8W Cs3 87.1(7) 3_475 4_575 ?
Na1 O9W Cs3 91.1(8) 2_445 . ?
Cs1 O12W Cs2 140.7(15) 2_545 . ?


_shelxl_version_number           2014/6

####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_lzg_CCDC1
_database_code_depnum_ccdc_archive 'CCDC 2013550'
loop_
_audit_author_name
_audit_author_address
'Bassem S Bassil'
;University of Balamand
Lebanon
;
_audit_update_record             
;
2021-01-20 deposited with the CCDC.	2021-01-26 downloaded from the CCDC.
;

_audit_creation_method           SHELXL-2014/6
_chemical_name_systematic        ?
_chemical_name_common            ?
_chemical_melting_point          ?
_chemical_formula_moiety         ?
_chemical_formula_sum            'Cs10 H29 Na3 O98 Si2 W20 Zn4'
_chemical_formula_weight         6989.96

loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Cs Cs -0.3680 2.1192 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Na Na 0.0362 0.0249 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Si Si 0.0817 0.0704 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
W W -0.8490 6.8722 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Zn Zn 0.2839 1.4301 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_space_group_crystal_system      monoclinic
_space_group_IT_number           14
_space_group_name_H-M_alt        'P 21/c'
_space_group_name_Hall           '-P 2ybc'

_shelx_space_group_comment       
; 
The symmetry employed for this shelxl refinement is uniquely defined 
by the following loop, which should always be used as a source of 
symmetry information in preference to the above space-group names. 
They are only intended as comments. 
;

loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x, y+1/2, -z+1/2'
'-x, -y, -z'
'x, -y-1/2, z-1/2'

_cell_length_a                   13.131(2)
_cell_length_b                   15.755(3)
_cell_length_c                   24.894(5)
_cell_angle_alpha                90
_cell_angle_beta                 110.408(10)
_cell_angle_gamma                90
_cell_volume                     4826.8(16)
_cell_formula_units_Z            2
_cell_measurement_temperature    100(2)
_cell_measurement_reflns_used    9833
_cell_measurement_theta_min      3.30
_cell_measurement_theta_max      26.34

_exptl_crystal_description       needle
_exptl_crystal_colour            colourless
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    ?
_exptl_crystal_density_diffrn    4.809
_exptl_crystal_F_000             6048
_exptl_transmission_factor_min   0.056
_exptl_transmission_factor_max   0.119
_exptl_crystal_size_max          0.240
_exptl_crystal_size_mid          0.170
_exptl_crystal_size_min          0.130
_exptl_absorpt_coefficient_mu    28.566
_shelx_estimated_absorpt_T_min   0.056
_shelx_estimated_absorpt_T_max   0.119
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_correction_T_min  0.056
_exptl_absorpt_correction_T_max  0.119
_exptl_absorpt_process_details   SADABS
_exptl_absorpt_special_details   ?
_diffrn_ambient_temperature      100(2)
_diffrn_radiation_wavelength     0.71073
_diffrn_radiation_type           MoK\a
_diffrn_source                   ?
_diffrn_measurement_device_type  'Bruker APEX-II CCD'
_diffrn_measurement_method       'φ and ω scans'
_diffrn_detector_area_resol_mean ?
_diffrn_reflns_number            106346
_diffrn_reflns_av_unetI/netI     0.0514
_diffrn_reflns_av_R_equivalents  0.0806
_diffrn_reflns_limit_h_min       -15
_diffrn_reflns_limit_h_max       16
_diffrn_reflns_limit_k_min       -19
_diffrn_reflns_limit_k_max       19
_diffrn_reflns_limit_l_min       -31
_diffrn_reflns_limit_l_max       31
_diffrn_reflns_theta_min         3.413
_diffrn_reflns_theta_max         26.370
_diffrn_reflns_theta_full        25.242
_diffrn_measured_fraction_theta_max 0.995
_diffrn_measured_fraction_theta_full 0.997
_diffrn_reflns_Laue_measured_fraction_max 0.995
_diffrn_reflns_Laue_measured_fraction_full 0.997
_diffrn_reflns_point_group_measured_fraction_max 0.995
_diffrn_reflns_point_group_measured_fraction_full 0.997
_reflns_number_total             9846
_reflns_number_gt                7667
_reflns_threshold_expression     'I > 2σ(I)'
_reflns_Friedel_coverage         0.000
_reflns_Friedel_fraction_max     .
_reflns_Friedel_fraction_full    .

_reflns_special_details          
; 
 Reflections were merged by SHELXL according to the crystal 
 class for the calculation of statistics and refinement. 
  
 _reflns_Friedel_fraction is defined as the number of unique 
 Friedel pairs measured divided by the number that would be 
 possible theoretically, ignoring centric projections and 
 systematic absences. 
;

_computing_data_collection       'Bruker APEX2'
_computing_cell_refinement       'Bruker SAINT'
_computing_data_reduction        'Bruker SAINT'
_computing_structure_solution    'SHELXS-97 (Sheldrick 2008)'
_computing_structure_refinement  'SHELXL-2014/6 (Sheldrick, 2014)'
_computing_molecular_graphics    'Bruker SHELXTL'
_computing_publication_material  'Bruker SHELXTL'
_refine_special_details          ?
_refine_ls_structure_factor_coef Fsqd
_refine_ls_matrix_type           full
_refine_ls_weighting_scheme      calc
_refine_ls_weighting_details     
'w=1/[σ²(Fo²)+(0.0300P)²+185.0000P] where P=(Fo²+2Fc²)/3'
_atom_sites_solution_primary     ?
_atom_sites_solution_secondary   ?
_atom_sites_solution_hydrogens   .
_refine_ls_hydrogen_treatment    undef
_refine_ls_extinction_method     none
_refine_ls_extinction_coef       .
_refine_ls_number_reflns         9846
_refine_ls_number_parameters     379
_refine_ls_number_restraints     0
_refine_ls_R_factor_all          0.0602
_refine_ls_R_factor_gt           0.0383
_refine_ls_wR_factor_ref         0.0889
_refine_ls_wR_factor_gt          0.0806
_refine_ls_goodness_of_fit_ref   1.003
_refine_ls_restrained_S_all      1.003
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_diff_density_max         3.034
_refine_diff_density_min         -2.424
_refine_diff_density_rms         0.410

loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
Si1 Si 0.8170(3) 0.3317(2) 0.85490(15) 0.0116(7) Uani 1 1 d . . . . .
W1 W 0.73644(4) 0.20114(3) 0.73348(2) 0.01246(12) Uani 1 1 d . . . . .
W2 W 0.54322(4) 0.31365(3) 0.76246(2) 0.01292(12) Uani 1 1 d . . . . .
W3 W 0.72422(4) 0.41206(4) 0.71498(2) 0.01481(13) Uani 1 1 d . . . . .
W4 W 0.62592(4) 0.45820(4) 0.88977(2) 0.01308(12) Uani 1 1 d . . . . .
W5 W 0.80395(4) 0.55473(4) 0.84318(2) 0.01500(13) Uani 1 1 d . . . . .
W6 W 1.01597(4) 0.42496(4) 0.80927(2) 0.01363(12) Uani 1 1 d . . . . .
W7 W 1.02842(4) 0.21558(3) 0.82905(2) 0.01255(12) Uani 1 1 d . . . . .
W8 W 0.63658(4) 0.22395(4) 0.91005(2) 0.01400(12) Uani 1 1 d . . . . .
W9 W 0.90463(4) 0.24569(4) 0.99613(2) 0.01650(13) Uani 1 1 d . . . . .
W10 W 0.82397(4) 0.10940(3) 0.87993(2) 0.01291(12) Uani 1 1 d . . . . .
Zn1 Zn 0.88522(12) 0.46823(10) 0.97222(7) 0.0142(3) Uani 1 1 d . . . . .
Zn2 Zn 0.09183(11) 0.15699(9) 0.44081(6) 0.0097(3) Uani 1 1 d . . . . .
O12 O 0.5834(7) 0.2169(6) 0.7260(4) 0.0140(19) Uiso 1 1 d . . . . .
O13 O 0.7217(7) 0.2970(6) 0.6841(4) 0.015(2) Uiso 1 1 d . . . . .
O17 O 0.8851(7) 0.2121(6) 0.7616(4) 0.018(2) Uiso 1 1 d . . . . .
O23 O 0.5725(7) 0.3838(6) 0.7078(4) 0.018(2) Uiso 1 1 d . . . . .
O24 O 0.5617(7) 0.4053(6) 0.8126(4) 0.015(2) Uiso 1 1 d . . . . .
O28 O 0.5705(7) 0.2425(6) 0.8285(4) 0.0128(19) Uiso 1 1 d . . . . .
O35 O 0.7255(7) 0.4951(6) 0.7661(4) 0.017(2) Uiso 1 1 d . . . . .
O36 O 0.8745(7) 0.4052(6) 0.7430(4) 0.0143(19) Uiso 1 1 d . . . . .
O45 O 0.6597(7) 0.5537(6) 0.8495(4) 0.016(2) Uiso 1 1 d . . . . .
O48 O 0.6238(7) 0.3441(6) 0.9164(4) 0.016(2) Uiso 1 1 d . . . . .
O56 O 0.9310(7) 0.5072(6) 0.8327(4) 0.015(2) Uiso 1 1 d . . . . .
O67 O 1.0562(7) 0.3141(6) 0.7894(4) 0.017(2) Uiso 1 1 d . . . . .
O89 O 0.7427(7) 0.2170(6) 0.9822(4) 0.0149(19) Uiso 1 1 d . . . . .
O101 O 0.7478(7) 0.1369(6) 0.8002(4) 0.0135(19) Uiso 1 1 d . . . . .
O710 O 0.9513(7) 0.1460(6) 0.8645(4) 0.0143(19) Uiso 1 1 d . . . . .
O810 O 0.6859(7) 0.1163(6) 0.8907(4) 0.0136(19) Uiso 1 1 d . . . . .
O910 O 0.8938(7) 0.1253(6) 0.9581(4) 0.0143(19) Uiso 1 1 d . . . . .
O1S O 0.7333(7) 0.3171(5) 0.7890(4) 0.0113(18) Uiso 1 1 d . . . . .
O2S O 0.7886(7) 0.4225(6) 0.8782(4) 0.015(2) Uiso 1 1 d . . . . .
O3S O 0.9410(7) 0.3291(6) 0.8552(4) 0.0136(19) Uiso 1 1 d . . . . .
O4S O 0.8012(7) 0.2556(6) 0.8959(4) 0.0130(19) Uiso 1 1 d . . . . .
O1T O 0.7161(7) 0.1231(6) 0.6819(4) 0.015(2) Uiso 1 1 d . . . . .
O2T O 0.4026(7) 0.3052(6) 0.7316(4) 0.015(2) Uiso 1 1 d . . . . .
O3T O 0.6991(8) 0.4675(6) 0.6518(4) 0.024(2) Uiso 1 1 d . . . . .
O4T O 0.5047(7) 0.4960(6) 0.8936(4) 0.019(2) Uiso 1 1 d . . . . .
O5T O 0.8004(8) 0.6551(6) 0.8130(4) 0.021(2) Uiso 1 1 d . . . . .
O6T O 1.0732(7) 0.4864(6) 0.7694(4) 0.018(2) Uiso 1 1 d . . . . .
O7T O 1.0949(7) 0.1398(6) 0.8029(4) 0.018(2) Uiso 1 1 d . . . . .
O8T O 0.5252(7) 0.1898(6) 0.9264(4) 0.020(2) Uiso 1 1 d . . . . .
O9T O 0.9542(8) 0.2060(6) 1.0659(4) 0.021(2) Uiso 1 1 d . . . . .
O10T O 0.8334(7) 0.0003(6) 0.8741(4) 0.018(2) Uiso 1 1 d . . . . .
O1Z1 O 0.8751(7) 0.3547(6) 1.0059(4) 0.018(2) Uiso 1 1 d . . . . .
O1Z2 O 0.2439(8) 0.1562(6) 0.5030(4) 0.022(2) Uiso 1 1 d . . . . .
O2Z1 O 0.7222(7) 0.4941(6) 0.9578(4) 0.0137(19) Uiso 1 1 d . . . . .
O2Z2 O 1.0259(7) 0.2617(6) 0.9798(4) 0.016(2) Uiso 1 1 d . . . . .
O3Z1 O 0.8718(7) 0.5766(6) 0.9172(4) 0.019(2) Uiso 1 1 d . . . . .
O3Z2 O 1.1311(7) 0.2441(6) 0.8953(4) 0.016(2) Uiso 1 1 d . . . . .
O4Z2 O 1.1248(8) 0.4238(6) 0.8782(4) 0.021(2) Uiso 1 1 d . . . . .
O5Z2 O 0.9647(7) 0.5466(6) 1.0395(4) 0.019(2) Uiso 1 1 d . . . . .
Cs1 Cs 0.33703(8) 0.15734(7) 0.81271(5) 0.0333(2) Uani 1 1 d . . . . .
Cs2 Cs 0.92107(8) 0.16270(6) 0.64677(4) 0.0247(2) Uani 1 1 d . . . . .
Cs3 Cs 0.21238(8) 0.30383(7) 0.59408(4) 0.0298(2) Uani 1 1 d . . . . .
Cs4 Cs 0.93934(7) 0.46050(6) 0.63842(4) 0.0226(2) Uani 1 1 d . . . . .
Cs5 Cs 0.30210(7) 0.45649(6) 0.76349(4) 0.0237(2) Uani 1 1 d . . . . .
Na1 Na 0.5827(5) 0.1142(4) 0.5843(2) 0.0245(13) Uiso 1 1 d . . . . .
Na2 Na 0.3999(10) 0.4391(8) 0.5194(5) 0.029(3) Uiso 0.5 1 d . . P . .
O1W O 0.6926(9) 0.0157(7) 0.5617(5) 0.034(3) Uiso 1 1 d . . . . .
O2W O 0.6656(10) 0.2394(8) 0.5701(5) 0.047(3) Uiso 1 1 d . . . . .
O3W O 0.4701(9) 0.1208(8) 0.4834(5) 0.038(3) Uiso 1 1 d . . . . .
O4W O 1.1243(8) 0.3154(7) 0.6999(5) 0.028(2) Uiso 1 1 d . . . . .
O5W O 0.3148(9) 0.3284(7) 0.8635(5) 0.033(3) Uiso 1 1 d . . . . .
O6W O 0.4483(8) 0.1908(7) 0.6163(4) 0.027(2) Uiso 1 1 d . . . . .
O7W O 0.5138(7) 0.0602(6) 0.7717(4) 0.019(2) Uiso 1 1 d . . . . .
O8W O 0.4006(10) 0.4480(8) 0.6138(6) 0.047(3) Uiso 1 1 d . . . . .
O9W O 0.7406(18) 0.4538(15) 0.5193(10) 0.037(6) Uiso 0.5 1 d . . P A .
O10W O 0.4138(17) 0.2861(14) 0.5195(9) 0.028(5) Uiso 0.5 1 d . . P . .
O11W O 0.592(4) 0.441(3) 0.5304(19) 0.035(11) Uiso 0.25 1 d . . P . .
O12W O 0.916(2) 0.5349(19) 0.5107(12) 0.060(8) Uiso 0.5 1 d . . P A 1
O13W O 0.138(3) 0.401(2) 0.4794(14) 0.011(7) Uiso 0.25 1 d . . P B 2


_geom_special_details            
; 
 All esds (except the esd in the dihedral angle between two l.s. planes) 
 are estimated using the full covariance matrix.  The cell esds are taken 
 into account individually in the estimation of esds in distances, angles 
 and torsion angles; correlations between esds in cell parameters are only 
 used when they are defined by crystal symmetry.  An approximate (isotropic) 
 treatment of cell esds is used for estimating esds involving l.s. planes. 
;

loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Si1 O3S 1.626(9) . ?
Si1 O2S 1.634(10) . ?
Si1 O4S 1.634(9) . ?
Si1 O1S 1.642(9) . ?
W1 O1T 1.730(9) . ?
W1 O17 1.837(9) . ?
W1 O101 1.906(9) . ?
W1 O13 1.915(9) . ?
W1 O12 1.968(8) . ?
W1 O1S 2.299(9) . ?
W2 O2T 1.740(9) . ?
W2 O24 1.869(9) . ?
W2 O23 1.894(9) . ?
W2 O28 1.918(9) . ?
W2 O12 1.939(9) . ?
W2 O1S 2.349(8) . ?
W3 O3T 1.726(10) . ?
W3 O35 1.822(9) . ?
W3 O36 1.853(9) . ?
W3 O13 1.965(9) . ?
W3 O23 1.987(9) . ?
W3 O1S 2.344(8) . ?
W4 O4T 1.733(9) . ?
W4 O2Z1 1.815(9) . ?
W4 O48 1.920(9) . ?
W4 O45 1.943(9) . ?
W4 O24 1.991(9) . ?
W4 O2S 2.322(8) . ?
W5 O5T 1.744(10) . ?
W5 O3Z1 1.778(9) . ?
W5 O56 1.928(8) . ?
W5 O45 1.955(9) . ?
W5 O35 2.060(9) . ?
W5 O2S 2.294(9) . ?
W6 O6T 1.734(9) . ?
W6 O4Z2 1.810(10) . ?
W6 O56 1.927(9) . ?
W6 O67 1.939(9) . ?
W6 O36 2.033(9) . ?
W6 O3S 2.313(9) . ?
W7 O7T 1.734(9) . ?
W7 O3Z2 1.786(9) . ?
W7 O710 1.904(9) . ?
W7 O67 1.941(9) . ?
W7 O17 2.041(9) . ?
W7 O3S 2.337(9) . ?
W8 O8T 1.734(9) . ?
W8 O89 1.854(9) . ?
W8 O48 1.911(9) . ?
W8 O28 1.931(9) . ?
W8 O810 1.936(9) . ?
W8 O4S 2.361(8) . ?
W9 O9T 1.744(10) . ?
W9 O2Z2 1.793(8) . ?
W9 O1Z1 1.795(9) . ?
W9 O89 2.081(9) . ?
W9 O910 2.103(9) . ?
W9 O4S 2.393(9) . ?
W10 O10T 1.733(9) . ?
W10 O910 1.855(9) . ?
W10 O810 1.925(8) . ?
W10 O710 1.930(8) . ?
W10 O101 1.935(9) . ?
W10 O4S 2.375(9) . ?
Zn1 O1Z1 2.000(9) . ?
Zn1 O5Z2 2.049(10) . ?
Zn1 O2Z1 2.084(9) . ?
Zn1 O5Z2 2.103(9) 3_767 ?
Zn1 O3Z1 2.159(10) . ?
Zn1 O2S 2.354(9) . ?
Zn1 Zn1 3.016(3) 3_767 ?
Zn2 O2Z2 1.979(9) 4_465 ?
Zn2 O5Z2 2.018(9) 2_646 ?
Zn2 O1Z2 2.057(10) . ?
Zn2 O3Z2 2.094(9) 4_465 ?
Zn2 O4Z2 2.170(9) 4_465 ?
Zn2 O3S 2.359(9) 4_465 ?
Zn2 Cs3 4.2666(19) . ?
O13 Cs2 3.727(9) . ?
O17 Cs2 3.152(9) . ?
O24 Cs5 3.296(9) . ?
O28 Cs1 3.242(8) . ?
O35 Cs1 3.152(9) 2_656 ?
O36 Cs4 3.131(8) . ?
O56 Cs2 3.057(9) 2_756 ?
O101 Cs5 3.208(9) 2_646 ?
O710 Cs4 3.267(9) 2_746 ?
O3S Zn2 2.359(9) 4_666 ?
O1T Na1 2.455(11) . ?
O1T Cs5 3.003(9) 2_646 ?
O1T Cs2 3.169(8) . ?
O2T Cs5 2.963(9) . ?
O2T Cs1 3.385(9) . ?
O2T Cs3 3.464(9) . ?
O3T Cs1 3.201(10) 2_656 ?
O3T Cs4 3.288(9) . ?
O4T Na1 2.351(11) 2_656 ?
O4T Cs5 3.456(10) . ?
O5T Cs1 3.019(10) 2_656 ?
O5T Cs3 3.338(10) 2_656 ?
O5T Cs2 3.441(9) 2_756 ?
O6T Cs5 3.096(9) 1_655 ?
O6T Cs4 3.146(9) . ?
O6T Cs2 3.459(9) 2_756 ?
O7T Cs1 3.115(9) 1_655 ?
O7T Cs4 3.283(9) 2_746 ?
O7T Cs2 3.777(9) . ?
O8T Cs1 3.081(10) . ?
O9T Cs2 3.022(10) 4_566 ?
O9T Cs3 3.217(9) 4_666 ?
O9T Cs4 3.229(10) 4_566 ?
O10T Cs4 3.170(9) 2_746 ?
O10T Cs3 3.301(9) 2_646 ?
O10T Cs5 3.335(9) 2_646 ?
O1Z1 Cs2 3.355(9) 4_566 ?
O1Z2 Cs3 3.372(10) . ?
O2Z2 Zn2 1.979(9) 4_666 ?
O2Z2 Cs3 3.209(9) 4_666 ?
O3Z1 Cs3 3.728(10) 2_656 ?
O3Z2 Zn2 2.094(9) 4_666 ?
O4Z2 Zn2 2.170(9) 4_666 ?
O5Z2 Zn2 2.018(9) 2_656 ?
O5Z2 Zn1 2.103(9) 3_767 ?
Cs1 O5T 3.019(10) 2_646 ?
Cs1 O5W 3.033(11) . ?
Cs1 O7T 3.115(9) 1_455 ?
Cs1 O35 3.152(9) 2_646 ?
Cs1 O3T 3.201(10) 2_646 ?
Cs1 O7W 3.228(9) . ?
Cs2 O9T 3.022(10) 4_565 ?
Cs2 O56 3.057(9) 2_746 ?
Cs2 O1Z1 3.355(9) 4_565 ?
Cs2 O5T 3.441(9) 2_746 ?
Cs2 O2W 3.448(13) . ?
Cs2 O6T 3.458(9) 2_746 ?
Cs2 O4W 3.492(11) . ?
Cs2 O1W 3.797(11) . ?
Cs3 O13W 3.08(3) . ?
Cs3 O2Z2 3.209(9) 4_465 ?
Cs3 O9T 3.217(9) 4_465 ?
Cs3 O4W 3.230(10) 1_455 ?
Cs3 O8W 3.265(13) . ?
Cs3 O10T 3.301(9) 2_656 ?
Cs3 O5T 3.338(10) 2_646 ?
Cs3 O6W 3.446(10) . ?
Cs3 O12W 3.61(3) 3_666 ?
Cs3 O3Z1 3.728(10) 2_646 ?
Cs4 O9W 3.20(2) . ?
Cs4 O10T 3.170(9) 2_756 ?
Cs4 O9T 3.229(10) 4_565 ?
Cs4 O710 3.267(9) 2_756 ?
Cs4 O7T 3.283(9) 2_756 ?
Cs4 O4W 3.299(11) . ?
Cs4 O12W 3.30(3) . ?
Cs4 O13W 3.51(3) 3_666 ?
Cs5 O1T 3.003(9) 2_656 ?
Cs5 O6T 3.096(9) 1_455 ?
Cs5 O5W 3.163(11) . ?
Cs5 O101 3.208(9) 2_656 ?
Cs5 O4W 3.213(11) 1_455 ?
Cs5 O7W 3.280(9) 2_656 ?
Cs5 O10T 3.336(9) 2_656 ?
Na1 O1W 2.318(12) . ?
Na1 O2W 2.338(14) . ?
Na1 O4T 2.351(11) 2_646 ?
Na1 O3W 2.432(13) . ?
Na1 O6W 2.487(11) . ?
Na1 Cs5 4.339(6) 2_646 ?
Na2 O11W 2.28(5) 3_666 ?
Na2 O8W 2.352(17) . ?
Na2 O10W 2.42(2) . ?
Na2 O9W 2.44(3) 3_666 ?
Na2 O11W 2.44(4) . ?
Na2 Na2 3.65(2) 3_666 ?
O4W Cs5 3.213(11) 1_655 ?
O4W Cs3 3.230(10) 1_655 ?
O7W Cs5 3.281(9) 2_646 ?
O9W Na2 2.44(3) 3_666 ?
O11W Na2 2.28(5) 3_666 ?
O12W Cs3 3.61(3) 3_666 ?
O13W Cs4 3.51(3) 3_666 ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O3S Si1 O2S 111.9(5) . . ?
O3S Si1 O4S 108.9(5) . . ?
O2S Si1 O4S 109.0(5) . . ?
O3S Si1 O1S 108.8(5) . . ?
O2S Si1 O1S 108.7(5) . . ?
O4S Si1 O1S 109.6(5) . . ?
O1T W1 O17 102.5(4) . . ?
O1T W1 O101 102.3(4) . . ?
O17 W1 O101 88.2(4) . . ?
O1T W1 O13 97.5(4) . . ?
O17 W1 O13 91.5(4) . . ?
O101 W1 O13 159.8(4) . . ?
O1T W1 O12 97.5(4) . . ?
O17 W1 O12 159.8(4) . . ?
O101 W1 O12 85.2(4) . . ?
O13 W1 O12 88.2(4) . . ?
O1T W1 O1S 168.6(4) . . ?
O17 W1 O1S 86.4(4) . . ?
O101 W1 O1S 84.9(3) . . ?
O13 W1 O1S 74.9(3) . . ?
O12 W1 O1S 74.1(3) . . ?
O1T W1 Cs2 55.3(3) . . ?
O17 W1 Cs2 55.2(3) . . ?
O101 W1 Cs2 122.5(3) . . ?
O13 W1 Cs2 72.8(3) . . ?
O12 W1 Cs2 142.7(3) . . ?
O1S W1 Cs2 127.9(2) . . ?
O1T W1 Cs5 47.4(3) . 2_646 ?
O17 W1 Cs5 102.3(3) . 2_646 ?
O101 W1 Cs5 55.1(3) . 2_646 ?
O13 W1 Cs5 144.0(3) . 2_646 ?
O12 W1 Cs5 89.5(3) . 2_646 ?
O1S W1 Cs5 138.2(2) . 2_646 ?
Cs2 W1 Cs5 88.07(2) . 2_646 ?
O2T W2 O24 103.0(4) . . ?
O2T W2 O23 100.2(4) . . ?
O24 W2 O23 91.0(4) . . ?
O2T W2 O28 100.7(4) . . ?
O24 W2 O28 86.4(4) . . ?
O23 W2 O28 159.0(4) . . ?
O2T W2 O12 98.8(4) . . ?
O24 W2 O12 158.0(4) . . ?
O23 W2 O12 88.0(4) . . ?
O28 W2 O12 86.7(4) . . ?
O2T W2 O1S 170.3(4) . . ?
O24 W2 O1S 85.2(3) . . ?
O23 W2 O1S 74.1(3) . . ?
O28 W2 O1S 84.9(3) . . ?
O12 W2 O1S 73.4(3) . . ?
O2T W2 Cs5 46.1(3) . . ?
O24 W2 Cs5 57.7(3) . . ?
O23 W2 Cs5 92.1(3) . . ?
O28 W2 Cs5 104.0(2) . . ?
O12 W2 Cs5 144.3(3) . . ?
O1S W2 Cs5 140.5(2) . . ?
O2T W2 Cs1 52.1(3) . . ?
O24 W2 Cs1 101.7(3) . . ?
O23 W2 Cs1 151.4(3) . . ?
O28 W2 Cs1 48.9(3) . . ?
O12 W2 Cs1 89.3(3) . . ?
O1S W2 Cs1 131.9(2) . . ?
Cs5 W2 Cs1 73.99(3) . . ?
O3T W3 O35 103.0(4) . . ?
O3T W3 O36 102.3(4) . . ?
O35 W3 O36 91.7(4) . . ?
O3T W3 O13 97.9(4) . . ?
O35 W3 O13 158.6(4) . . ?
O36 W3 O13 87.9(4) . . ?
O3T W3 O23 99.4(4) . . ?
O35 W3 O23 89.3(4) . . ?
O36 W3 O23 157.4(4) . . ?
O13 W3 O23 83.0(4) . . ?
O3T W3 O1S 168.4(4) . . ?
O35 W3 O1S 85.6(4) . . ?
O36 W3 O1S 84.9(3) . . ?
O13 W3 O1S 73.0(3) . . ?
O23 W3 O1S 72.7(3) . . ?
O3T W3 Cs1 52.1(3) . 2_656 ?
O35 W3 Cs1 51.1(3) . 2_656 ?
O36 W3 Cs1 104.3(3) . 2_656 ?
O13 W3 Cs1 149.1(3) . 2_656 ?
O23 W3 Cs1 93.8(3) . 2_656 ?
O1S W3 Cs1 135.4(2) . 2_656 ?
O3T W3 Cs4 53.9(3) . . ?
O35 W3 Cs4 111.1(3) . . ?
O36 W3 Cs4 49.7(3) . . ?
O13 W3 Cs4 84.7(2) . . ?
O23 W3 Cs4 148.6(3) . . ?
O1S W3 Cs4 130.3(2) . . ?
Cs1 W3 Cs4 82.24(2) 2_656 . ?
O4T W4 O2Z1 101.3(4) . . ?
O4T W4 O48 100.3(4) . . ?
O2Z1 W4 O48 93.3(4) . . ?
O4T W4 O45 98.1(4) . . ?
O2Z1 W4 O45 91.8(4) . . ?
O48 W4 O45 159.5(4) . . ?
O4T W4 O24 96.2(4) . . ?
O2Z1 W4 O24 162.5(4) . . ?
O48 W4 O24 83.6(4) . . ?
O45 W4 O24 85.6(4) . . ?
O4T W4 O2S 172.9(4) . . ?
O2Z1 W4 O2S 79.7(3) . . ?
O48 W4 O2S 86.6(3) . . ?
O45 W4 O2S 74.8(3) . . ?
O24 W4 O2S 82.9(3) . . ?
O4T W4 Cs5 49.6(3) . . ?
O2Z1 W4 Cs5 150.5(3) . . ?
O48 W4 Cs5 96.7(3) . . ?
O45 W4 Cs5 88.5(3) . . ?
O24 W4 Cs5 46.9(2) . . ?
O2S W4 Cs5 128.5(2) . . ?
O5T W5 O3Z1 101.5(4) . . ?
O5T W5 O56 100.8(4) . . ?
O3Z1 W5 O56 94.1(4) . . ?
O5T W5 O45 99.3(4) . . ?
O3Z1 W5 O45 93.9(4) . . ?
O56 W5 O45 156.4(4) . . ?
O5T W5 O35 94.7(4) . . ?
O3Z1 W5 O35 163.8(4) . . ?
O56 W5 O35 82.7(4) . . ?
O45 W5 O35 83.5(4) . . ?
O5T W5 O2S 173.8(4) . . ?
O3Z1 W5 O2S 82.1(4) . . ?
O56 W5 O2S 83.9(3) . . ?
O45 W5 O2S 75.3(3) . . ?
O35 W5 O2S 81.8(3) . . ?
O5T W5 Cs2 61.3(3) . 2_756 ?
O3Z1 W5 Cs2 74.4(3) . 2_756 ?
O56 W5 Cs2 49.9(3) . 2_756 ?
O45 W5 Cs2 153.5(3) . 2_756 ?
O35 W5 Cs2 114.1(2) . 2_756 ?
O2S W5 Cs2 124.8(2) . 2_756 ?
O5T W5 Cs1 44.3(3) . 2_656 ?
O3Z1 W5 Cs1 145.0(3) . 2_656 ?
O56 W5 Cs1 98.9(3) . 2_656 ?
O45 W5 Cs1 87.0(3) . 2_656 ?
O35 W5 Cs1 51.0(3) . 2_656 ?
O2S W5 Cs1 131.4(2) . 2_656 ?
Cs2 W5 Cs1 89.48(3) 2_756 2_656 ?
O5T W5 Cs3 47.6(3) . 2_656 ?
O3Z1 W5 Cs3 60.8(3) . 2_656 ?
O56 W5 Cs3 124.4(3) . 2_656 ?
O45 W5 Cs3 78.7(3) . 2_656 ?
O35 W5 Cs3 133.5(3) . 2_656 ?
O2S W5 Cs3 132.5(2) . 2_656 ?
Cs2 W5 Cs3 74.91(2) 2_756 2_656 ?
Cs1 W5 Cs3 85.30(3) 2_656 2_656 ?
O6T W6 O4Z2 101.0(4) . . ?
O6T W6 O56 102.1(4) . . ?
O4Z2 W6 O56 94.0(4) . . ?
O6T W6 O67 98.4(4) . . ?
O4Z2 W6 O67 92.2(4) . . ?
O56 W6 O67 157.1(4) . . ?
O6T W6 O36 94.4(4) . . ?
O4Z2 W6 O36 164.5(4) . . ?
O56 W6 O36 83.5(4) . . ?
O67 W6 O36 84.7(4) . . ?
O6T W6 O3S 172.9(4) . . ?
O4Z2 W6 O3S 81.7(4) . . ?
O56 W6 O3S 84.2(3) . . ?
O67 W6 O3S 74.9(3) . . ?
O36 W6 O3S 82.9(3) . . ?
O6T W6 Cs2 62.2(3) . 2_756 ?
O4Z2 W6 Cs2 74.0(3) . 2_756 ?
O56 W6 Cs2 50.2(3) . 2_756 ?
O67 W6 Cs2 152.2(3) . 2_756 ?
O36 W6 Cs2 114.7(3) . 2_756 ?
O3S W6 Cs2 124.9(2) . 2_756 ?
O6T W6 Cs4 47.3(3) . . ?
O4Z2 W6 Cs4 145.2(3) . . ?
O56 W6 Cs4 105.5(3) . . ?
O67 W6 Cs4 81.2(3) . . ?
O36 W6 Cs4 49.2(2) . . ?
O3S W6 Cs4 128.1(2) . . ?
Cs2 W6 Cs4 96.45(2) 2_756 . ?
O6T W6 Cs5 36.3(3) . 1_655 ?
O4Z2 W6 Cs5 77.2(3) . 1_655 ?
O56 W6 Cs5 130.6(3) . 1_655 ?
O67 W6 Cs5 72.3(3) . 1_655 ?
O36 W6 Cs5 115.9(2) . 1_655 ?
O3S W6 Cs5 140.0(2) . 1_655 ?
Cs2 W6 Cs5 81.09(2) 2_756 1_655 ?
Cs4 W6 Cs5 68.14(2) . 1_655 ?
O7T W7 O3Z2 101.7(4) . . ?
O7T W7 O710 101.3(4) . . ?
O3Z2 W7 O710 94.0(4) . . ?
O7T W7 O67 98.7(4) . . ?
O3Z2 W7 O67 93.0(4) . . ?
O710 W7 O67 157.0(4) . . ?
O7T W7 O17 96.5(4) . . ?
O3Z2 W7 O17 161.8(4) . . ?
O710 W7 O17 83.0(4) . . ?
O67 W7 O17 83.5(4) . . ?
O7T W7 O3S 172.7(4) . . ?
O3Z2 W7 O3S 80.5(4) . . ?
O710 W7 O3S 85.4(3) . . ?
O67 W7 O3S 74.2(3) . . ?
O17 W7 O3S 81.3(3) . . ?
O7T W7 Cs4 50.8(3) . 2_746 ?
O3Z2 W7 Cs4 94.1(3) . 2_746 ?
O710 W7 Cs4 51.5(3) . 2_746 ?
O67 W7 Cs4 149.4(3) . 2_746 ?
O17 W7 Cs4 97.9(3) . 2_746 ?
O3S W7 Cs4 136.3(2) . 2_746 ?
O7T W7 Cs1 37.3(3) . 1_655 ?
O3Z2 W7 Cs1 73.1(3) . 1_655 ?
O710 W7 Cs1 126.2(3) . 1_655 ?
O67 W7 Cs1 76.8(3) . 1_655 ?
O17 W7 Cs1 123.0(2) . 1_655 ?
O3S W7 Cs1 139.3(2) . 1_655 ?
Cs4 W7 Cs1 76.93(2) 2_746 1_655 ?
O7T W7 Cs2 59.9(3) . . ?
O3Z2 W7 Cs2 151.6(3) . . ?
O710 W7 Cs2 110.0(3) . . ?
O67 W7 Cs2 70.8(3) . . ?
O17 W7 Cs2 42.6(2) . . ?
O3S W7 Cs2 115.3(2) . . ?
Cs4 W7 Cs2 89.53(2) 2_746 . ?
Cs1 W7 Cs2 80.42(2) 1_655 . ?
O8T W8 O89 99.5(4) . . ?
O8T W8 O48 100.5(4) . . ?
O89 W8 O48 92.1(4) . . ?
O8T W8 O28 100.7(4) . . ?
O89 W8 O28 159.7(4) . . ?
O48 W8 O28 85.3(4) . . ?
O8T W8 O810 99.8(4) . . ?
O89 W8 O810 89.2(4) . . ?
O48 W8 O810 159.2(4) . . ?
O28 W8 O810 86.4(4) . . ?
O8T W8 O4S 172.3(4) . . ?
O89 W8 O4S 74.9(3) . . ?
O48 W8 O4S 85.1(3) . . ?
O28 W8 O4S 84.9(3) . . ?
O810 W8 O4S 75.2(3) . . ?
O8T W8 Cs1 47.5(3) . . ?
O89 W8 Cs1 145.6(3) . . ?
O48 W8 Cs1 102.4(3) . . ?
O28 W8 Cs1 54.0(2) . . ?
O810 W8 Cs1 87.9(3) . . ?
O4S W8 Cs1 136.7(2) . . ?
O9T W9 O2Z2 102.9(4) . . ?
O9T W9 O1Z1 103.3(4) . . ?
O2Z2 W9 O1Z1 98.4(4) . . ?
O9T W9 O89 95.3(4) . . ?
O2Z2 W9 O89 158.3(4) . . ?
O1Z1 W9 O89 88.5(4) . . ?
O9T W9 O910 93.9(4) . . ?
O2Z2 W9 O910 87.2(4) . . ?
O1Z1 W9 O910 160.0(4) . . ?
O89 W9 O910 79.9(3) . . ?
O9T W9 O4S 160.1(4) . . ?
O2Z2 W9 O4S 88.9(4) . . ?
O1Z1 W9 O4S 90.5(4) . . ?
O89 W9 O4S 70.5(3) . . ?
O910 W9 O4S 70.4(3) . . ?
O9T W9 Cs2 46.2(3) . 4_566 ?
O2Z2 W9 Cs2 113.9(3) . 4_566 ?
O1Z1 W9 Cs2 57.7(3) . 4_566 ?
O89 W9 Cs2 87.2(2) . 4_566 ?
O910 W9 Cs2 136.8(2) . 4_566 ?
O4S W9 Cs2 142.0(2) . 4_566 ?
O9T W9 Cs3 51.4(3) . 4_666 ?
O2Z2 W9 Cs3 51.5(3) . 4_666 ?
O1Z1 W9 Cs3 108.9(3) . 4_666 ?
O89 W9 Cs3 144.6(3) . 4_666 ?
O910 W9 Cs3 89.7(2) . 4_666 ?
O4S W9 Cs3 137.2(2) . 4_666 ?
Cs2 W9 Cs3 77.51(2) 4_566 4_666 ?
O10T W10 O910 101.4(4) . . ?
O10T W10 O810 99.5(4) . . ?
O910 W10 O810 89.5(4) . . ?
O10T W10 O710 100.8(4) . . ?
O910 W10 O710 91.3(4) . . ?
O810 W10 O710 159.1(4) . . ?
O10T W10 O101 99.4(4) . . ?
O910 W10 O101 159.2(4) . . ?
O810 W10 O101 87.4(4) . . ?
O710 W10 O101 84.4(4) . . ?
O10T W10 O4S 173.3(4) . . ?
O910 W10 O4S 74.8(3) . . ?
O810 W10 O4S 75.1(3) . . ?
O710 W10 O4S 85.0(3) . . ?
O101 W10 O4S 84.5(3) . . ?
O10T W10 Cs4 48.4(3) . 2_746 ?
O910 W10 Cs4 94.5(3) . 2_746 ?
O810 W10 Cs4 147.8(3) . 2_746 ?
O710 W10 Cs4 52.9(3) . 2_746 ?
O101 W10 Cs4 99.0(2) . 2_746 ?
O4S W10 Cs4 136.7(2) . 2_746 ?
O10T W10 Cs5 51.0(3) . 2_646 ?
O910 W10 Cs5 152.2(3) . 2_646 ?
O810 W10 Cs5 92.3(3) . 2_646 ?
O710 W10 Cs5 96.6(3) . 2_646 ?
O101 W10 Cs5 48.5(3) . 2_646 ?
O4S W10 Cs5 132.3(2) . 2_646 ?
Cs4 W10 Cs5 69.96(2) 2_746 2_646 ?
O1Z1 Zn1 O5Z2 106.6(4) . . ?
O1Z1 Zn1 O2Z1 91.9(4) . . ?
O5Z2 Zn1 O2Z1 102.9(4) . . ?
O1Z1 Zn1 O5Z2 99.3(4) . 3_767 ?
O5Z2 Zn1 O5Z2 86.9(4) . 3_767 ?
O2Z1 Zn1 O5Z2 162.5(4) . 3_767 ?
O1Z1 Zn1 O3Z1 166.3(4) . . ?
O5Z2 Zn1 O3Z1 87.0(4) . . ?
O2Z1 Zn1 O3Z1 83.4(3) . . ?
O5Z2 Zn1 O3Z1 82.7(4) 3_767 . ?
O1Z1 Zn1 O2S 93.0(4) . . ?
O5Z2 Zn1 O2S 160.4(4) . . ?
O2Z1 Zn1 O2S 74.0(3) . . ?
O5Z2 Zn1 O2S 92.0(3) 3_767 . ?
O3Z1 Zn1 O2S 73.4(3) . . ?
O1Z1 Zn1 Zn1 107.8(3) . 3_767 ?
O5Z2 Zn1 Zn1 44.1(3) . 3_767 ?
O2Z1 Zn1 Zn1 144.8(3) . 3_767 ?
O5Z2 Zn1 Zn1 42.7(3) 3_767 3_767 ?
O3Z1 Zn1 Zn1 82.9(3) . 3_767 ?
O2S Zn1 Zn1 131.6(2) . 3_767 ?
O2Z2 Zn2 O5Z2 100.2(4) 4_465 2_646 ?
O2Z2 Zn2 O1Z2 96.3(4) 4_465 . ?
O5Z2 Zn2 O1Z2 98.9(4) 2_646 . ?
O2Z2 Zn2 O3Z2 90.9(4) 4_465 4_465 ?
O5Z2 Zn2 O3Z2 162.5(4) 2_646 4_465 ?
O1Z2 Zn2 O3Z2 93.1(4) . 4_465 ?
O2Z2 Zn2 O4Z2 164.3(4) 4_465 4_465 ?
O5Z2 Zn2 O4Z2 81.4(4) 2_646 4_465 ?
O1Z2 Zn2 O4Z2 98.8(4) . 4_465 ?
O3Z2 Zn2 O4Z2 84.2(4) 4_465 4_465 ?
O2Z2 Zn2 O3S 90.5(3) 4_465 4_465 ?
O5Z2 Zn2 O3S 92.0(3) 2_646 4_465 ?
O1Z2 Zn2 O3S 165.8(3) . 4_465 ?
O3Z2 Zn2 O3S 74.3(3) 4_465 4_465 ?
O4Z2 Zn2 O3S 73.8(3) 4_465 4_465 ?
O2Z2 Zn2 Cs3 45.6(3) 4_465 . ?
O5Z2 Zn2 Cs3 107.7(3) 2_646 . ?
O1Z2 Zn2 Cs3 50.9(3) . . ?
O3Z2 Zn2 Cs3 89.8(3) 4_465 . ?
O4Z2 Zn2 Cs3 148.8(3) 4_465 . ?
O3S Zn2 Cs3 133.6(2) 4_465 . ?
W2 O12 W1 119.3(5) . . ?
W1 O13 W3 119.5(5) . . ?
W1 O13 Cs2 77.8(3) . . ?
W3 O13 Cs2 134.8(4) . . ?
W1 O17 W7 150.3(5) . . ?
W1 O17 Cs2 96.2(4) . . ?
W7 O17 Cs2 111.5(3) . . ?
W2 O23 W3 121.0(5) . . ?
W2 O24 W4 151.7(5) . . ?
W2 O24 Cs5 93.7(3) . . ?
W4 O24 Cs5 106.9(3) . . ?
W2 O28 W8 150.5(5) . . ?
W2 O28 Cs1 104.6(3) . . ?
W8 O28 Cs1 97.1(3) . . ?
W3 O35 W5 149.1(5) . . ?
W3 O35 Cs1 102.2(4) . 2_656 ?
W5 O35 Cs1 98.5(3) . 2_656 ?
W3 O36 W6 148.0(5) . . ?
W3 O36 Cs4 103.5(3) . . ?
W6 O36 Cs4 101.3(3) . . ?
W4 O45 W5 116.7(5) . . ?
W8 O48 W4 152.4(5) . . ?
W6 O56 W5 157.1(5) . . ?
W6 O56 Cs2 100.9(3) . 2_756 ?
W5 O56 Cs2 101.3(3) . 2_756 ?
W7 O67 W6 118.3(4) . . ?
W8 O89 W9 121.8(4) . . ?
W1 O101 W10 150.2(5) . . ?
W1 O101 Cs5 95.7(3) . 2_646 ?
W10 O101 Cs5 104.6(3) . 2_646 ?
W7 O710 W10 154.3(5) . . ?
W7 O710 Cs4 101.3(3) . 2_746 ?
W10 O710 Cs4 98.9(3) . 2_746 ?
W10 O810 W8 119.8(4) . . ?
W10 O910 W9 121.7(5) . . ?
Si1 O1S W1 124.4(5) . . ?
Si1 O1S W3 121.9(5) . . ?
W1 O1S W3 92.4(3) . . ?
Si1 O1S W2 124.0(4) . . ?
W1 O1S W2 93.0(3) . . ?
W3 O1S W2 92.1(3) . . ?
Si1 O2S W5 126.8(5) . . ?
Si1 O2S W4 126.2(5) . . ?
W5 O2S W4 91.9(3) . . ?
Si1 O2S Zn1 120.7(5) . . ?
W5 O2S Zn1 90.6(3) . . ?
W4 O2S Zn1 90.1(3) . . ?
Si1 O3S W6 125.4(5) . . ?
Si1 O3S W7 127.3(5) . . ?
W6 O3S W7 91.5(3) . . ?
Si1 O3S Zn2 121.8(5) . 4_666 ?
W6 O3S Zn2 91.0(3) . 4_666 ?
W7 O3S Zn2 89.1(3) . 4_666 ?
Si1 O4S W8 124.8(5) . . ?
Si1 O4S W10 123.8(5) . . ?
W8 O4S W10 89.7(3) . . ?
Si1 O4S W9 123.4(5) . . ?
W8 O4S W9 92.7(3) . . ?
W10 O4S W9 93.0(3) . . ?
W1 O1T Na1 130.3(5) . . ?
W1 O1T Cs5 107.6(4) . 2_646 ?
Na1 O1T Cs5 104.9(3) . 2_646 ?
W1 O1T Cs2 98.0(3) . . ?
Na1 O1T Cs2 96.9(3) . . ?
Cs5 O1T Cs2 120.4(3) 2_646 . ?
W2 O2T Cs5 108.9(4) . . ?
W2 O2T Cs1 103.9(4) . . ?
Cs5 O2T Cs1 99.5(2) . . ?
W2 O2T Cs3 136.5(4) . . ?
Cs5 O2T Cs3 92.0(2) . . ?
Cs1 O2T Cs3 109.8(2) . . ?
W3 O3T Cs1 102.8(4) . 2_656 ?
W3 O3T Cs4 101.0(4) . . ?
Cs1 O3T Cs4 107.4(3) 2_656 . ?
W4 O4T Na1 144.8(5) . 2_656 ?
W4 O4T Cs5 108.0(4) . . ?
Na1 O4T Cs5 94.8(3) 2_656 . ?
W5 O5T Cs1 112.0(4) . 2_656 ?
W5 O5T Cs3 109.8(4) . 2_656 ?
Cs1 O5T Cs3 123.6(3) 2_656 2_656 ?
W5 O5T Cs2 92.3(4) . 2_756 ?
Cs1 O5T Cs2 119.5(3) 2_656 2_756 ?
Cs3 O5T Cs2 94.5(2) 2_656 2_756 ?
W6 O6T Cs5 124.3(4) . 1_655 ?
W6 O6T Cs4 108.9(4) . . ?
Cs5 O6T Cs4 97.6(2) 1_655 . ?
W6 O6T Cs2 91.5(3) . 2_756 ?
Cs5 O6T Cs2 109.5(3) 1_655 2_756 ?
Cs4 O6T Cs2 128.0(3) . 2_756 ?
W7 O7T Cs1 122.9(4) . 1_655 ?
W7 O7T Cs4 105.1(4) . 2_746 ?
Cs1 O7T Cs4 109.6(3) 1_655 2_746 ?
W7 O7T Cs2 96.8(4) . . ?
Cs1 O7T Cs2 107.8(2) 1_655 . ?
Cs4 O7T Cs2 114.4(3) 2_746 . ?
W8 O8T Cs1 108.0(4) . . ?
W9 O9T Cs2 109.1(4) . 4_566 ?
W9 O9T Cs3 103.5(4) . 4_666 ?
Cs2 O9T Cs3 105.9(3) 4_566 4_666 ?
W9 O9T Cs4 140.7(5) . 4_566 ?
Cs2 O9T Cs4 97.6(3) 4_566 4_566 ?
Cs3 O9T Cs4 95.9(3) 4_666 4_566 ?
W10 O10T Cs4 107.5(4) . 2_746 ?
W10 O10T Cs3 152.3(4) . 2_646 ?
Cs4 O10T Cs3 95.4(2) 2_746 2_646 ?
W10 O10T Cs5 105.2(4) . 2_646 ?
Cs4 O10T Cs5 92.4(2) 2_746 2_646 ?
Cs3 O10T Cs5 88.6(2) 2_646 2_646 ?
W9 O1Z1 Zn1 138.6(5) . . ?
W9 O1Z1 Cs2 95.5(3) . 4_566 ?
Zn1 O1Z1 Cs2 119.8(4) . 4_566 ?
Zn2 O1Z2 Cs3 100.8(3) . . ?
W4 O2Z1 Zn1 116.0(4) . . ?
W9 O2Z2 Zn2 141.0(5) . 4_666 ?
W9 O2Z2 Cs3 102.5(4) . 4_666 ?
Zn2 O2Z2 Cs3 108.3(3) 4_666 4_666 ?
W5 O3Z1 Zn1 113.9(5) . . ?
W5 O3Z1 Cs3 94.6(4) . 2_656 ?
Zn1 O3Z1 Cs3 139.8(4) . 2_656 ?
W7 O3Z2 Zn2 116.0(4) . 4_666 ?
W6 O4Z2 Zn2 113.4(5) . 4_666 ?
Zn2 O5Z2 Zn1 126.3(5) 2_656 . ?
Zn2 O5Z2 Zn1 124.8(5) 2_656 3_767 ?
Zn1 O5Z2 Zn1 93.1(4) . 3_767 ?
O5T Cs1 O5W 109.4(3) 2_646 . ?
O5T Cs1 O8T 162.1(2) 2_646 . ?
O5W Cs1 O8T 68.5(3) . . ?
O5T Cs1 O7T 72.1(2) 2_646 1_455 ?
O5W Cs1 O7T 82.4(3) . 1_455 ?
O8T Cs1 O7T 123.8(2) . 1_455 ?
O5T Cs1 O35 54.1(3) 2_646 2_646 ?
O5W Cs1 O35 159.7(3) . 2_646 ?
O8T Cs1 O35 131.1(2) . 2_646 ?
O7T Cs1 O35 80.9(2) 1_455 2_646 ?
O5T Cs1 O3T 100.5(3) 2_646 2_646 ?
O5W Cs1 O3T 132.1(3) . 2_646 ?
O8T Cs1 O3T 92.9(3) . 2_646 ?
O7T Cs1 O3T 72.1(2) 1_455 2_646 ?
O35 Cs1 O3T 51.9(2) 2_646 2_646 ?
O5T Cs1 O7W 84.4(2) 2_646 . ?
O5W Cs1 O7W 137.5(3) . . ?
O8T Cs1 O7W 86.2(2) . . ?
O7T Cs1 O7W 139.5(2) 1_455 . ?
O35 Cs1 O7W 58.6(2) 2_646 . ?
O3T Cs1 O7W 80.6(2) 2_646 . ?
O5T Cs1 O28 109.2(2) 2_646 . ?
O5W Cs1 O28 78.8(3) . . ?
O8T Cs1 O28 53.0(2) . . ?
O7T Cs1 O28 160.4(2) 1_455 . ?
O35 Cs1 O28 116.2(2) 2_646 . ?
O3T Cs1 O28 125.3(2) 2_646 . ?
O7W Cs1 O28 58.7(2) . . ?
O5T Cs1 O2T 64.8(2) 2_646 . ?
O5W Cs1 O2T 73.6(3) . . ?
O8T Cs1 O2T 98.3(2) . . ?
O7T Cs1 O2T 118.6(2) 1_455 . ?
O35 Cs1 O2T 104.6(2) 2_646 . ?
O3T Cs1 O2T 154.3(2) 2_646 . ?
O7W Cs1 O2T 77.2(2) . . ?
O28 Cs1 O2T 50.3(2) . . ?
O5T Cs1 W3 78.23(19) 2_646 2_646 ?
O5W Cs1 W3 153.7(2) . 2_646 ?
O8T Cs1 W3 111.78(18) . 2_646 ?
O7T Cs1 W3 76.12(18) 1_455 2_646 ?
O35 Cs1 W3 26.74(17) 2_646 2_646 ?
O3T Cs1 W3 25.17(18) 2_646 2_646 ?
O7W Cs1 W3 66.85(17) . 2_646 ?
O28 Cs1 W3 123.44(16) . 2_646 ?
O2T Cs1 W3 130.29(16) . 2_646 ?
O5T Cs1 W8 137.90(18) 2_646 . ?
O5W Cs1 W8 74.3(2) . . ?
O8T Cs1 W8 24.52(17) . . ?
O7T Cs1 W8 146.84(17) 1_455 . ?
O35 Cs1 W8 125.54(16) 2_646 . ?
O3T Cs1 W8 106.80(18) 2_646 . ?
O7W Cs1 W8 69.52(17) . . ?
O28 Cs1 W8 28.83(15) . . ?
O2T Cs1 W8 77.20(16) . . ?
W3 Cs1 W8 117.50(3) 2_646 . ?
O5T Cs1 W5 23.78(19) 2_646 2_646 ?
O5W Cs1 W5 133.0(2) . 2_646 ?
O8T Cs1 W5 155.08(17) . 2_646 ?
O7T Cs1 W5 76.97(17) 1_455 2_646 ?
O35 Cs1 W5 30.53(17) 2_646 2_646 ?
O3T Cs1 W5 80.05(18) 2_646 2_646 ?
O7W Cs1 W5 69.10(17) . 2_646 ?
O28 Cs1 W5 112.46(15) . 2_646 ?
O2T Cs1 W5 80.10(16) . 2_646 ?
W3 Cs1 W5 56.004(18) 2_646 2_646 ?
W8 Cs1 W5 136.14(3) . 2_646 ?
O9T Cs2 O56 115.4(2) 4_565 2_746 ?
O9T Cs2 O17 122.5(3) 4_565 . ?
O56 Cs2 O17 109.5(2) 2_746 . ?
O9T Cs2 O1T 130.7(2) 4_565 . ?
O56 Cs2 O1T 110.3(2) 2_746 . ?
O17 Cs2 O1T 52.3(2) . . ?
O9T Cs2 O1Z1 51.3(2) 4_565 4_565 ?
O56 Cs2 O1Z1 89.0(2) 2_746 4_565 ?
O17 Cs2 O1Z1 159.8(2) . 4_565 ?
O1T Cs2 O1Z1 114.3(2) . 4_565 ?
O9T Cs2 O5T 80.4(2) 4_565 2_746 ?
O56 Cs2 O5T 51.3(2) 2_746 2_746 ?
O17 Cs2 O5T 103.0(2) . 2_746 ?
O1T Cs2 O5T 146.3(2) . 2_746 ?
O1Z1 Cs2 O5T 95.0(2) 4_565 2_746 ?
O9T Cs2 O2W 74.3(3) 4_565 . ?
O56 Cs2 O2W 144.3(3) 2_746 . ?
O17 Cs2 O2W 89.5(3) . . ?
O1T Cs2 O2W 57.7(3) . . ?
O1Z1 Cs2 O2W 70.4(3) 4_565 . ?
O5T Cs2 O2W 154.6(3) 2_746 . ?
O9T Cs2 O6T 166.8(2) 4_565 2_746 ?
O56 Cs2 O6T 51.4(2) 2_746 2_746 ?
O17 Cs2 O6T 68.3(2) . 2_746 ?
O1T Cs2 O6T 61.1(2) . 2_746 ?
O1Z1 Cs2 O6T 121.5(2) 4_565 2_746 ?
O5T Cs2 O6T 89.9(2) 2_746 2_746 ?
O2W Cs2 O6T 115.3(3) . 2_746 ?
O9T Cs2 O4W 60.8(3) 4_565 . ?
O56 Cs2 O4W 97.6(2) 2_746 . ?
O17 Cs2 O4W 79.8(2) . . ?
O1T Cs2 O4W 129.9(2) . . ?
O1Z1 Cs2 O4W 106.7(2) 4_565 . ?
O5T Cs2 O4W 47.1(2) 2_746 . ?
O2W Cs2 O4W 115.9(3) . . ?
O6T Cs2 O4W 118.1(2) 2_746 . ?
O9T Cs2 O13 93.1(2) 4_565 . ?
O56 Cs2 O13 150.9(2) 2_746 . ?
O17 Cs2 O13 45.1(2) . . ?
O1T Cs2 O13 46.0(2) . . ?
O1Z1 Cs2 O13 114.9(2) 4_565 . ?
O5T Cs2 O13 135.6(2) 2_746 . ?
O2W Cs2 O13 46.1(3) . . ?
O6T Cs2 O13 100.1(2) 2_746 . ?
O4W Cs2 O13 91.4(2) . . ?
O9T Cs2 O7T 125.1(2) 4_565 . ?
O56 Cs2 O7T 68.3(2) 2_746 . ?
O17 Cs2 O7T 47.0(2) . . ?
O1T Cs2 O7T 87.9(2) . . ?
O1Z1 Cs2 O7T 153.1(2) 4_565 . ?
O5T Cs2 O7T 59.8(2) 2_746 . ?
O2W Cs2 O7T 136.5(2) . . ?
O6T Cs2 O7T 54.9(2) 2_746 . ?
O4W Cs2 O7T 64.4(2) . . ?
O13 Cs2 O7T 91.3(2) . . ?
O9T Cs2 O1W 108.4(3) 4_565 . ?
O56 Cs2 O1W 86.4(2) 2_746 . ?
O17 Cs2 O1W 108.5(2) . . ?
O1T Cs2 O1W 56.8(2) . . ?
O1Z1 Cs2 O1W 63.1(2) 4_565 . ?
O5T Cs2 O1W 133.9(2) 2_746 . ?
O2W Cs2 O1W 58.5(3) . . ?
O6T Cs2 O1W 72.2(2) 2_746 . ?
O4W Cs2 O1W 169.2(2) . . ?
O13 Cs2 O1W 89.9(2) . . ?
O7T Cs2 O1W 126.3(2) . . ?
O13W Cs3 O2Z2 55.9(7) . 4_465 ?
O13W Cs3 O9T 81.4(6) . 4_465 ?
O2Z2 Cs3 O9T 51.0(2) 4_465 4_465 ?
O13W Cs3 O4W 129.7(6) . 1_455 ?
O2Z2 Cs3 O4W 111.2(2) 4_465 1_455 ?
O9T Cs3 O4W 62.0(3) 4_465 1_455 ?
O13W Cs3 O8W 77.0(7) . . ?
O2Z2 Cs3 O8W 131.4(3) 4_465 . ?
O9T Cs3 O8W 138.7(3) 4_465 . ?
O4W Cs3 O8W 107.8(3) 1_455 . ?
O13W Cs3 O10T 74.4(7) . 2_656 ?
O2Z2 Cs3 O10T 111.6(2) 4_465 2_656 ?
O9T Cs3 O10T 80.3(2) 4_465 2_656 ?
O4W Cs3 O10T 66.7(2) 1_455 2_656 ?
O8W Cs3 O10T 60.2(3) . 2_656 ?
O13W Cs3 O5T 156.0(6) . 2_646 ?
O2Z2 Cs3 O5T 100.4(2) 4_465 2_646 ?
O9T Cs3 O5T 79.2(2) 4_465 2_646 ?
O4W Cs3 O5T 49.9(2) 1_455 2_646 ?
O8W Cs3 O5T 127.1(3) . 2_646 ?
O10T Cs3 O5T 115.8(2) 2_656 2_646 ?
O13W Cs3 O1Z2 78.1(6) . . ?
O2Z2 Cs3 O1Z2 54.3(2) 4_465 . ?
O9T Cs3 O1Z2 100.8(2) 4_465 . ?
O4W Cs3 O1Z2 138.6(3) 1_455 . ?
O8W Cs3 O1Z2 108.5(3) . . ?
O10T Cs3 O1Z2 152.0(2) 2_656 . ?
O5T Cs3 O1Z2 91.7(2) 2_646 . ?
O13W Cs3 O2T 143.1(6) . . ?
O2Z2 Cs3 O2T 160.5(2) 4_465 . ?
O9T Cs3 O2T 123.9(2) 4_465 . ?
O4W Cs3 O2T 62.2(2) 1_455 . ?
O8W Cs3 O2T 66.4(3) . . ?
O10T Cs3 O2T 83.4(2) 2_656 . ?
O5T Cs3 O2T 60.8(2) 2_646 . ?
O1Z2 Cs3 O2T 117.0(2) . . ?
O13W Cs3 O6W 112.5(6) . . ?
O2Z2 Cs3 O6W 109.9(2) 4_465 . ?
O9T Cs3 O6W 146.1(2) 4_465 . ?
O4W Cs3 O6W 117.1(3) 1_455 . ?
O8W Cs3 O6W 75.2(3) . . ?
O10T Cs3 O6W 132.4(2) 2_656 . ?
O5T Cs3 O6W 77.6(2) 2_646 . ?
O1Z2 Cs3 O6W 55.8(2) . . ?
O2T Cs3 O6W 63.0(2) . . ?
O2Z2 Cs3 O12W 64.3(5) 4_465 3_666 ?
O9T Cs3 O12W 71.6(5) 4_465 3_666 ?
O4W Cs3 O12W 109.8(5) 1_455 3_666 ?
O8W Cs3 O12W 76.0(5) . 3_666 ?
O10T Cs3 O12W 55.6(5) 2_656 3_666 ?
O5T Cs3 O12W 150.5(5) 2_646 3_666 ?
O1Z2 Cs3 O12W 97.8(5) . 3_666 ?
O2T Cs3 O12W 134.8(5) . 3_666 ?
O6W Cs3 O12W 130.4(5) . 3_666 ?
O13W Cs3 O3Z1 114.6(7) . 2_646 ?
O2Z2 Cs3 O3Z1 60.6(2) 4_465 2_646 ?
O9T Cs3 O3Z1 71.0(2) 4_465 2_646 ?
O4W Cs3 O3Z1 86.2(2) 1_455 2_646 ?
O8W Cs3 O3Z1 150.3(3) . 2_646 ?
O10T Cs3 O3Z1 147.6(2) 2_656 2_646 ?
O5T Cs3 O3Z1 45.0(2) 2_646 2_646 ?
O1Z2 Cs3 O3Z1 52.4(2) . 2_646 ?
O2T Cs3 O3Z1 100.0(2) . 2_646 ?
O6W Cs3 O3Z1 75.1(2) . 2_646 ?
O12W Cs3 O3Z1 124.7(5) 3_666 2_646 ?
O36 Cs4 O6T 52.4(2) . . ?
O36 Cs4 O9W 113.0(4) . . ?
O6T Cs4 O9W 161.2(4) . . ?
O36 Cs4 O10T 132.5(2) . 2_756 ?
O6T Cs4 O10T 82.6(2) . 2_756 ?
O9W Cs4 O10T 114.0(4) . 2_756 ?
O36 Cs4 O9T 109.0(2) . 4_565 ?
O6T Cs4 O9T 124.4(2) . 4_565 ?
O9W Cs4 O9T 69.1(5) . 4_565 ?
O10T Cs4 O9T 82.1(2) 2_756 4_565 ?
O36 Cs4 O710 121.1(2) . 2_756 ?
O6T Cs4 O710 79.4(2) . 2_756 ?
O9W Cs4 O710 103.4(4) . 2_756 ?
O10T Cs4 O710 52.1(2) 2_756 2_756 ?
O9T Cs4 O710 127.0(2) 4_565 2_756 ?
O36 Cs4 O3T 51.4(2) . . ?
O6T Cs4 O3T 95.7(2) . . ?
O9W Cs4 O3T 66.0(4) . . ?
O10T Cs4 O3T 166.7(2) 2_756 . ?
O9T Cs4 O3T 109.3(2) 4_565 . ?
O710 Cs4 O3T 114.6(2) 2_756 . ?
O36 Cs4 O7T 75.6(2) . 2_756 ?
O6T Cs4 O7T 62.7(2) . 2_756 ?
O9W Cs4 O7T 104.3(4) . 2_756 ?
O10T Cs4 O7T 98.8(2) 2_756 2_756 ?
O9T Cs4 O7T 172.9(2) 4_565 2_756 ?
O710 Cs4 O7T 50.9(2) 2_756 2_756 ?
O3T Cs4 O7T 68.9(2) . 2_756 ?
O36 Cs4 O4W 77.9(2) . . ?
O6T Cs4 O4W 63.5(2) . . ?
O9W Cs4 O4W 129.7(5) . . ?
O10T Cs4 O4W 67.4(2) 2_756 . ?
O9T Cs4 O4W 61.2(3) 4_565 . ?
O710 Cs4 O4W 111.8(2) 2_756 . ?
O3T Cs4 O4W 123.6(3) . . ?
O7T Cs4 O4W 125.7(2) 2_756 . ?
O36 Cs4 O12W 159.9(5) . . ?
O6T Cs4 O12W 141.5(5) . . ?
O9W Cs4 O12W 49.3(6) . . ?
O10T Cs4 O12W 66.9(5) 2_756 . ?
O9T Cs4 O12W 75.7(5) 4_565 . ?
O710 Cs4 O12W 63.6(5) 2_756 . ?
O3T Cs4 O12W 108.5(5) . . ?
O7T Cs4 O12W 98.2(5) 2_756 . ?
O4W Cs4 O12W 119.9(5) . . ?
O36 Cs4 O13W 141.7(5) . 3_666 ?
O6T Cs4 O13W 132.8(6) . 3_666 ?
O9W Cs4 O13W 48.8(7) . 3_666 ?
O10T Cs4 O13W 78.5(5) 2_756 3_666 ?
O9T Cs4 O13W 95.4(6) 4_565 3_666 ?
O710 Cs4 O13W 54.9(6) 2_756 3_666 ?
O3T Cs4 O13W 93.3(5) . 3_666 ?
O7T Cs4 O13W 78.0(6) 2_756 3_666 ?
O4W Cs4 O13W 140.3(5) . 3_666 ?
O36 Cs4 W3 26.81(16) . . ?
O6T Cs4 W3 76.27(16) . . ?
O9W Cs4 W3 87.2(4) . . ?
O10T Cs4 W3 158.71(17) 2_756 . ?
O9T Cs4 W3 107.59(17) 4_565 . ?
O710 Cs4 W3 124.79(15) 2_756 . ?
O3T Cs4 W3 25.11(18) . . ?
O7T Cs4 W3 73.90(16) 2_756 . ?
O4W Cs4 W3 100.08(18) . . ?
O12W Cs4 W3 133.2(5) . . ?
O13W Cs4 W3 118.2(5) 3_666 . ?
O2T Cs5 O1T 159.6(2) . 2_656 ?
O2T Cs5 O6T 131.7(2) . 1_455 ?
O1T Cs5 O6T 67.3(2) 2_656 1_455 ?
O2T Cs5 O5W 78.0(3) . . ?
O1T Cs5 O5W 101.1(3) 2_656 . ?
O6T Cs5 O5W 81.1(3) 1_455 . ?
O2T Cs5 O101 127.8(2) . 2_656 ?
O1T Cs5 O101 54.2(2) 2_656 2_656 ?
O6T Cs5 O101 81.6(2) 1_455 2_656 ?
O5W Cs5 O101 154.1(3) . 2_656 ?
O2T Cs5 O4W 68.1(3) . 1_455 ?
O1T Cs5 O4W 132.0(2) 2_656 1_455 ?
O6T Cs5 O4W 65.1(3) 1_455 1_455 ?
O5W Cs5 O4W 77.0(3) . 1_455 ?
O101 Cs5 O4W 112.4(3) 2_656 1_455 ?
O2T Cs5 O7W 83.7(2) . 2_656 ?
O1T Cs5 O7W 82.4(2) 2_656 2_656 ?
O6T Cs5 O7W 139.0(2) 1_455 2_656 ?
O5W Cs5 O7W 133.3(3) . 2_656 ?
O101 Cs5 O7W 57.9(2) 2_656 2_656 ?
O4W Cs5 O7W 133.6(2) 1_455 2_656 ?
O2T Cs5 O24 53.3(2) . . ?
O1T Cs5 O24 106.3(2) 2_656 . ?
O6T Cs5 O24 156.3(2) 1_455 . ?
O5W Cs5 O24 77.8(2) . . ?
O101 Cs5 O24 114.0(2) 2_656 . ?
O4W Cs5 O24 119.6(2) 1_455 . ?
O7W Cs5 O24 57.1(2) 2_656 . ?
O2T Cs5 O10T 91.1(2) . 2_656 ?
O1T Cs5 O10T 100.7(2) 2_656 2_656 ?
O6T Cs5 O10T 80.7(2) 1_455 2_656 ?
O5W Cs5 O10T 143.4(3) . 2_656 ?
O101 Cs5 O10T 50.6(2) 2_656 2_656 ?
O4W Cs5 O10T 66.5(2) 1_455 2_656 ?
O7W Cs5 O10T 78.5(2) 2_656 2_656 ?
O24 Cs5 O10T 123.0(2) . 2_656 ?
O2T Cs5 O4T 97.3(2) . . ?
O1T Cs5 O4T 64.9(2) 2_656 . ?
O6T Cs5 O4T 111.8(2) 1_455 . ?
O5W Cs5 O4T 64.2(3) . . ?
O101 Cs5 O4T 105.1(2) 2_656 . ?
O4W Cs5 O4T 140.9(2) 1_455 . ?
O7W Cs5 O4T 76.3(2) 2_656 . ?
O24 Cs5 O4T 48.5(2) . . ?
O10T Cs5 O4T 152.3(2) 2_656 . ?
O2T Cs5 W2 25.03(17) . . ?
O1T Cs5 W2 134.57(17) 2_656 . ?
O6T Cs5 W2 153.36(18) 1_455 . ?
O5W Cs5 W2 79.42(19) . . ?
O101 Cs5 W2 122.36(15) 2_656 . ?
O4W Cs5 W2 92.84(18) 1_455 . ?
O7W Cs5 W2 66.99(16) 2_656 . ?
O24 Cs5 W2 28.64(16) . . ?
O10T Cs5 W2 104.87(15) 2_656 . ?
O4T Cs5 W2 75.42(15) . . ?
O2T Cs5 W1 151.02(17) . 2_656 ?
O1T Cs5 W1 25.07(17) 2_656 2_656 ?
O6T Cs5 W1 73.34(18) 1_455 2_656 ?
O5W Cs5 W1 126.0(2) . 2_656 ?
O101 Cs5 W1 29.16(15) 2_656 2_656 ?
O4W Cs5 W1 128.17(19) 1_455 2_656 ?
O7W Cs5 W1 67.97(16) 2_656 2_656 ?
O24 Cs5 W1 111.08(16) . 2_656 ?
O10T Cs5 W1 77.80(16) 2_656 2_656 ?
O4T Cs5 W1 82.32(16) . 2_656 ?
W2 Cs5 W1 133.19(3) . 2_656 ?
O1W Na1 O2W 99.5(5) . . ?
O1W Na1 O4T 85.6(4) . 2_646 ?
O2W Na1 O4T 173.9(5) . 2_646 ?
O1W Na1 O3W 89.0(4) . . ?
O2W Na1 O3W 87.4(5) . . ?
O4T Na1 O3W 96.0(4) 2_646 . ?
O1W Na1 O1T 89.4(4) . . ?
O2W Na1 O1T 83.8(4) . . ?
O4T Na1 O1T 92.9(4) 2_646 . ?
O3W Na1 O1T 170.7(4) . . ?
O1W Na1 O6W 166.9(5) . . ?
O2W Na1 O6W 93.4(4) . . ?
O4T Na1 O6W 81.4(4) 2_646 . ?
O3W Na1 O6W 93.8(4) . . ?
O1T Na1 O6W 89.8(4) . . ?
O1W Na1 Cs2 63.1(3) . . ?
O2W Na1 Cs2 54.5(3) . . ?
O4T Na1 Cs2 126.3(3) 2_646 . ?
O3W Na1 Cs2 123.6(3) . . ?
O1T Na1 Cs2 48.0(2) . . ?
O6W Na1 Cs2 124.5(3) . . ?
O1W Na1 Cs5 76.8(3) . 2_646 ?
O2W Na1 Cs5 125.2(4) . 2_646 ?
O4T Na1 Cs5 52.5(3) 2_646 2_646 ?
O3W Na1 Cs5 145.9(4) . 2_646 ?
O1T Na1 Cs5 42.0(2) . 2_646 ?
O6W Na1 Cs5 93.9(3) . 2_646 ?
Cs2 Na1 Cs5 77.34(10) . 2_646 ?
O11W Na2 O8W 120.6(13) 3_666 . ?
O11W Na2 O10W 143.9(13) 3_666 . ?
O8W Na2 O10W 94.8(7) . . ?
O11W Na2 O9W 52.1(12) 3_666 3_666 ?
O8W Na2 O9W 95.3(7) . 3_666 ?
O10W Na2 O9W 137.5(9) . 3_666 ?
O11W Na2 O11W 78.9(18) 3_666 . ?
O8W Na2 O11W 104.1(12) . . ?
O10W Na2 O11W 86.5(12) . . ?
O9W Na2 O11W 130.2(13) 3_666 . ?
O11W Na2 Na2 41.1(11) 3_666 3_666 ?
O8W Na2 Na2 118.8(7) . 3_666 ?
O10W Na2 Na2 117.6(7) . 3_666 ?
O9W Na2 Na2 92.7(7) 3_666 3_666 ?
O11W Na2 Na2 37.8(11) . 3_666 ?
O11W Na2 Cs3 144.6(12) 3_666 . ?
O8W Na2 Cs3 51.6(4) . . ?
O10W Na2 Cs3 62.9(5) . . ?
O9W Na2 Cs3 92.7(6) 3_666 . ?
O11W Na2 Cs3 135.0(11) . . ?
Na2 Na2 Cs3 169.4(6) 3_666 . ?
Na1 O1W Cs2 83.9(3) . . ?
Na1 O2W Cs2 92.0(4) . . ?
Cs5 O4W Cs3 92.0(3) 1_655 1_655 ?
Cs5 O4W Cs4 92.3(3) 1_655 . ?
Cs3 O4W Cs4 94.3(3) 1_655 . ?
Cs5 O4W Cs2 172.4(3) 1_655 . ?
Cs3 O4W Cs2 95.5(3) 1_655 . ?
Cs4 O4W Cs2 87.7(2) . . ?
Cs1 O5W Cs5 103.0(3) . . ?
Na1 O6W Cs3 153.9(4) . . ?
Cs1 O7W Cs5 177.1(3) . 2_646 ?
Na2 O8W Cs3 94.0(5) . . ?
Na2 O9W Cs4 127.2(9) 3_666 . ?
Na2 O10W Cs3 81.9(6) . . ?
Na2 O11W Na2 101.1(17) 3_666 . ?
Cs4 O12W Cs3 143.9(9) . 3_666 ?
Cs3 O13W Cs4 171.2(12) . 3_666 ?


_shelxl_version_number           2014/6

